# electronic and transport properties of nanotubes

TRANSCRIPT

Electronic and transport properties of nanotubes

Jean-Christophe Charlier*

Unité de Physico-Chimie et de Physique des Matériaux (PCPM), Université Catholique deLouvain, 1 Place Croix du Sud, B-1348 Louvain-la-Neuve, Belgium

Xavier Blase†

Université de Louvain, F-69000, France, Laboratoire de Physique de la MatièreCondensée et Nanostructures, Université Lyon I, CNRS, UMR 5586, Domaine scientifiquede la Doua, F-69622 Villeurbanne Cedex, France

Stephan Roche‡

Commissariat à l’Energie Atomique, DSM/DRFMC/SPSMS/GT, 17 rue des Martyrs, 38054Grenoble Cedex 9, France

!Published 16 May 2007"

This article reviews the electronic and transport properties of carbon nanotubes. The focus is mainlytheoretical, but when appropriate the relation with experimental results is mentioned. While simpleband-folding arguments will be invoked to rationalize how the metallic or semiconducting character ofnanotubes is inferred from their topological structure, more sophisticated tight-binding and ab initiotreatments will be introduced to discuss more subtle physical effects, such as those induced bycurvature, tube-tube interactions, or topological defects. The same approach will be followed fortransport properties. The fundamental aspects of conduction regimes and transport length scales willbe presented using simple models of disorder, with the derivation of a few analytic results concerningspecific situations of short- and long-range static perturbations. Further, the latest developments insemiempirical or ab initio simulations aimed at exploring the effect of realistic static scatterers!chemical impurities, adsorbed molecules, etc." or inelastic electron-phonon interactions will beemphasized. Finally, specific issues, going beyond the noninteracting electron model, will beaddressed, including excitonic effects in optical experiments, the Coulomb-blockade regime, and theLuttinger liquid, charge density waves, or superconducting transition.

DOI: 10.1103/RevModPhys.79.677 PACS number!s": 73.63.Fg, 73.22.!f, 78.67.Ch, 61.46.Fg

CONTENTS

I. Introduction 678II. Structure of Carbon Nanotubes 679

III. Electronic Properties of Carbon Nanotubes 681A. From graphite to nanotubes 682B. Tight-binding model of graphene 683C. Zone-folding approximation 684

1. Metallic nanotubes 6842. Semiconducting nanotubes 684

D. Band structures and densities of states 686E. Band structures in a magnetic field 688

1. Aharonov-Bohm quantum phase 6882. Parallel field: The band-gap opening and

orbital degeneracy splitting 6893. Perpendicular field: The onset of Landau

levels 691F. Curvature effects: Beyond the zone-folding model 692G. Nanotube bundle and multiwall system 694H. Structural defects in carbon nanotubes 695

1. Finite length and capping topologies 6952. Connecting nanotubes 6963. Vacancies, adatoms, Stone-Wales, etc. 697

I. Optical properties and excitonic effects 698IV. Transport Properties of Carbon Nanotubes 700

A. Preliminary remarks 700B. The clean limit 702

1. Ballistic motion and conductancequantization 702

2. Transport properties of CNT-basedjunctions and contact resistance 702

C. Effect of disorder on transport 7041. Electronic eigenstates and pseudospin

symmetry 7042. Long-range disorder and the absence of

backscattering 7053. Short-range disorder and elastic mean free

path: Model analysis 7064. Influence of doping on transport properties 7075. Multishell conduction 709

a. Commensurate multiwalled nanotubes 709b. Incommensurate multiwalled nanotubes 710c. Crossed carbon nanotubes junctions,

bending and twisting deformations 711D. Quantum interference effects 711

1. Weak localization and the Aharonov-Bohm

*Electronic address: [email protected]†Electronic address: [email protected]‡Electronic address: [email protected]

REVIEWS OF MODERN PHYSICS, VOLUME 79, APRIL–JUNE 2007

0034-6861/2007/79!2"/677!56" ©2007 The American Physical Society677

effect 711a. Application to metallic !armchair" carbon

nanotubes 7122. From weak to strong localization 714

E. Inelastic scattering 7141. Electron-phonon coupling 7142. Inelastic transport length scales 7163. Electron-electron scattering and

Luttinger-liquid models 7174. Transport spectroscopy in the Coulomb

blockade regime 721F. Superconducting and charge-density-wave

instabilities 722G. Field emission from nanotubes 724

V. Conclusion 726Acknowledgments 726References 726

I. INTRODUCTION

The physics of one-dimensional !1D" systems has beena rich and active playground for theorists for more than50 years, with major conceptual breakthroughs arisingfrom the specific properties of the confined electron gas.While the reduced dimensionality is often used in intro-ductory textbooks as a convenient way to simplify theanalytic study of electronic properties, the enhanced in-teraction between electrons in 1D yields several insta-bilities that are not reproduced by standard tools devel-oped for 3D solids. This richness and complexityinvolved in extending the basics of condensed matterphysics to low-dimensionality systems explain the wealthof work and theories developed to deal with 1D solids ormolecular chains.

The difficulty in synthesizing clean 1D systems withmetallic behavior has for many decades confined thistheoretical work to formal developments and unverifiedpredictions. However, progress in synthesis and charac-terization techniques in the late 1970s allowed a con-frontation between theory and experiments. Besidesthese fundamental aspects, the technological interest incontrolling the properties of nanosized and/or plasticconductors was a strong driver for exploring this field.The attribution of the chemistry Nobel prize in 2000 toA. J. Heeger, A. G. MacDiarmid, and H. Shirakawa forthe “discovery and development of conductive poly-mers” was a clear recognition from the community ofthe importance, and the difficulty, of obtaining conju-gated one-dimensional metallic systems. Further, evenwhen metallic, the conductivity in such systems has beenshown to usually remain very low, with in most casespolaron-assisted transport leading to very large effectivemasses for the carriers. As a paradigmatic example, theconducting !and even superconducting" properties ofDNA, at the frontiers of physics, chemistry, and biology,are currently generating fierce controversies in the lit-erature.

The field of nanotubes has strongly benefited fromthis broad fundamental and technological interest. Notonly can nanotubes be metallic, they are also mechani-

cally very stable and strong, and their carrier mobility isequivalent to that of good metals, suggesting that theywould make ideal interconnects in nanosized devices.Further, the intrinsic semiconducting character of othertubes, as controlled by their topology, allows us to buildlogic devices at the nanometer scale, as already demon-strated in many laboratories. Finally, the large fullerenecommunity !yet another area recognized by the Nobelprize in chemistry in 1996", and the even larger family ofresearchers interested in carbon-based systems, natu-rally joined this novel and promising field. This mergingof interests and communities can certainly explain theformidable success and burgeoning activity generated bythe discovery of nanotubes in 1991.

A nanotube is a honeycomb lattice rolled into a hol-low cylinder with nanometric diameter and "m length.Depending on the community, specific interests, and tar-geted applications, nanotubes are regarded as eithersingle molecules or quasi-one-dimensional crystals withtranslational periodicity along the tube axis. As thereare an infinite number of ways of rolling a sheet into acylinder, the large variety of possible helical geometries,defining the tube chirality, provides a family of nano-tubes with different diameters and microscopic struc-tures. Some properties of these nanotubes, such as theelastic ones, can be explained within a macroscopicmodel of a homogeneous cylinder. Others depend cru-cially on the atomic configuration. For instance, the elec-tronic and transport properties, which constitute thescope of the present review, are certainly among themost significant physical properties of carbon nanotubes,and crucially depend on the diameter and chirality. Thisdependence on the atomic configuration, an effect ex-plained below, is quite unique in solid-state physics. Thissensitivity constitutes a challenge for synthesis tech-niques, since well-controlled properties are often de-sired, but it is also a source of innovation for applica-tions.

In the following sections, we show how carbon nano-tubes can be either !semi"metallic or semiconducting,with a band gap varying from zero to a few tenths of aneV, depending on their diameter and chirality. Further,the band gap of semiconducting tubes, or the energydifference between the peaks in the electronic density ofstates !the so-called van Hove singularities", can beshown to first order to be simply related to the tubediameter. Such remarkable results can be obtained froma variety of considerations, starting from the so-calledband-folding approach, based on knowledge of the elec-tronic properties of the graphene sheet, to the directstudy of nanotubes using semiempirical tight-binding ap-proaches. The comparison with more sophisticated abinitio calculations, and with available experimental re-sults, allows us to set the limits of these simple treat-ments, with the introduction of finer considerations,such as curvature or trigonal warping effects.

Knowledge of the electronic properties of nanotubesfurther permits one to study their response to externalprobes. This is a crucial issue as it conditions most of thepotentiality for the integration of tubes in real devices

678 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

and allows us to relate the structural and electronicproperties with the experimental optical, Raman, etc.,spectra. In particular, the effect of a magnetic field onthe electronic band structure, the optical absorption andemission spectra, and finally the transport properties oftubes will be presented.

The tremendous importance of the transport proper-ties of nanotubes, from both a fundamental and techno-logical point of view, justifies devoting the second part ofthis review to that subject. First, the main characteristicsof ballistic transport will be clarified, followed by a fewanalytical results about the absence of backscattering inthe presence of long-range disorder and the derivationof the elastic mean free path induced by short-range dis-order. All transport regimes will be reviewed in the pres-ence of elastic disorder, starting with the simple Ander-son model, followed by an extended analysis of morerealistic disorders such as chemical substitutions or func-tionalization, topological defects, and so on. Quantuminterference effects will then be addressed with a focuson weak- and strong-localization regimes, in light of re-cent experiments. Further, the contribution of inelasticscattering mechanisms !through electron-electron andelectron-phonon interactions" will be scrutinized, with adiscussion of the inelastic scattering times and decoher-ence mechanisms. As a specific case of transport !or tun-neling", with much technological importance, the physicsof field emission from nanotubes will be briefly pre-sented.

Several topics strongly related to quantum confine-ment and dimensionality effects will be addressed at theend of this review. At the heart of the complex behaviorof 1D systems, the physics of the Luttinger-liquid transi-tion will be highlighted and the signature of this transi-tion in available transport experiments will be put inperspective. Coulomb-blockade effects and their mani-festation in transport measurements will then be sum-marized. Finally, the competing charge-density-wave !orPeierls" and superconducting instabilities upon switchingon the electron-phonon interaction, observed experi-mentally, will be discussed.

The contents of the present review are theoretical,and experimental results are used primarily to providethe necessary and crucial evidence for validation of thetheory. As a matter of fact, the difficulty in performingthe synthesis and characterization of well-defined andisolated nanotubes has on many occasions granted totheory the important, but also dangerous, role of predic-tion. In return, these experimental difficulties have fos-tered the elaboration of original and creative experi-mental techniques. As emphasized below, most of thetheoretical predictions seem now to be confirmed bymany experimental results.

Even with a focus on theoretical results, space limita-tions impose a drastic, and necessarily subjective, selec-tion of topics and references. Thorough lists of refer-ences and a more complete picture !with, e.g., adescription of the synthesis and characterization tech-niques" can be found in the excellent books devoted tothe subject !Dresselhaus et al., 1996, 2001; Endo et al.,

1996; Ebbesen, 1997; Saito et al., 1998; Harris, 1999;Tománek and Enbody, 1999; Reich et al., 2004; Loiseauet al., 2006".

II. STRUCTURE OF CARBON NANOTUBES

Carbon nanotubes were discovered and first charac-terized in 1991 by Iijima from NEC laboratories !Japan"!Iijima, 1991". This discovery was made possible thanksto the use of state-of-the-art transmission microscopy.The first nanotubes discovered were made of severalconcentric cylindrical-like shells regularly spaced by anamount of about 3.4 Å as in conventional graphitematerials !Fig. 1, left". These multiwall nanotubes!MWNTs" were first synthesized with diameters rangingfrom a few nanometers to several hundred nanometersfor the inner and outer shells, respectively. As for thelength, MWNTs extending over several microns are cur-rently synthesized.

Shortly after the discovery of multiwall carbon nano-tubes, single-wall carbon nanotubes !SWNTs" were syn-thesized in abundance using arc-discharge methods withtransition-metal catalysts !Bethune et al., 1993; Iijimaand Ichihashi, 1993". A carbon nanotube made of asingle graphite layer !the graphene sheet" rolled up intoa hollow cylinder is called a single-wall nanotube. Thesetubes have quite small and uniform diameter, on the or-der of 1 nm=10−9 m. This unprecedentedly small diam-eter, combined with the crystalline perfection of theatomic network, explains why these objects were quicklyconsidered as the ultimate carbon-based 1D systems.

Crystalline ropes !or bundles" of SWNTs, with eachrope containing tens to hundreds of tubes of similar di-ameter, closely packed in a hexagonal configuration,have also been synthesized using a laser vaporizationmethod !Guo et al., 1995" and arc-discharge and chemi-cal vapor deposition !CVD" techniques !Fig. 1, right".Various synthesis methods have provided ampleamounts of sufficiently characterized samples for study-ing the fundamental properties of SWNTs.

Because the microscopic structure of SWNTs isclosely related to that of graphene, the tubes are usuallylabeled in terms of the graphene lattice vectors. As illus-trated in Fig. 2 a single-wall carbon nanotube is geo-metrically obtained by rolling up a single graphene strip!Saito et al., 1998". Its structure can be specified or in-dexed by its circumferential vector !Ch", as defined bythe chiral vector !AA! in Fig. 2" which connects twocrystallographically equivalent sites !A and A!" on agraphene sheet. In this way, a SWNT’s geometry is com-pletely specified by a pair of integers !n ,m" denoting therelative position Ch=na1+ma2 of the pair of atoms on agraphene strip which, when rolled onto each other, forma tube !a1 and a2 are unit vectors of the hexagonal hon-eycomb lattice; see Fig. 2".

This chiral vector Ch defines the circumference of thetube. The diameter dt of the nanotube can thus be esti-mated from

679Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

dt = #Ch#/# =a#

$n2 + nm + m2, !1"

where a is the lattice constant of the honeycomb net-work: a=$3$acc !acc%1.42 Å, the C-C bond length".The chiral vector Ch uniquely defines a particular !n ,m"tube, as well as its chiral angle %, which is the anglebetween Ch and a1 !zigzag direction of the graphenesheet; see Fig. 2". The chiral angle % can be calculated asfollows:

cos % =Ch · a1

#Ch##a1#=

2n + m

2$n2 + nm + m2. !2"

The value of % is in the range 0& #%#&30°, because of thehexagonal symmetry of the graphene lattice. This chiralangle % also denotes the tilt angle of the hexagons withrespect to the direction of the nanotube axis. Nanotubesof the type !n ,0" !%=0° " are called zigzag tubes, becausethey exhibit a zigzag pattern along the circumference.Such tubes display carbon-carbon bonds parallel to thenanotube axis. Nanotubes of the type !n ,n" !%=30° " arecalled armchair tubes, because they exhibit an armchairpattern along the circumference. Such tubes displaycarbon-carbon bonds perpendicular to the nanotubeaxis. Both zigzag and armchair nanotubes are achiraltubes, in contrast with general !n ,m#n#0" chiral tubes!Fig. 3".

The geometry of the graphene lattice and the chiralvector determine not only the diameter of the tube, butalso the unit cell and its number of carbon atoms. Thesmallest graphene lattice vector T perpendicular to Ch

FIG. 1. High-resolution transmission electron microscopy pictures of a multiwall carbon nanotube !left" and a bundle of single-wall nanotubes !right", illustrating two different possible geometries for nanotubes. Courtesy of Gavillet, 2001.

FIG. 2. Graphene honeycomb network with lattice vectors a1and a2. The chiral vector Ch=5a1+3a2 represents a possiblewrapping of the two-dimensional graphene sheet into a tubularform. The direction perpendicular to Ch is the tube axis. Thechiral angle % is defined by the Ch vector and the a1 zigzagdirection of the graphene lattice. In the present example, a!5,3" nanotube is under construction and the resulting tube isillustrated on the right.

FIG. 3. Atomic structures of !12,0" zigzag, !6,6" armchair, and!6,4" chiral nanotubes.

680 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

defines the translational period t along the tube axis.The lattice vector T can also be expressed in terms ofthe basis vectors a1 and a2 as T= t1a1+ t2a2. Using Ch ·T=0, the expressions for t1 and t2 are given by

t1 =2m + n

NR, t2 = −

2n + mNR

, !3"

where NR is the greatest common divisor of !2m+n" and!2n+m". The length of the translational vector t is givenby

t = #T# = $3a$n2 + nm + m2/NR. !4"

The nanotube unit cell is thus formed by a cylindricalsurface with height t and diameter dt. The number ofcarbon atoms per unit cell NC can also be expressed as afunction of n and m:

NC = 4!n2 + nm + m2"/NR. !5"

The symmetry of carbon nanotubes can be described bythe so-called line groups, which are full space groups ofone-dimensional systems including translations in addi-tion to the point-group symmetries like rotations or re-flections. The carbon-nanotube line groups are nonsym-morphic groups as they always contain a screw axis.Every !n ,m" carbon nanotube belongs to a different linegroup !Damnjanovic et al., 1999; Reich et al., 2004". Only

armchair !n ,n" and zigzag !n ,0" tubes with the same nbelong to the same symmetry group. Moreover, by start-ing with a single carbon atom and successively applyingall symmetry operations of the line group, the wholetube is constructed. However, for many applications,such as optical transitions or first-order Raman scatter-ing, it is not necessary to work with the full line group,the point group being quite sufficient. These pointgroups are Dq for chiral nanotubes !n ,m#n#0" andD2nh for achiral tubes such as !n ,n" or !n ,0". After thesymmetry operations of the nanotube have been deter-mined using its point group and its most basic structuralproperties !diameter, chirality, lattice, and reciprocal lat-tice vectors, as summarized in Table I", the correspond-ing graphene strip can be constructed and rolled up intoa cylinder. The next step is now to predict its electronicbehavior.

III. ELECTRONIC PROPERTIES OF CARBONNANOTUBES

Carbon nanotubes are characterized by two types ofbond, in analogy with graphene, which exhibits so-calledplanar sp2 hybridization. Among the four valence orbit-als of the carbon atom !the 2s, 2px, 2py, and 2pz orbitals,z perpendicular to the sheet", the !s ,px ,py" orbitals com-bine to form in-plane ' !bonding or occupied" and '*

TABLE I. Structural parameters for a !n ,m" carbon nanotube. In this table, n, m, t1, t2 are integers.

Symbol Name Formula Value

a lattice constant a=$3acc%2.46 Å acc%1.42 Å

a1, a2 basis vectors !$32

;12 "a, !$3

2;−

12 "a

b1, b2 reciprocal-latticevectors ! 1

$3;1"2#

a, ! 1

$3;−1"2#

a

Ch chiral vector Ch=na1+ma2&!n ,m" !0& #m#&n"

dt tube diameterdt=

#Ch##

=a#

$n2+nm+m2

% chiral anglesin %=

$3m

2$n2+nm+m20& #%#&

#

6

cos %=2n+m

2$n2+nm+m2 tan %=$3m

2n+m

T translational vector T= t1a1+ t2a2&!t1 , t2" gcd!t1 , t2"=1a

t1=2m+n

NR, t2=−

2n+mNR

NR=gcd!2m+n ,2n+m"a

NC number of C atomsper unit cell NC=

4!n2+nm+m2"NR

agcd!n ,m" denotes the greatest common divisor of the two integers n and m.

681Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

!antibonding or unoccupied" orbitals !Fig. 4". Such orbit-als are even with respect to planar symmetry. The 'bonds are strong covalent bonds responsible for most ofthe binding energy and elastic properties of thegraphene sheet. The remaining pz orbital, pointing outof the graphene sheet, is odd with respect to the planarsymmetry and cannot couple with the ' states. The lat-eral interaction with neighboring pz orbitals !labeled thepp# interaction" creates delocalized # !bonding" and #*

!antibonding" orbitals. In analogy, the ' bonds in thenanotube form a hexagonal network which strongly con-nects the carbon atoms in the cylinder wall of the tube.The # bonds are perpendicular to the surface of thenanotube and are responsible for the weak interactionbetween SWNTs in a bundle, similar to the weak inter-action between carbon layers in pure graphite !Charlieret al., 1991". The energy levels associated with the in-plane ' bonds are known to be far away from the Fermienergy in graphite !Fig. 4, right" and thus do not play akey role in its electronic properties. In contrast, thebonding and antibonding # bands cross the Fermi level

at high-symmetry points in the Brillouin zone ofgraphene !Wallace, 1947". For a good understanding ofthe electronic properties of SWNTs, the electronic struc-ture of graphene will be briefly discussed in the nextsection.

A. From graphite to nanotubes

Although graphite has been studied for decades,graphene was only isolated experimentally in 2004 aftera long struggle !Novoselov et al., 2004". Further, and de-spite early predictions !Wallace, 1947", its remarkableconducting properties, in which electrons mimic the be-havior of massless, relativistic particles, have only beenobserved recently !Novoselov et al., 2005; Zhang et al.,2005".

The electronic bands of graphene along the high-symmetry M-(-K directions are presented in Fig. 5. The# and #* bands cross at the vertices of the hexagonalBrillouin zone !Fig. 6". Such vertices are labeled by theirmomentum vector usually written as K. Consequently,graphene is a special semimetal whose Fermi surface isreduced to the six distinct K points of the hexagonalBrillouin zone. Close to the Fermi energy, the # and #*

bands are nearly linear, in contrast with the quadraticenergy-momentum relation obeyed by electrons at bandedges in conventional semiconductors. This linearenergy-momentum relation of electrons will explain theextremely good conductivity in graphene and bearsmuch importance in the Luttinger-liquid !LL" behaviorfor low-energy excitations in nanotubes !see Sec.IV.E.3".

The bonding and antibonding ' bands are well sepa-rated in energy !)10 eV at (". These bands are fre-quently neglected in semiempirical calculations as theyare too far away from the Fermi level to play a role inthe electronic properties of graphene. The remainingtwo # bands can be simply described with a rathersimple tight-binding Hamiltonian, leading to analyticalsolutions for their energy dispersion and the relatedeigenstates. This simple approach can be further ex-

FIG. 5. Electronic properties of graphene. !a" Electronic band structure of graphene. The bonding ' and antibonding '* bands areseparated by a large energy gap. The bonding # !last valence" band and antibonding #* !first conduction" band cross at the Kpoints of the Brillouin zone. The Fermi energy is set to zero, and * indicates the work function. Above the vaccuum level !dottedhorizontal line", the states of the continuum are difficult to describe and merge with the '* bands. !b",!d" # state at K and !c",!e"' state at (, seen from above and from the side of the graphene plane. Note that the # wave function cancels on a hexagonalsublattice due to the exp!iK ·r" phase factor. The # !'" state is odd !even" with respect to the graphene plane reflection. Courtesyof Fernández-Serra, 2006.

FIG. 4. The ' bonds in the carbon hexagonal network connectthe carbon atoms and are responsible for the binding energyand the elastic properties of the graphene sheet !left". The #bonds are perpendicular to the surface of the sheet. The cor-responding bonding and antibonding ' bands are separated bya large energy gap !right", while the bonding and antibonding# states lie in the vicinity of the Fermi level !EF". Adaptedfrom Loiseau et al., 2006.

682 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

tended to study the properties of nanotubes by combin-ing these analytic results with the requirement that thewave functions in tubes must satisfy the proper bound-ary conditions around the tube circumference. This iswhat we show in the next sections.

B. Tight-binding model of graphene

As mentioned in the previous section, the grapheneplane is a hexagonal lattice with two atoms per unit cell!A and B" and a basis defined by vectors !a1 ,a2" !see Fig.6". The condition ai ·bj=2#+ij allows one to obtain thereciprocal-lattice vectors !b1 ,b2". Every carbon atompossesses four valence electrons !two 2s and two 2p elec-trons". When the atoms are placed onto the graphenehexagonal lattice, as in Fig. 6, the electronic wave func-tions from different atoms overlap. However, such anoverlap between the pz orbitals and the s or px and pyelectrons is strictly zero by symmetry. Consequently, thepz electrons, which form the # bonds in graphene, canbe treated independently of other valence electrons.Within this #-band approximation, the A atom !B atom"is uniquely defined by one orbital per atom site pz!r−rA" 'pz!r−rB"(.

To derive the electronic spectrum of the total Hamil-tonian, the corresponding Schrödinger equation has tobe solved, and by applying the Bloch theorem, the wavefunctions can be written as follows:

,!k,r" = cA!k"pzA!k,r" + cB!k"pz

B!k,r" , !6"

with

pzA!k,r" =

1$Ncells

)!

eik·!pz!r − rA − !" , !7"

pzB!k,r" =

1$Ncells

)!

eik·!pz!r − rB − !" , !8"

where k is the electron momentum !the quantum num-ber", Ncells is the number of unit cells in the graphenesheet, and ! is the cell position index. The spectrum isderived by solving the Schrödinger equation which re-duces to a 2$2 matrix diagonalization:

*HAA − E HAB

HBA HBB − E+ , !9"

where the matrix elements are defined as

HAA!k" =1

Ncells)!,!!

eik·!!!−!",pzA,!#H#pz

A,!!- , !10"

HAB!k" =1

Ncells)!,!!

eik·!!!−!",pzA,!#H#pz

B,!!- , !11"

with the notation pzA/B,-=pz!r−rA/B−-". Here we have

neglected the overlap matrix elements S= ,pzA # pz

B- be-tween neighboring pz orbitals !neglect of overlap inte-grals defines the so-called orthogonal tight-bindingschemes". After simple manipulations and restricting in-teractions to first nearest neighbors only, one gets

HAB!k" = ,pzA,0#H#pz

B,0- + e−ik·a1,pzA,0#H#pz

B,−a1-

+ e−ik·a2,pzA,0#H#pz

B,−a2- = − .0/!k" , !12"

with .0 the transfer integral between first-neighbor #orbitals !a typical value for .0 is 2.9 eV", /!k"= !1+e−ik·a1 +e−ik·a2", and ,pz

A,0#H#pzA,0-= ,pz

B,0#H#pzB,0-=0 as

the energy reference. The dispersion relations are thenreadily obtained:

E±!k" = ± .0$3 + 2 cos!k · a1" + 2 cos!k · a2" + 2 cos'k · !a2 − a1"( , !13"

which can be further developed as

E±!kx,ky" = ± .0$1 + 4 cos$3kxa

2cos

kya2

+ 4 cos2 kya2

!14"

by setting a=$3acc !acc=1.42 Å". The k= !kx ,ky" vectorsthat belong to the first hexagonal Brillouin zone !BZ"

constitute an ensemble of available electronic momenta.In Fig. 7, these simple tight-binding dispersion relationsare represented with dashed lines along high symmetrydirections of the BZ, defined by the ( and M pointstogether with the six BZ vertices !K points".

With one pz electron per atom in the #-#* model !thethree other s, px, and py electrons fill the low-lying 'band", the !!" band !negative energy branch" in Eq. !14"

FIG. 6. Brillouin zone and reciprocal space. !a" Basis vectorsin the hexagonal lattice of graphene. !b" Brillouin zone. Thecorresponding reciprocal basis vectors read b1=b!1/2 ,$3/2"and b2=b!1/2 ,−$3/2", with b=4# /a$3.

683Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

is fully occupied, while the !0" branch is empty. Theseoccupied and unoccupied bands cross at the K points'one verifies that /!k=K"=0(. The Fermi level EF !orcharge-neutrality point" is therefore the zero-energy ref-erence in Fig. 7, and the Fermi surface is defined by theset of K points. Since the occupied and unoccupiedbands do cross, the graphene sheet displays a metallic!zero-gap" character. However, as the Fermi surface is ofzero dimension !since it is reduced to a discrete and fi-nite set of points", the term semimetal is usually used.

This simple orthogonal tight-binding model yields #and #* zone-center ( energies which are symmetric!±.0" with respect to EF. In fact, the antibonding !unoc-cupied" #* bands are located at a higher energy if theoverlap integral S is not set to zero !see Fig. 7". A better,but more complicated, #-#* parametrization can befound in Reich, Maultzsch, Thomsen, and Ordejón!2002" where a careful comparison between ab initio andvarious tight-binding schemes is presented for grapheneand several nanotubes. The main advantage of thepresent nearest-neighbor approximation is the verysimple analytical expression for the # electronic states ofgraphene.

C. Zone-folding approximation

Due to periodic boundary conditions along the cir-cumferential direction of the tube, the allowed wavevectors “around” the nanotube circumference are quan-tized: they can take only a set of discrete values. In con-trast, the wave vectors along the nanotube axis remaincontinuous !for infinite tubes". Plotting these allowedvectors for a given nanotube onto the Brillouin zone ofgraphene generates a series of parallel lines. The length,number, and orientation of these cutting lines depend onthe chiral indices !n ,m" of the nanotube. The basic ideabehind the zone-folding approximation is that the elec-

tronic band structure of a specific nanotube is given bysuperposition of the graphene electronic energy bandsalong the corresponding allowed k lines. This is what weexplain now.

A specific carbon nanotube defines a unique chiralvector Ch= !n ,m" expressed in the basis !a1 ,a2" !Fig. 2"that fixes its symmetry and its diameter. As mentioned inSec. II, the chiral vector length #Ch# equals$3acc$n2+nm+m2 or #dt !dt being the nanotube diam-eter". The application of periodic boundary conditionsaround the tube circumference leads to some restrictionson the allowed wave function quantum phase:

,k!r + Ch" = eik·Ch,k!r" = ,k!r" , !15"

with the vectors r and k taken on the tube surface. Thefirst equality stems from the Bloch theorem. Dependingon the tube symmetry, that is, on the chiral vector Ch= !n ,m", two situations can occur.

1. Metallic nanotubes

We make an analysis in the neighborhood of theFermi surface, so that we write k=K++k, with +k small,taking, e.g., K= !b1−b2" /3= !0,4# /3a", so that k= !+kx ,4# /3a++ky". When eiK·Ch =1 !which is possibleonly when n−m=3l, with l an integer", then the con-straint on the wave function becomes +k ·Ch=2#q !q in-teger". Each index q defines a line of allowed k vectors,and each line contributes to one occupied # band andone unoccupied #* band. The condition n−m=3l is al-ways satisfied for armchair tubes and for the subset ofthe !n ,0" zigzag tubes with n multiples of 3. Rewritingthe dispersion relation in the general case as E2!kx ,ky"=.0

2#/#2 and performing a second-order perturbation ex-pansion in the vicinity of the K points, one finally ob-tains #/!kx ,ky"#2% 3

4 !+kx2++ky

2"+O!+k3" !with +kx and +kyrelated by +k ·Ch=2#q". Close to EF, the dispersion re-lation then reads E±!+k"% ± !$3a /2".0.+k., a linearenergy-momentum relation mentioned above. There-fore, states arbitrarily close in energy to the Fermi levelcan be found for q=0 and the system is metallic !see Fig.8". The Fermi velocity vF=$3a.0 /21= 3

2acc.0 /1 is typi-cally given by vF%8$105 m s−1 for .0=2.9 eV. The lin-ear band dispersion close to EF will be shown to haveuseful consequences.

A simple expression for the eigenstates can also bederived close to EF within the same type of approxima-tion. Such an expression will be used in Sec. IV.C.2 toshow that elastic backscattering is quenched in nano-tubes if the disorder is long ranged. One notes that, for ageneral helical symmetry, the full properties of theeigenstates can be derived by constructing generalizedBloch states satisfying helical !rototranslation" symme-tries !Mintmire et al., 1992".

2. Semiconducting nanotubes

The second possible choice for !n ,m" nanotubes isgiven by the condition n−m=3l±1. In this situation

FIG. 7. Limitations of the #-#* model. !a" Ab initio !solidlines" and nearest-neighbor orthogonal tight-binding 'dashedlines, from Eq. !14"( # and #* electronic bands for graphene.!b" Difference 2E between the ab initio and tight-binding bandstructures. Adapted from Reich, Maultzsch, Thomsen, and Or-dejón, 2002.

684 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

eiK·Ch = ±e2i#/3, and one gets +k= !2# / #Ch#"!q±1/3"3!

+k.3. with 3! and 3. the basis vectors along the Ch andT directions, respectively, where T is the translationalvector along the tube axis, as defined in Sec. II. By fol-lowing a similar calculation as for the prior case, oneobtains in the vicinity of the Fermi level a new disper-sion relation, namely,

Eq±!k." % ±

$3a2.0$* 2#

#Ch#+2*q ±13+2

+ k.2, !16"

where the integer variable q counts the available bands,whereas k. is the part of the wave vector that continu-ously describes the states within a given subband !andassociated with the direction parallel to the tube axis".

This case leads to an obvious gap opening at the Fermilevel !Fig. 9" since

Eq=0+ !k. = 0" − Eq=0

− !k. = 0" =2#a.0

$3#Ch#= 2Eg

1. !17"

It appears that 2Eg1 decreases as the inverse of the tube

diameter dt !dt= #Ch# /#". For a very large diameter, onefinds as expected a zero-gap semiconductor since we re-cover the graphene sheet. For realistic tubes, with, e.g., adiameter of 1.4 nm 'helical vector !17,0"(, one gets 2Eg

1

%0.59 eV. This 1 /d dependence of the gap on the diam-eter relies on the assumption of a linear dispersion ofthe bands around EF, a result first derived by White andMintmire !1998". In reality, the bands are not linearaway from EF, an effect called trigonal warping !Saito,Dresselhaus, and Dresselhaus, 2000" which induces a de-pendence of the band gap not only on the diameter, buton the !n ,m" indices as well.

In relation to the study of transport properties an im-portant quantity linked to the dispersion relation is theso-called effective mass of the charge carriers. In semi-conducting nanotubes, this quantity can be derived fromEq. !16",

Eq=0± = ± $!m*vF

2"2 + !1k.vF"2,

defining m*=2#1 /3#Ch#vF, which is thus inversely pro-portional to the nanotube diameter and tends to zero asthe diameter tends to infinity !graphene limit". This con-cept has been used !Zhou et al., 2005" to estimate thecharge mobility properties in semiconducting nanotubes.

In summary, early theoretical calculations !Hamada etal., 1992; Mintmire et al., 1992; Saito et al., 1992" showedthat the electronic properties of carbon nanotubes arevery sensitive to their geometric structure. Althoughgraphene is a semimetal, theory has predicted that car-bon nanotubes can be metals or semiconductors with anenergy gap that depends on the tube diameter and he-licity, i.e., on the indices !n ,m". These results can besimply understood within a band-folding picture, as il-lustrated in the present section. This approach is maderelatively simple in nanotubes because of the specialshape of the graphene Fermi surface and the restrictionof the electronic bands to the #-#* manifold.

FIG. 8. The band-folding scheme. !a" Brillouin zone ofgraphene. The white rectangle is the Brillouin zone associatedwith the four-atom cell with lattice vectors Ch /n=a1+a2 and T!T=a1−a2 for an armchair tube". Thick lines are the allowed klines for the !5,5" armchair tube. To obtain the !5,5" band struc-ture in the band-folding approach, fold the colored cornersonto the rectangular cell and superimpose the graphene energybands calculated along the obtained thick lines of length2# / #T#. In particular, the K points are folded at two-thirds of(X !or its inversion symmetry image". The bands are indexedby the integer q such that k ·Ch=2#q. In the corresponding!5,5" tube, q is also the azimuthal quantum number. !b" Disper-sion relations E±!kx ,ky" for the graphene plane, together withthat of an armchair nanotube !bold line".

FIG. 9. Dispersion relations E±!kx ,ky" for the graphene plane,together with that of a zigzag semiconducting nanotube !boldline".

685Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

When forming a tube, owing to the periodic boundaryconditions imposed in the circumferential direction, onlya certain set of k vectors in the graphene BZ are al-lowed. This allowed set of Bloch momenta depends onthe diameter and helicity of the tube. Whenever the al-lowed k vectors include the point K, the system is ametal with a nonzero density of states at the Fermi level,resulting in a one-dimensional metal with two bands dis-persing linearly close to EF. When the K point is notincluded, the system is a semiconductor with a smallband gap that depends mainly on the diameter. In thiscase, the conduction- and valence-band edges comefrom states with k vectors located on the allowed line!s"closest to the K point.

Within the zone-folding approximation, the generalrules for the metallicity of single-wall carbon nanotubesare as follows: a nanotube defined by the !n ,m" indiceswill be metallic !semiconductor" if n−m=3l, with l aninteger !n−m=3l±1". Consequently, most carbon nano-tubes are semiconductors and only a fraction !1/3" aremetallic !or semimetallic".

To conclude this subsection, we note that the index q,as defined above by the condition k ·Ch=2#q 'Eq. !15"(is also the azimuthal quantum number associated withthe states on the corresponding allowed k line. Thisquantum number therefore characterizes the behaviorof eigenstates with respect to rotations around the axisthat transform the tube into itself. It can be used in par-ticular to study, on the basis of symmetry-related selec-tion rules !Vucovic et al., 2002", the effect of a perturba-tion on various subbands and their mixing upon static!e.g., tube squashing, interaction with a substrate, etc."or time-dependent !e.g., optical excitation" perturba-tions.

D. Band structures and densities of states

As the nanotubes are one dimensional, their Brillouinzone is one dimensional as well, with zone edges usuallylabeled X, namely, X= ± !# /T"!., with !. and T definedabove. The nanotube band structure is therefore repre-sented along the (X direction !(X! with X!=−X sym-metric by time reversal". In the band-folding approach,one obtains therefore a superposition of all allowedEq

±!k." graphene eigenvalues, with q the allowed line in-dex !two bands per line" and k. the continuous momen-tum along 3. !from now on, as there is only one direc-tion, we drop the . subscript and write k. =k". One saysthat the allowed k lines are “folded” onto the (X direc-tion 'see Fig. 8!a" for armchair tubes(. We now study theband structure and related density of states of !n ,m"tubes as given by the band folding of the #-#* bands ofgraphene within the orthogonal tight-binding schemepresented above.

The electronic band structure of an armchair !5,5" car-bon nanotube is presented in Fig. 10. Six bands for theconduction and an equal number for the valence statesare observable. However, four of them are degenerate,leading to ten electronic levels in each case, consistent

with the ten hexagons around the circumference of the!5,5" nanotube. Indeed, the bands coming from two al-lowed lines with opposite q index, for q= ±1 to q= ±4'see Fig. 8!a"(, are degenerate by symmetry. For all arm-chair nanotubes, the energy bands exhibit a large degen-eracy at the zone boundary, where k= ±# /a !X point",so that Eq. !14" becomes E!k= ±# /a"= ±.0. This comesfrom the absence of dispersion along the segments con-necting the neighboring centers of the BZ sides !the Mpoints", an effect that will yield the so-called trigonalwarping of the bands as discussed below. The valenceand conduction bands for armchair nanotubes cross atk=kF= ±2# / !3a", a point that is located at two-thirds of(X 'Fig. 8!a"(. This means that the original K vertices ofthe original graphene hexagonal BZ are folded at two-thirds of the (X line !or its inversion symmetry image".As discussed above, the !5,5" armchair nanotube is thusa zero-gap semiconductor which will exhibit metallicconduction at finite temperatures, since only infinitesi-mal excitations are needed to promote carriers into theconduction bands.

The density of states !DOS" 2N /2E represents thenumber of available states 2N for a given energy inter-val 2E !2E→0". This DOS is a quantity that can bemeasured experimentally under some approximations.The shape of the density of states is known to dependdramatically on dimensionality. In 1D, as shown below,the density of states diverges as the inverse of the squareroot of the energy !1/$E" close to band extrema. These“spikes” in the DOS are called Van Hove singularities!VHSs" and manifest the confinement properties in di-rections perpendicular to the tube axis. As carbon nano-tubes are one dimensional, their corresponding DOSsexhibit such a spiky behavior at energies close to bandedges !see Fig. 10". The position of these Van Hove sin-gularities can be analytically derived from the dispersionrelations. The density of states is defined by

FIG. 10. Band structure and density of states for a !5, 5" arm-chair nanotube within the zone-folding model. The 1D energydispersion relations are presented in the '−3.0 ;3.0( energy in-terval in dimensionless units !.0 being the nearest-neighborC-C tight-binding overlap energy /2.9 eV". The energy bandsare plotted along the X-(-X direction. The Fermi level is lo-cated at zero energy.

686 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

4!E" =15

Tr'+!E − H"( , !18"

where +!E−H" is the spectral measure; the trace is ex-panded within a complete basis, and 5 is the volume ofthe considered system. For the set of eigenvalues Eq

s !k",where s=± refers to the sign of the solution in Eq. !14",the DOS can be expressed as

4!E" =25

)q

)s=±

0 dk+„E − Eqs !k"…

=25

)q

)s=±

0 dk+!k − kqs"1 $Eqs !k"

$k1−1

, !19"

where kqs are the roots of the equation E−Eqs !k"=0,

while 5=4##Ch# /$3a2 is the volume !surface" of the re-ciprocal space for each allowed state divided by the dis-tance between allowed lines in the graphene Brillouinzone !see above". In the vicinity of K, where one can usethe linear energy-momentum relation, the contributionof k to the density of states is related to

1 $Eqs !k"

$k1−1

=2

$3.0a

#Eqs !k"#

$!Eqs "2!k" − 6qs

2, !20"

where 6qs gives the energy position of the Van Hovesingularities. In the vicinity of EF, those positions aregiven by #6qs#=$3.0a2k!

q /2 with 2k!q = 2!k−K" ·Ch / #Ch#2

=2##3q−n+m# /3#Ch#. Hence #6qs#=#.0acc#3q−n+m# / #Ch#, and one finally obtains the density of states

4!E" =2a

#.0#Ch# )q=1

2n

)s=±

#Eqs !k"#

$!Eqs "2!k" − 6qs

2. !21"

For all metallic nanotubes, the density of states per unitlength along the nanotube axis is a constant at the Fermienergy !EF" and can be expressed analytically !Mintmireand White, 1998":

4!6F" = 2$3acc/!#.0#Ch#" . !22"

Beyond the linear-band approximation, one can rewriteEq. !14" for metallic armchair !n ,n" nanotubes to obtainthe following band dispersion relation:

Eq±!k" = ± .0$1 + 4 cos

ka2

cosq#n

+ 4 cos2 ka2

, !23"

where q=1,2n corresponds to the discrete part of thewave vector !band index" and k is the continuous partof the wave vector, describing states in a specific band!−#7ka7#". The positions of the Van Hove singulari-ties can then be derived analytically directly from Eq.!23", and a simple calculation gives 6q,s=±= ±.0 sin q# /n.In Fig. 10, the spikes in the DOS are localized at6q=1,10;s=±= ±.0 sin q# /5.

We now turn to zigzag tubes. The calculated 1D dis-persion relations E!k" for the !9,0" and !10,0" zigzagnanotubes are illustrated in Figs. 11 and 12, respectively.As expected, the !9,0" tube is metallic, with the Fermisurface located at (, whereas the !10,0" nanotube exhib-

its a finite energy gap at (. In particular, in the case ofthe !10,0" nanotube, there is a dispersionless energyband at E /.0= ±1, which gives a singularity in the DOSat these particular energies. For a general !n ,0" zigzagnanotube, when n is a multiple of 3, the energy gap atk=0 !( point" becomes zero. However, when n is not amultiple of 3, an energy gap opens at (. The correspond-ing densities of states have a zero value at the Fermienergy for the semiconducting nanotube and a smallnonzero value for the metallic one.

It should be noted that the k values for the bandcrossing at EF in metallic nanotubes are k= ±2# /3T ork=0 for armchair or zigzag tubes, respectively. These kvalues are also the locations of the band gaps for semi-conducting zigzag nanotubes. The same k values denoteas well the positions of the energy gaps !including zeroenergy gaps" for the general case of chiral nanotubes. InFig. 13, the dispersion relations E!k" for the !8,2" chiralnanotube are shown. Since n−m is a multiple of 3, thisnanotube exhibits a metallic behavior with a band cross-ing at k= ±2# /3T. Other chiral nanotubes, like the !9,6",display a zero energy gap at k=0. The DOS of chiral

FIG. 11. Band structure and density of states for a !9, 0" zigzagnanotube within the zone-folding model. The Fermi level islocated at zero energy.

FIG. 12. Band structure and density of states for a !10,0" zigzagnanotube within the zone-folding model. The Fermi level islocated at zero energy.

687Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

nanotubes !see Fig. 13" also displays Van Hove singulari-ties as for achiral tubes !Charlier and Lambin, 1998;Mintmire and White, 1998; White and Mintmire, 1998".

In semiconducting zigzag or chiral nanotubes, theband gap 'as expressed by Eq. !17"( is independent ofthe chiral angle and varies inversely with the nanotubediameter: 2Eg

1=2.0acc /dt !in the linear-band approxima-tion". Density-of-states measurements by scanning tun-neling spectroscopy !STS" provide a powerful tool forprobing the electronic structure of carbon nanotubes. Itcan be shown, indeed, that under some assumptions thevoltage-current derivative dI /dV is proportional to theDOS. These experiments !Odom et al., 1998; Wildöer etal., 1998" confirmed that the energy band gap of semi-conducting tubes is roughly proportional to 1/dt andthat about 1/3 of nanotubes are conducting, while theother 2/3 are semiconducting. Resonances in the DOShave also been observed experimentally !Odom et al.,1998; Wildöer et al., 1998" on both metallic and semicon-ducting nanotubes whose diameters and chiral angleswere determined using a scanning tunneling microscope!STM" !Venema et al., 2000". Several other experimentaltechniques, such as resonant Raman scattering !Jorio etal., 2001" and optical absorption and emission measure-ments !Bachilo et al., 2002; O’Connell et al., 2002; Le-febvre et al., 2003", have also confirmed this structure inVan Hove singularities of the electronic densities ofstates in single-wall carbon nanotubes.

E. Band structures in a magnetic field

The application of a uniform external magnetic fieldhas profound consequences on the electronic band struc-ture of carbon nanotubes. There exist two cases of highsymmetry for the direction of the magnetic field withrespect to the nanotube axis. When the magnetic field isapplied parallel to the tube axis, electrons within thenanotube are influenced by the electromagnetic poten-tial, whose dominating effect is to add a new phase fac-tor to the quantum wave function !with subsequentmodification of the associated momentum", and in the

cylinder geometry this phase factor will be driven in aperiodic fashion by the magnetic flux threading thenanotube cross section. This quantum phenomenon wasfirst described theoretically by Aharonov and Bohm!1959", whereas field-periodic oscillations of the magne-toresistance were experimentally measured in ordinarymetallic rings !Webb et al., 1985", opening a new field formesoscopic physics !Imry, 1997".

Given that the metallic or semiconducting characterof carbon nanotubes results from the existence of theallowed momentum k at the K points of the hexagonalBrillouin zone, the superimposed Aharonov-Bohmphase factor, modulated by the field, will induce somefield-dependent disruption of the initial eigenstate distri-bution in reciprocal space, with a first spectacular effectof the band gap opening for an initially metallic system,as first described by Ajiki and Ando !1993". In this sec-tion, we provide the basics for understanding theAharonov-Bohm phenomenon in carbon nanotubes andits consequences on the electronic spectrum. In Sec.IV.D.1, its corresponding effects on transport propertieswill be further described.

1. Aharonov-Bohm quantum phase

To further deepen and illustrate these effects, let usdescribe the modifications of the quantum phase factor,driven by the vector potential A and associated with theexternal magnetic field B=B!ux ,uy ,uz" !with B=rotA".Within the tight-binding scheme, the Bloch functions inthe static B can be written as

,!k,r" =1

$N)R

eik·Rei8R9!rR" .

With R a lattice vector and 8R the phase factor associ-ated with the magnetic field, it can be shown that 8R!r"=3R

r A!r!"dr!=301!r−R" ·A!R+:'r−R("d: !Luttinger,

1951", so that the total matrix elements of H= !p /2m−eA"2+V!r", in the presence of B, are simply obtainedthrough multiplication of those in the zero-field case bythe phase factor !Saito et al., 1998". For a general de-scription of the B-dependent band-structure effects, onepossibility is to adopt the Cartesian basis !ex ,ey ,ez"where ez and ex are, respectively, taken along and per-pendicular to the tube axis. In the Landau gauge A=B!0,uzx ,uxy", the Aharonov-Bohm phase acquiredduring an electronic motion between an orbital locatedat !xi ,yi ,zi" and another located at !xj ,yj ,zj" can be eas-ily derived:

8ij =2#*0

B4!yj − yi"uzxi + xj

2+ !zj − zi"ux

yi + yj

2 5 , !24"

where *0 is the quantum flux. This result is applicablewhatever the direction of B with respect to the tube axisand gives the axial configuration for !ux=0,uz=1" andthe perpendicular configuration for !ux=1,uz=0". Thisfurther allows us to compute the remormalized field-dependent coupling overlap between # orbitals, .ij!B"

FIG. 13. Band structure and density of states for a !8,2" chiralnanotube within the zone-folding model. The Fermi level islocated at zero energy.

688 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

=.0 exp'!2i# /*0"3ri

rjA!r"dr(=.0e−i8ij, known as thePeierls substitution !Peierls, 1933".

2. Parallel field: The band-gap opening and orbitaldegeneracy splitting

In the axial case, however, the use of another basis setmakes understanding of the Aharonov-Bohm effectstraightforward. Indeed, if one considers the two-dimensional Cartesian coordinates r= !x , y" in the basisdefined by the directions !Ch ,T", then the vector poten-tial is recast as A= !* / #Ch# ,0" and the magnetic phasefactor between two # orbitals located at ri= !xi , yi" andrj= !xj , yj" is simply written as 8i−8j= i*!xi− xj" / #Ch#. Ac-cordingly, the periodic boundary conditions on the quan-tum phase will be modified as

,k!r + #Ch#" = eik·Chexp*!2#/*0"0r

r+Ch

A!r!"dr!+,k!r" ,

and since the additional magnetic phase factor thus re-duces to 2#* /*0, the change in the quantum momentumbecomes

3! → 3!!*" =2##Ch# *q ±

/

3+*

*0+ , !25"

with /=0 for metallic tubes, and /= ±1 for semiconduct-ing tubes. In Fig. 14 the effect of this change in momen-tum is illustrated in reciprocal space. From Eqs. !16" and!25", the field-dependent gap oscillation for an initiallymetallic tube is obtained,

2EB = Eq=0+ !k.,*/*0" − Eq=0

− !k.,*/*0" = 32Eg1*/*0,

if *&*0 /2, where 2Eg1=2#acc.0 /$3#Ch# denotes the gap

at zero flux as given by Eq. !17". If *0 /2&*&*0, then2EB=32Eg

1#1−* /*0#, so that the band gap exhibits an

oscillation between 0 and 2Eg1 with a period *0 !Ajiki

and Ando, 1993, 1994, 1996; Tian and Datta, 1994; Lin etal., 1995; Lu, 1995". For instance, 2EB675 meV at 50 Tfor the !22,22" tube !diameter63 nm", while 2EB640 meV at 60 T for the !10,10" tube !diameter=1.4 nm". In addition, to obtain a field equivalent to *=*0 in nanotubes with diameters of 1, 10, 20, and 40 nm,one typically needs magnetic fields of 5325, 53, 13, and3 T, respectively.

In addition to such *0-periodic band-gap oscillations,the Aharonov-Bohm effect more generally affects thewhole subband structure, as evidenced by Van Hove sin-gularity splitting and shifts !Jiang et al., 2000; Roche etal., 2000; Shyu et al., 2003". These effects result from theinfluence of the magnetic field on the orbital degeneracy.Indeed, the initial symmetry of the carbon nanotubesimplies that each available energy level is initially four-fold degenerate !including spin and orbital degeneracy".The orbital degeneracy is attributed to the symmetrybetween clockwise !0" and counterclockwise !!" elec-tronic motions around the tube. In the presence of anexternal magnetic field, electrons in degenerate !0" and!!" eigenstates will acquire opposite orbital magneticmoments ±"orb, which will thus produce an upshift ofthe energy of !0" and a downshift of the energy of !!",resulting in lifting the orbital degeneracy !or Van Hovesingularity splitting".

This mechanism is illustrated in the DOS plots for the!5,5" and !10,10" tubes in Figs. 15 and 16, respectively,which are both metallic nanotubes at zero magnetic field!Roche et al., 2000". The calculations have been per-formed using a simple tight-binding model in the#-orbital approximation, while nearest-neighbor hop-ping integrals have been renormalized in the presence ofa magnetic field using Eq. !24".

FIG. 14. Representation of the first Brillouin zone of agraphene sheet together with allowed states for an armchairtube !dashed lines" at zero flux. Modifications of allowed statesin the vicinity of k points, under the effect of a magnetic fieldapplied parallel to the tube axis !circles give the equipotentialsclose to the Fermi energy".

FIG. 15. !Color online" Density of states of the !5,5" carbonnanotube for several magnetic flux values: * /*0=0 !a", * /*0=0.1 !b", * /*0=0.2 !c", and * /*0=0.5 !d". This is a metallictube at zero magnetic flux but a gap opens up once a finite fluxis applied and increases with the flux.

689Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

As predicted theoretically, by applying a finite mag-netic flux * threading the tube, the band gap opens andincreases linearly with *, to reach a maximum value athalf the quantum flux !*0 /2". Further, the band gap islinearly reduced until it finally closes back when the fieldreaches one quantum flux. The labels !a"–!e" in Fig. 16are the DOSs for the !10,10" tube at * /*0= !a" 0, !b"0.125, !c" 0.25, !d" 0.375, and !e" 0.5. For * /*0=0.125'trace !b"(, one notices that in the vicinity of the charge-neutrality point !i.e., 6=0", a new VHS appears, indicat-ing the gap opening. In !c", !d", and !e", the gap is seen toincrease, reaching its maximum value at * /*0=0.5. Theevolution of the VHS is then reversed and the gap closesagain at * /*0=1. For VHSs at higher energies !e.g.,those located at 6q=1", the oscillatory behavior is slightlymore involved: at low fields a splitting is observed foreach VHS, which is followed by crossing at higher flux,and finally all VHSs return to the original positionswhen * /*0=1 !see the inset of Fig. 16".

In the case of armchair !n ,n" metallic tubes, the mag-nitude of the field-dependent splitting of the qth VHScan be analytically ascertained:

2EB!6q,*/*0" = 2.04sin#

q*cos

#*

q*0− 1+

− cos#

qsin

#*

q*05 . !26"

Semiconducting tubes 'i.e., !n ,m" tubes with n−m=3l±1 !l being an integer"( are affected in a similar way,but the gap expression is slightly different. One finds2EB=2Eg

1#1−3* /*0# if 0&*&*0 /2 and 2EB=2Eg1#2

−3* /*0# when *0 /2&*&*0. Hence, the initial zero-field energy gap !2Eg

1" continuously decreases with in-creasing *, to reach zero at *=*0 /3. The gap furtheropens as * increases from *0 /3, reaching a local maxi-

mum !2Eg1 /2" at *=*0 /2, before closing again at *

=2*0 /3, and finally recovering its original value 2Eg1 at

*=*0. In Fig. 17, the DOS of a 3-nm-diameter semicon-ducting single-walled tube for various magnetic flux isillustrated. One notes that magnetic-field-induced liftingof the spin degeneracy brings some additional contribu-tion to the total electron magnetic moment !Zeeman ef-fect". This effect has been shown to yield an energy leveldisplacement between spin up and spin down, linearwith the magnetic flux, but inversely proportional to thesquared radius of the tube !Jiang et al., 2000".

The Van Hove singularity splitting was recently ob-served by spectroscopic experiments !Zaric et al., 2004".In addition, several experimental studies of electronictransport spectroscopy at low temperature in the Cou-lomb blockade regime !Kanda et al., 2002; Coskun et al.,2004; Jarillo-Herrero et al., 2004; Minot et al., 2004" or inthe Fabry-Perot regime !Cao et al., 2004; Jarillo-Herreroet al., 2005" have also provided compelling evidences ofthe Aharonov-Bohm effect. The experimental estima-tion of the orbital magnetic moment was found to be ofthe order of %0.7–1.5 meV/T !Minot et al., 2004;Jarillo-Herrero et al., 2005".

Magnetoresistance oscillations were also a subject ofintense controversy in the early stage of carbon nano-tube studies, since the origin and value of the Aharonov-Bohm oscillation period were apparently of different na-tures. Indeed, while some studies of large-diametermultiwall carbon nanotubes !Bachtold et al., 1999" firstrevealed clear signatures of weak localization, withnegative magnetoresistance and !*0 /2"-periodicAharonov-Bohm oscillations driven by quantum inter-ferences !Altshuler and Aronov, 1985", other reports as-signed their magnetoresistance oscillations to field-modulated band structure effects, assuming a negligiblecontribution from interference effects !Fujiwara et al.,1999; Lee et al., 2000". The superimposed contributionsto the Aharonov-Bohm oscillations from both band-structure and quantum interferences effects have beenclearly disentangled recently !Stojetz et al., 2005" andwill be discussed in Sec. IV.D.1.

FIG. 16. Density of states of the !10,10" metallic tube as afunction of energy for several magnetic flux values !see text".Curves have been vertically offset for clarity. Inset: Evolutionof one VHS with magnetic flux. Adapted from Roche et al.,2000.

FIG. 17. Density of states of the !21,23" tube at zero and finiteflux. Top inset: Expanded plot of the DOS. Bottom inset: Evo-lution of the VHS splitting 2B as a function of magnetic field.

690 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

3. Perpendicular field: The onset of Landau levels

In the situation where the magnetic field is appliedperpendicular to the tube axis, the modifications of theelectronic spectrum are profoundly different. First thetwo-dimensional vector potential within the Landaugauge for the nanotube surface is now given by A= „0, !#Ch#B /2#"sin!2#x / #Ch#"…, keeping !x , y" as the co-ordinates along the circumferential and nanotube axisdirections. For evident symmetry reasons, the net mag-netic flux threading the tube is now zero. The phase fac-tors can be computed using either this basis or the Car-tesian basis defined earlier. The energy dispersion canthen be evaluated as a function of magnetic field inten-sity !Ajiki and Ando, 1993, 1996; Saito et al., 1994". InFig. 18, the dispersion relation of the energy E /.0 isreported as a function of the dimensionless wave vectork.#T# /2# !Saito et al., 1994", for several values of thedimensionless inverse magnetic length ;= #Ch# /2#!m,where !m=$1 /eB is the magnetic length !first cyclotronorbit radius".

As seen in Fig. 18, as the intensity of the magneticfield is enhanced, the subband dispersion is reduced,with a particularly strong effect in the vicinity of thecharge-neutrality point. This onset of a Landau-typesubband can be further rationalized analytically. Indeed,by using the k ·p method, an expression for the eigen-states under magnetic field close to the K points can bederived analytically for metallic tubes !see Sec. IV.C.1

for the zero-field case". The k ·p equation at the charge-neutrality point !"k=0" in the presence of a perpendicu-lar magnetic field can be decoupled into two equations!Ando and Seri, 1997":

4−$

$x+

#Ch#2#!m

2 sin*2#x#Ch# +5FA

k !x" = 0, !27"

4+$

$x+

#Ch#2#!m

2 sin*2#x#Ch# +5FB

k !x" = 0, !28"

from which two independent solutions can be obtained:

,A!x" = *10+FA!x", ,B!x" = *0

1+FB!x" ,

FA!x" =1

$#Ch#I0!2;2"exp4− ;2 cos*2#x

#Ch# +5 ,

FB!x" =1

$#Ch#I0!2;2"exp4+ ;2 cos*2#x

#Ch# +5 ,

where I0!2;2" is a modified Bessel function of the firstkind. Note that for sufficiently large magnetic field !;<1" these wave functions become strongly localized inthe circumference direction; that is, ,A!x" is a wavefunction localized around x= ± #Ch# /2 at the bottom sideof the cylinder, whereas ,B!x" is localized around the

FIG. 18. Energy dispersion relation of a !10,0" tube as a function of the dimensionless wave vector ==k.#T# /2# for several valuesof the dimensionless inverse magnetic length ;. !a" ;=0.0, !b" 1.0, !c" 2.0, and !d" 3.0. !e", !f", !g" The energy at k. =0 as a functionof ;2 /NR 'NR is the highest common divisor of !2n+m ,n+2m"( for tubes !20,0", !20,20", and !9,9", respectively. Adapted fromSaito, Dresselhaus, and Dresselhaus, 1994.

691Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

top side x=0. As a result, the boundary condition on thewave function becomes irrelevant and the resulting bandstructures, starting from an initially metallic or semicon-ducting nanotube, become identical !Ajiki and Ando,1993". For a small +k around the K points, the low-energy properties are described by an effective Hamil-tonian, which can be determined by the two degeneratestates ,A and ,B as

Heff = * 0 − i.0+kI0−1!2;2"

+ i.0+kI0−1!2;2" 0

+ , !29"

whose eigenvalues are Eq=0± = ±.0#+k# /I0!2;2", with a

group velocity given by v=.0 /1I0!2;2", while the densityof states becomes 4!EF"/I0!2;2" /#.0/e;

2/$4#;2!;

<1" !Ando and Seri, 1997". The DOS at the charge-neutrality point thus diverges exponentially with in-creasing magnetic field. This is shown in Fig. 19 for the!10,10" tube for several magnetic field strengths.

Given the diameter-dependent scaling property of theband structure, the larger the tube diameter, the smallerthe required value of the magnetic field to fully developsuch a Landau subband at the charge-neutrality point.This effect has also been investigated analytically using asupersymmetry framework !Lee and Novikov, 2003".The appearance of the so-called Hofstadter butterflywas further explored numerically for large diameternanotubes !Nemec and Cuniberti, 2006". As alreadyseen in the field-dependent band structures !Fig. 18", thewhole DOS also progressively degrades as the Landausubbands start to emerge within the whole spectrum, al-though strong mixing between high-energy subbands re-mains !Fig. 19".

As soon as ;= #Ch# /2#!m>1 is satisfied, the electronicspectrum becomes fully dominated by Landau levels.One finds that for tubes with diameters of 1, 10, 20, and40 nm, the condition ;=1 corresponds to magnetic fieldstrengths of 2635, 26, 6.6, and 1.6 T, respectively.

In each case, !m?!e !or @c-e<1" has to be furthersatisfied for clear observation of Landau quantization,where !e is the mean free path, @c=eB /m is the cyclo-tron frequency, and -e is the scattering time !this condi-tion is easily met at such high magnetic fields in carbonnanotubes since !e can be as long as 1 "m". Some signa-ture of such Landau level formation was first reportedby Kanda and co-workers !Kanda et al., 2002".

F. Curvature effects: Beyond the zone-folding model

In the preceding sections, a model for the electronicproperties of SWNTs was based on the confinement ofelectrons around the tube circumference, a confinementshown to induce selection on allowed k! Bloch vectorcomponents. As a matter of fact, since the states se-lected in the band-folding scheme were those of the pla-nar graphene sheet, curvature effects are neglected.However, carbon nanotubes are not just stripes ofgraphene but small cylinders. Carbon atoms are placedon a cylindrical wall, a topology that induces several ef-fects different from those of a planar graphene sheet: !a"the C-C bonds perpendicular and parallel to the axis areslightly different, so that the a1 and a2 basis vectors nowhave different lengths; !b" these bond length changes,and the formation of an angle for the two pz orbitalslocated on bonds not strictly parallel to the axis, yielddifferences in the three hopping terms .0 between a car-bon atom and its three neighbors; and !c" the planarsymmetry is broken so that the # and ' states can mixand form hybrid orbitals that exhibit partial sp2 and sp3

character. Such curvature effect is not taken into ac-count in the zone-folding model of graphene, where the# orbitals cannot mix with the ' states as they showdifferent parity with respect to planar reflection. In thepresent section, the effect of finite curvature on the elec-tronic properties of single-wall nanotubes will be inves-tigated.

The effects labeled !a" and !b" modify the conditionsthat define the k point at which occupied and unoccu-pied bands do cross !a point we label kF" and shift thisFermi vector kF away from the Brillouin zone corners!K point" of the graphene sheet !Kane and Mele, 1997;Yang and Han, 2000". For armchair nanotubes, takingcurvature into account shifts the Fermi wave vectoralong an allowed line of the graphene Brillouin zone.Consequently, for symmetry reasons, armchair tubes al-ways preserve their metallic character with finite curva-ture. However, for metallic nonarmchair nanotubes, kFmoves away from the K point perpendicularly to theallowed k lines such that the allowed 1D subband !k ,q"no longer passes through kF, opening a very small bandgap at EF !see Fig. 20".

In summary, when accounting for curvature effects,the only zero-band-gap tubes are the !n ,n" armchairnanotubes. The !n ,m" tubes with n−m=3l, where l is anonzero integer, are tiny-gap semiconductors. Armchairtubes are sometimes labeled type-I metallic tubes, whilethe others are of type-II. All other nanotubes are

FIG. 19. Density of states of the !10,10" tube in a perpendicu-lar magnetic field for several field strengths. The field strengthsare expressed in terms of the dimensionless parameter ;= #Ch# /2#!m, where !m=$1 /eB is the magnetic length.

692 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

intermediate-gap !a few tenths of an eV" semiconduc-tors. For the tiny-gap semiconducting nanotubes, the so-called secondary gap !due to the curvature" depends onthe diameter and the chiral angle, and scales as 1/dt

2

!Kane and Mele, 1997". For the quasimetallic zigzagnanotubes !chiral angle=0", this secondary gap is givenby

2Eg2 =

3.0acc2

4dt2 !30"

and is so small that, for most practical purposes, all n−m=3l tubes can be considered as metallic at room tem-perature !see Fig. 20". Density-of-states measurementsby scanning tunneling spectroscopy !Ouyang et al.,2001b" confirm the expected 1/dt

2 dependence for threezigzag nanotubes and show that armchair nanotubes re-main truly metallic. Consequently, the band-folding pic-ture, based on the tight-binding approach !Hamada etal., 1992; Mintmire et al., 1992; Saito et al., 1992", contin-ues to be valid for large diameter tubes.

We now discuss point !c". For small tubes, the curva-ture is so strong that some rehybridization among the 'and # states appears. In such a case, the zone-foldingpicture may fail completely and ab initio calculationsshould be performed to predict the electronic propertiesof small diameter nanotubes. As an example, the ab ini-tio band structure of the !6,0" tube is shown in Fig. 21.These first-principles pseudopotential local density func-tional !LDA" calculations !Blase, Benedict, Shirley, andLouie, 1994" indeed revealed that hybridization effectscan occur in small radius nanotubes sufficiently strong tosignificantly alter their electronic structure. Stronglymodified low-lying conduction band states are intro-duced into the band gap of insulating tubes because of

hybridization of the '* and #* states. As a result, theenergy gaps of some small radius tubes are decreased bymore than 50%. In the specific case of the !6,0" tube,which is predicted to be a semimetal in the band-foldingscheme, a singly degenerate hybrid '*-#* state !see Fig.21" is found to lie 0.83 eV !at (" below the doubly de-generate state that forms the top of the valence band inthe zone-folding model. This band overlap makes the!6,0" tube a true metal within the LDA, with a density ofstates at the Fermi level equal to 0.07 state/eV atom.The '*-#* hybridization can be clearly observed bydrawing the charge density associated with the statesaround the Fermi level. Such states are no longer anti-symmetric with respect to the tube wall, with a clear“charge spilling” out of the tube. For nanotubes withdiameters greater than 1 nm, these rehybridization '-#effects are unimportant. Further, as discussed above,symmetry considerations suggest that armchair tubes areless affected by such rehybridization.

Ultrasmall radius single-wall carbon nanotubes !diam-eter of about 4 Å" have been produced by confiningtheir synthesis inside inert AlPO4-5 zeolite channels!with inner diameter of about 7.3 Å" !Wang et al., 2000".The diameter of these tubes gives them many unusualproperties such as superconductivity !Tang et al., 2001".Such a narrow distribution of diameters around 4 Å re-duces the potential carbon nanotube candidates tothree: the !3,3", !4,2", and !5,0". The properties of theseultrasmall tubes have already been extensively investi-gated by ab initio simulations !Dubay et al., 2002; Liuand Chan, 2002; Machón et al., 2002; Cabria et al., 2003".In particular, it was shown that the !5,0" tube, expectedto be semiconducting following the band-folding picture,is actually a metal with two bands !one doubly degener-ate" crossing the Fermi level !yielding two different kF".

FIG. 20. Magnitude of primary !Eg1" and secondary !Eg

2" gapsin carbon nanotubes with radii less than 15 Å. The primarygap !2Eg

1" scales as 1/R !top panel". The secondary gap !2Eg2

or cuvature-induced gap" scales as 1/R2. The dots at 2Eg1

=2Eg2=0 correspond to the armchair nanotubes which always

preserve their metallic character. Adapted from Kane andMele, 1997.

FIG. 21. Ab initio electronic band structure and density ofstates of a !6,0" carbon nanotube, illustrating the strong hybrid-ization that occurs between # and ' states in a small-diametertube. A new band '* appears and crosses the # states aroundthe center of the Brillouin zone. The Fermi level is at zeroenergy. Adapted from Blase, Benedict, Shirley, and Louie,1994.

693Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

This is a clear manifestation of curvature effects. We willcome back to such small tubes when discussing thePeierls and superconducting instabilities in Sec. IV.F.The armchair !3,3" tube remains semimetallic, but with a#-#* band crossing at EF that is displaced off its ideal2(X /3 position, confirming as described above that arm-chair tubes are much less sensitive to curvature effects.

G. Nanotube bundle and multiwall system

From the previous section, we can deduce that only aspecial achiral subset of these carbon structures !arm-chair nanotubes" exhibits a true metallic behavior. Suchmetallic character can be explained by the high symme-try of these !n ,n" tubes, namely, the n vertical planesand glide planes. Incorporating an armchair tube into abundle, or inside another nanotube as in a multiwall sys-tem, could modify its intrinsic electronic properties asthe symmetry is lowered.

Single-wall carbon nanotubes are grown by a laser-ablation, arc-discharge, or CVD method and always oc-cur in bundles of 10–100 nanotubes. These bundles usu-ally consist of nanotubes with different chirality andslightly different diameter. Even a “perfect” crystalmade of identical tubes will alter the properties of theconstituent CNTs through tube-tube interaction. Indeed,first-principles calculations reveal that broken symmetryof the !10,10" tube caused by interactions between tubesin a bundle induces a pseudogap of about 0.1 eV at theFermi energy !Delaney et al., 1998". This pseudogapstrongly modifies many of the fundamental electronicproperties of the armchair tubes, with a specific signa-ture in the temperature dependence of the electricalconductivity and in the infrared absorption spectrum.

In the limit of an isolated !10,10" tube, the two bandscrossing at EF belong to different irreducible represen-tations with respect to the tube symmetry planes, so thatcrossing is allowed. Upon breaking of this symmetry bytube-tube interaction in the hexagonal bundle symmetry,these bands can mix and start to repel at EF !Fig. 22".The presence and magnitude !which depends inverselyon the nanotube radius" of this pseudogap have beenobserved experimentally using low-temperature scan-

ning tunneling spectroscopy !Ouyang et al., 2001b". Incontrast, if !6,6" nanotubes are arranged in a hexagonallattice which fully preserves the D6h symmetry of thehexagonal packing, the band gap due to these intertubeinteractions is not observed !Charlier et al., 1995". Asmall rotation of the !6,6" tubes in such an arrangementwould break the D6h symmetry of the !6,6" bundle andwould open up this expected gap at the Fermi energy!Reich, Thomsen, and Ordejón, 2002".

Another possibility to tailor the electronic propertiesof nanotubes can be observed in the multilayering effect.In fact, the weak interaction between the concentricshells in a multiwall nanotube may have important ef-fects on the electronic properties of the constituent iso-lated nanotubes !Lambin et al., 1994; Kwon andTománek, 1998". Interwall coupling, which, as just men-tioned, opens a pseudogap in bundles of single-wallnanotubes !due to symmetry lowering", may periodicallyopen and close four such pseudogaps near the Fermienergy in a metallic double-wall nanotube upon rotationof its inner shell with respect to the nanotube axis.

Figure 23 illustrates the intriguing interplay betweengeometry and electronic structure during the rotation ofan inside !5,5" armchair nanotube in an outside !10,10"nanotube !both tubes sharing the same axis". The indi-vidual !5,5" and !10,10" tubes are both metallic and showthe preferred graphitic interwall separation of 3.4 Åwhen nested. To determine the electronic properties ofthe double-wall nanotube, a tight-binding techniquewith parameters determined by ab initio calculations forsimpler structures has been used !Lambin et al., 1994;Kwon and Tománek, 1998". Due to the relatively highsymmetry of the coaxial system, consisting of a D10h !5,5"nanotube nested inside a D20h !10,10" nanotube, the de-pendence of the intertube interaction on the tube orien-tation shows a periodicity of 18°. In the absence of theintertube interaction, the band structure of each tube ischaracterized by two crossing linear bands near EF, onefor left- and one for right-moving electrons. The bandstructure of a pair of decoupled !5,5" and !10,10" nano-tubes, a mere superposition of the individual band struc-tures, is shown in Fig. 23!a". Switching on the intertubeinteraction in the !5,5"@!10,10" double-wall tube re-

FIG. 22. Band crossing and band repulsion. !a" Schematic diagram of the crossing of the two linear bands for an isolated !n ,n"carbon nanotube. One band has #-bonding character and the other has #-antibonding !#*" character. EF is the Fermi energy andk is the wave vector. !b" Repulsion of the bands due to breaking of mirror symmetry. Adapted from Delaney et al., 1998.

694 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

moves the near degeneracy of the bands near EF as well'see Figs. 23!b" and 23!c"(. In the most stable orienta-tion, the double-wall system is still characterized by theD10h symmetry of the inner tube. The four bands cross,with a very small change in the slope 'Fig. 23!b"(. Whilethe same argument also applies to the least-stable con-figuration, a markedly different behavior is obtained atany other tube orientation that lowers the symmetry,giving rise to four band crossings 'Fig. 23!c"(. This trans-lates into four pseudogaps in the density of states nearEF.

At the Fermi level, the density of states of double-wallnanotubes is thus affected by the mutual orientation ofthe two constituent nanotubes, since the positions of thefour pseudogaps depend significantly on it. The openingand closing of pseudogaps during the libration motion ofthe double-wall tube is a unique property that cannot beobserved in single-wall nanotube ropes !Kwon andTománek, 1998".

Finally, self-consistent charge-density and potentialprofiles for double-wall nanotubes, considering variouschiralities, have been determined !Miyamoto et al., 2001"and demonstrate that the inner tube modifies the chargedensity associated with states near EF, even outside theouter tube. A significant amount of charge, originatingmainly from # electrons, is transferred into an interwallstate, related to the interlayer state in graphite. In thelimit of small tubes, the significant evolution of the CNTwork function with respect to diameter shows as wellthat charge transfer may occur from one tube to another.

H. Structural defects in carbon nanotubes

In the previous sections, curvature effects and inter-tube and intershell interactions have been shown to sig-nificantly modify the electronic properties of carbonnanotubes from those obtained by a simple band foldingof the graphene band structure. However, until now,each constituent nanotube was assumed to be perfect. Inreality, the intrinsic honeycomb network of CNTs isprobably not as perfect as usually assumed. Defects likepentagons, heptagons, vacancies, adatoms, or substitu-

tional impurities have been proposed theoretically andrecently observed experimentally !Hashimoto et al.,2004; Fan et al., 2005". These defects are found tomodify, at least locally, the electronic properties of thehost nanotubes. Consequently, the introduction of de-fects in the carbon network is an interesting way to tai-lor its intrinsic properties, enabling new potential nano-devices and fostering innovative applications in nano-electronics !Gómez-Navarro et al., 2005". The cases ofchemical doping and functionalization will be exploredin Sec. IV.C.4 where their effect on conductance will beanalyzed.

1. Finite length and capping topologies

We have dealt so far with the properties of infinitelylong nanotubes. In reality, nanotubes have a finite length!up to a few microns", a property which has two mainconsequences: !a" the confinement of the electronicstates along the tube length; and !b" the disruption of theatomic network at the two ends, also labeled tips orapexes, with specific reconstructions and local electronicproperties.

A conducting nanotube cut to a finite length shoulddisplay standing waves characteristic of a one-dimensional particle-in-a-box model. Indeed, when elec-trons are confined in a box, quantum mechanics tells usthat electrons can have only discrete values of kineticenergy. The energy spacing of the eigenvalues dependsdirectly on the dimensions of the box: 2E=h2 /2mL2,with L the length of the box. If this energy spacing ismuch higher than the thermal energy !2E<kBT", thereare only completely occupied and completely empty lev-els and the system is an insulator. Further, the eigen-states are standing waves of the form sin!kz", with k=2#m /L and m an integer !the variable z is along thenanotube axis".

These standing waves have been studied theoreticallyby Rubio et al. !1999", and the highest occupied molecu-lar orbital !HOMO", lowest unoccupied molecular or-bital !LUMO", and “tip states” associated with a typicalfinite-length tube are illustrated in Fig. 24. Such station-ary states have also been observed experimentally by

FIG. 23. Band structures of the same double-wall tube for different relative orientations. Near-degenerate bands with no gapcharacterize the !5,5"@!10,10" double-wall nanotube without intertube interaction !a". In the presence of intertube interaction,depending on the mutual tube orientation, the !5,5"@!10,10" system may show a zero gap !b" in the most symmetric !point groupsymmetry D10h" or four pseudogaps !c" in a less symmetric and stable configuration !point group symmetry C5". Adapted fromKwon and Tománek, 1998.

695Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

means of STS !Venema et al., 1999; Lemay et al., 2001"which essentially sees the square of the wave functionsclose to the Fermi level 'dI!V ,x" /dV/#,F!x"#2(. TheSTS scans display several maxima repeated with a peri-odicity :F60.74 nm. Such an observation requires ahigher energy resolution than the eigenstate separation!2E" and an electron coherence length larger than thetube length, which was satisfied for Ltube/30 nm andT=4 K.

We now turn to the properties of tube tips or apexes.Due to the finite length, interesting structural featuresoccur near the ends of all tubes. The closure of thegraphene cylinder results from incorporation of topo-logical defects, such as pentagons, which induce a discli-nation in the planar hexagonal carbon lattice. Suchmodifications of the structure modify, even though fairlylocally, the tube electronic properties, while the tubebody properties are essentially unchanged due to thelarge aspect ratio of most CNTs. Complex apex struc-tures can arise, for instance, conical-shaped sharp tips,due to the way pentagons are distributed near the endsfor full closure. Each topology leads to a specific localelectronic structure !Tamura and Tsukada, 1995; Char-lier and Rignanese, 2001".

These topological changes in the atomic structuresnear the end of closed carbon nanotubes are known toinitiate sharp resonances in the DOS close to the Fermienergy region !Carroll et al., 1997", affecting locally theelectronic properties of the system, with, for example,expected consequences on field-emission energy-resolved spectra !see Sec. IV.G", or the chemical activity

of the apex, such as an enhanced sensitivity to oxidation!Ajayan et al., 1993", a property used for selective tubeopening at the apex. The energy positions of these reso-nant states with respect to the Fermi level depend sen-sitively on the relative positions of pentagons and theirdegree of confinement at the tube ends !De Vita et al.,1999". The variations of the density of states along a !10,10" nanotube capped by a hemispherical C240 tip apex,containing six pentagons in a fivefold-symmetric ar-rangement, are shown in Fig. 25 for illustration.

2. Connecting nanotubes

Since carbon nanotubes can be metallic or semicon-ducting, depending on their structure, they can beused to form metal-semiconductor, semiconductor-semiconductor, or metal-metal junctions. These junc-tions have an interesting potential for applications inlogical devices. The key issue is to connect two semi-infinite nanotubes of different chirality but with equiva-lent diameters to allow for a smooth !energetically rea-sonable" tube-tube junction. It has been shown that theintroduction of pentagon-heptagon pair defects into thehexagonal network of a single carbon nanotube canchange the helicity of the carbon nanotube and funda-mentally alter its electronic structure !Dunlap, 1994;Lambin et al., 1995; Charlier et al., 1996; Chico, Crespsi,Benedict, Louie, and Cohen, 1996; Saito et al., 1996".Both the existence of such local atomic rearrangementsand the measurement of their respective electronic andtransport properties have been resolved experimentally!Yao et al., 1999; Ouyang et al., 2001a".

Such defects must induce zero net curvature to pre-vent the tube from flaring or closing. The smallest topo-logical defect with minimal local curvature !hence mini-

FIG. 24. Ab initio simulated STS images of the !a" HOMO, !b"LUMO, and !c" tip states of a 4.18-nm-long armchair tube. Thesolid line !A" in !b" corresponds to the line scan shown in !d"where the maxima of the electronic wave function are com-pared to the Fermi wavelength !:F". Adapted from Rubio etal., 1999.

FIG. 25. !Color online" Densities of states along a !10,10"nanotube capped with half a C240 molecule. The horizontalbars indicate zero densities. The Fermi level is located at zeroenergy. The DOS curves are averaged over the atoms compos-ing the sections labeled by a–g on the right-hand side.Adapted from Charlier, 2002.

696 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

mizing the energy cost" and zero net curvature is apentagon-heptagon pair. When the pentagon is attachedto the heptagon, as in the aniline structure, it only cre-ates topological changes !but no net disclination" whichcan be treated as a single local defect. Such a pair willcreate only a small local deformation and may also gen-erate a small change in the helicity, depending on itsorientation in the hexagonal network.

Figure 26 depicts the connection, using a single 5-7pair, between two nanotubes exhibiting different elec-tronic properties. The !8,0" nanotube has a 1.2-eV gap inthe tight-binding approximation, and the !7,1" tube is asemimetal !although a small curvature-induced gap ispresent close to the Fermi energy". Such a system repre-sents thus a semiconductor/metal Schottky junctionwhich could be used, together with similar junctions, asbuilding blocks in nanoscale electronic devices, providedthat their growth is controlled. These carbon-carbonjunctions have been generalized to the case of C/BNheterojunctions !Blase et al., 1997", with BN !boron-nitride" tubes displaying a large band gap !see Sec. III.I".Such junctions could result from the segregation of car-bon atoms in composite boron-carbon-nitrogen tubes, asegregation which is energetically favorable and hasbeen observed experimentally !Suenaga et al., 1997".

While the spontaneous formation during growth of5-7 pairs conveying the synthesis of tube-tube junctionsseems difficult to engineer, another approach has beendeveloped to connect nanotubes. The beam of a trans-

mission electron microscope can indeed be used to lo-cally irradiate carbon-based nanostructures. Covalentlyconnected crossed single-wall carbon nanotubes havebeen created using electron beam welding at elevatedtemperatures !Terrones, Terrones, Banhart, Charlier,and Ajayan, 2000; Terrones et al., 2002". These molecu-lar junctions of various geometries !X, Y, and T" arefound to be stable after the irradiation process. Figure27!a" depicts an ideal X-shaped nanotube connection,where a !5,5" armchair nanotube intersects a !11,0" zig-zag tube. In order to generate a smooth topologicalwelding at the junctions, six heptagons are introduced ateach crossing point to create the needed negative curva-ture. The electronic properties of such junctions, withthe signature of the heptagonal rings, are characterizedby an enhancement of the DOS close to EF, an effectsimilar to that described in the case of pentagons at thetube apex !Charlier, 2002".

Electronic transport measurements on multiwallY-shaped junctions showed that these carbon nanostruc-tures behave as intrinsic nonlinear devices, displayingstrong rectifying behavior at room temperature !Papa-dopoulos et al., 2000". However, theoretical calculationshave shown that the rectifying behavior of Y-shapedjunctions is not an intrinsic property of the branching,but is solely due to the properties of the interfaces be-tween the nanotube branches and metallic leads !Meu-nier et al., 2002". Much more research is needed to pavethe way toward the controlled fabrication of nanotube-based molecular junctions and network architectures ex-hibiting interesting electronic behavior.

3. Vacancies, adatoms, Stone-Wales, etc.

As in many other materials, the existence of defects innanotubes affects the material properties. These defectscan occur in various forms, among which are atomic va-cancies !El-Barbary et al., 2003". A vacancy is simply theabsence of a carbon atom in the hexagonal network.However, as illustrated in Fig. 28!a", an atomic recon-struction of the vacancy !Cs" is found to be more stableenergetically as compared to the unreconstructed va-cancy !D3h" in the graphene sheet. Removing the re-maining two-coordinated C atom 'see Fig. 28!a"( leads toa “divacancy,” which is composed of two pentagonsseparated by an octagon !Gómez-Navarro et al., 2005".

FIG. 26. !Color online" Nanotube-based junctions. !a" Atomicstructure of a !8,0" / !7,1" intramolecular carbon nanotubejunction. The large balls denote atoms forming the heptagon-pentagon pair. !b" The electron densities of states related tothe two perfect !8,0" and !7,1" nanotubes are illustrated withthick and thin lines, respectively. Adapted from Charlier, 2002.

FIG. 27. Carbon-based ideal junctions, exhibiting, respectively,!a" X, !b" T, and !c" Y geometries, respectively. Adapted fromTerrones et al., 2002.

697Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Electron irradiation induces structural transforma-tions in carbon nanotubes, mainly vacancies and intersti-cials, created by the impact of high-energy electrons, fol-lowed by saturation of highly reactive dangling bonds atundercoordinated carbon atoms !Banhart, 1999". De-fects have been intensively studied in irradiated graphite!Telling et al., 2003", and the carbon vacancy-adatompair is certainly one of the most common !Ewels et al.,2002". In addition, it is suggested that both the adatomand the single monatomic vacancy induce magneticproperties in these carbon nanostructures !Lehtinen etal., 2003".

Another well-known form of defect that occurs in car-bon nanotubes is the Stone-Wales reconstruction 'Fig.28!b"(, which creates two pentagon-heptagon pairs bythe 90° rotation of any C-C bond in the hexagonal net-work !Stone and Wales, 1986". Such a topological defectcan be induced by strain and determines the plastic re-sponse and mechanical resistance to tension applied tothe nanotube !Orlikowski et al., 2000; Jensen et al.,2002".

Most of the outstanding properties of carbon nano-tubes rely on them being almost atomically perfect, butthe amount of imperfections and the effect that theyhave on the tube properties have been poorly under-stood to date. Defects are known to modify the elastic,mechanical, and electrical response of carbon nano-tubes. Such defects are present in as-grown tubes, butcontrolling their density externally !i.e., using ion irra-diation" may open a path toward the tuning of the elec-tronic characteristics of the nanotube !Gómez-Navarroet al., 2005".

Following the previous idea of introducing five- andseven-membered rings into hexagonal networks, a novelclass of perfect crystals, consisting of layered sp2-likecarbon sheets containing periodic arrangements of pen-tagons, heptagons, and hexagons, has been proposed!Terrones, Terrones, Hernandez, Grobert, Charlier, andAjayan, 2000". These sheets are rolled up so as to gen-erate single-wall nanotubes !Fig. 29", which resemble lo-cally the radiolaria drawings of Haeckel !1998".

Calculations indicate that these Haeckelite structuresare more stable than C60 and have energies of the orderof 0.3–0.4 eV/atom with respect to graphene. These ide-

ally defective tubes exhibit intriguing electronic proper-ties: density-of-states calculations of Haeckelite tubesrevealed an intrinsic metallic behavior, independent oforientation, tube diameter, and chirality. Further, arather large DOS at the Fermi level is noticed for thefamily of tubes depicted in Fig. 29!b". Such propertiesare clearly related to our discussion of the 5-7 defectsand extend an early prediction on the evolution of elec-tronic properties with increasing defect concentration!Crespi et al., 1997". The predicted ab initio infrared andRaman frequencies !Rocquefelte et al., 2004" allow oneto distinguish these structures unambiguously and mayhelp in identifying them in future syntheses.

I. Optical properties and excitonic effects

We conclude this section on the electronic propertiesof nanotubes by exploring their optical response. As op-tical absorption spectra are conventionally interpretedin terms of transitions between the valence and conduc-tion bands, discussing the interaction with photons justafter discussing the electronic band structure looks like agood idea. However, the importance of many-body ef-fects !electron-hole interactions or excitons" significantlycomplicates this interpretation.

The optical properties of nanotubes are of major im-portance not only for potential applications of CNTs inoptoelectronic devices !Misewich et al., 2003", but also asa powerful tool to relate the observed absorption orphotoluminescence !PL" spectra to the !n ,m" indices ofthe tubes, complementing other techniques such as Ra-man, diffraction, or STM studies. Experimentally, an im-portant step forward was taken with the observation of arather bright and structured PL spectra in the infrared,associated with CNTs isolated in cylindrical micelles!Bachilo et al., 2002; O’Connell et al., 2002". The aggre-gation of tubes in bundles is indeed expected to strongly

FIG. 28. Defects in the hexagonal network. !a" Graphene por-tion containing a vacancy. The carbon network exhibits somereconstruction. !b" Graphene portion displaying a Stone-Walesdefect !two adjacent heptagons surrounded by two pentagons".Adapted from Ewels et al., 2002. FIG. 29. Nonchiral Haeckelite nanotubes of similar diameter

!1.4 nm". !a" Nanotube segment containing only heptagons andpentagons paired symmetrically. !b" Nanotube segment exhib-iting repetitive units of three agglomerated heptagons, sur-rounded by alternating pentagons and hexagons. !c" Nanotubesegment containing pentalene and heptalene units bound to-gether and surrounded by six-membered rings. Adapted fromTerrones, Terrones, Hernandez, Grobert, Charlier, andAjeyan, 2000.

698 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

quench and broaden the luminescence of carbon tubesthrough transfer of hot electrons to metallic tubes wherethey can recombine nonradiatively. This subject of theoptical properties of SWNTs is rapidly growing, and thefollowing topics should be considered as a brief intro-duction to the field.

The first analysis of the optical data relied on the as-sumption that the absorption peaks can be mapped ontothe energy differences between Van Hove singularitiesin the valence and conduction bands. In the case ofnanotubes, the accumulation of states at VHS suggeststhat the optical spectrum will be dominated by transi-tions between these spikes in the density of states. Fur-ther, as the absorption is strongly quenched by the de-polarizing fields for light polarized in transversedirections !Benedict, Louie, and Cohen, 1995;Marinopoulos et al., 2003", the selection rules associatedwith light polarized parallel to the tube !2q=0, q theazimuthal quantum number" will even specify that thestrongest optical transitions will take place between sub-bands with the same angular momentum, yielding theso-called Eii excitation energies. We recall that in theorthogonal !#-#*" model, each q index yields two sym-metric bands, one occupied and one unoccupied, andtransitions between these two subbands are thereforeallowed.

This analysis led to the useful Kataura’s plot !Katauraet al., 1999; Saito, Dresselhaus, and Dresselhaus, 2000;Popov and Henrard, 2004" which gathers on the samegraph the Eii!dt" transition energies as a function of di-ameter dt. The interest of such a representation !see Fig.30" stems from an early remark by White and Mintmire!1998" that the Eii transitions should depend only on thenanotube diameter, and not its chirality, leading to well-defined and -separated Eii!dt" lines !see Sec. III.D

above". The same arguments were developed for the pri-mary band gaps in semiconducting tubes. In particular, itwas suggested that the diameter of CNTs could bestraightforwardly inferred from the optical absorptionpeaks or the resonance energies in Raman spectra,complementing data obtained from the evolution withdiameter of the RBM frequency. This diameter-only de-pendence of Eii transitions works remarkably well at lowexcitation energies, but strong deviations can be seen onthe plot of Kataura et al. by a marked broadening of thehigh-energy Eii lines. This broadening was shown tooriginate in deviations from the linear dispersion of theenergy bands away from the Fermi level, an effect des-ignated as “trigonal warping” !Saito, Dresselhaus, andDresselhaus, 2000".

However, accurate absorption studies on well-calibrated !n ,m" nanotubes showed evidence for somedeviations from the analysis of Kataura et al. since peaksin the absorption spectra and Eii transition energies inbetween Van Hove singularities showed systematic de-viations !Bachilo et al., 2002; O’Connell et al., 2002;Wang and Griffoni, 2005". In particular, the ratioE22/E11, predicted to be equal to 2 in the approximationwhere bands are linear close to EF !Mintmire and White,1998", was found to be significantly smaller !Bachilo etal., 2002", even in the limit of large tubes where the ap-proximation is supposed to work best. While trigonalwarping effects can easily account for deviations from 2of the E22/E11 ratio in small SWNTs, it was a puzzlingresult in the limit of large tubes. This is the so-calledratio problem in SWNTs !Kane and Mele, 2003". Fur-ther, Bachilo et al. !2002" reported the decrease of thePL intensity for SWNTs with small chiral angles !zigzagtubes", an effect that is difficult to understand within theindependent-electron model.

These deviations triggered several theoretical studiesto explore excitonic effects in the CNT optical spectra.Excitonic effects in purely 1D systems have been shownto exhibit very specific features, such as a divergency ofthe binding energy of the electron-hole pairs !Loudon,1959" in a simple 1D generalization of the Mott-Wanniermodel !Elliott, 1957", or the quenching of the so-calledSommerfeld factors !Ogawa and Takagahara, 1991a,1991b" which compensates for the Van Hove singularityat the E11 edge. It is not clear, however, that such effects,valid for strictly 1D objects, should be easily observed incarbon nanotubes.

Following early predictions based on semiempiricalapproaches !Ando, 1997; Kane and Mele, 2003; Perebei-nos et al., 2004", accurate ab initio calculations showedthat bound excitons with binding energies of up to an eVcould be found in semiconducting tubes !Chang et al.,2004; Spataru et al., 2004". This is shown in Fig. 31 in thecase of the !8,0" carbon nanotube. Such calculationswere based on the resolution of the so-called Bethe-Salpeter equations which can be written as follows:

FIG. 30. Energy separation Eii!d" for all !n ,m" values as afunction of CNT diameter dt, with 0.7&dt&3.0 nm. Crossesand open circles denote the peaks of semiconducting and me-tallic tubes, respectively. Solid squares denote Eii!d" values forzigzag tubes. Adapted from Saito, Dresselhaus, and Dressel-haus, 2000.

699Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

!Eck − Evk"AvckS + )

v!c!k!

,vck#Keh#v!c!k!-AvckS = 5SAvck

S ,

!31"

where AvckS is the exciton amplitude, Keh is the electron-

hole kernel, and #vck- is the electron-hole two-bodywave functions in the absence of interactions !taken as abasis to expand the interacting electron-hole eigen-states". The first term on the left-hand side of Eq. !31"corresponds to the quasiparticle spectrum in the absenceof electron-hole interactions !yielding the Eii energies".The second term accounts for the electron-hole interac-tions. The kernel Keh includes two contributions:screened Coulomb interaction and an exchange term.This latter stabilizes triplet states, yielding potentiallylow-lying dark excitons with vanishingly small dipolematrix elements with the ground state which is a singlet.This is a crucial issue since the existence of low-lyingdark excitons dramatically reduces the PL efficiency ofisolated tubes. The application of a magnetic field, bymixing singlet and triplet states, allows us to bypass thisproblem, even though very large fields are needed !Zaricet al., 2005". Clearly, as the electron-hole interactions arescreened, excitonic effects will be predominant when-ever screening is weak, namely, in semiconducting tubes.Further, the binding energy is expected to be large insmall tubes where holes and electrons are spatially con-fined.

These theoretical evaluations of the exciton bindingenergies were confirmed by experimental measurementsyielding values of 0.3–0.4 eV for nanotubes with diam-eters in the 0.7–0.9-nm range !Maultzsch et al., 2005;Wang et al., 2005a". Concerning the helicity-related PLintensity, it was suggested by Reich et al. !2005" thatexciton-exciton resonance effects, strongly depending onthe E22/E11 ratio, and thus on chirality through trigonalwarping, might explain the experimental observations.On more general grounds, the PL efficiency of nano-tubes is found to be rather small. This suggests the exis-tence of rather long radiative lifetimes, allowing for non-radiative processes and/or the existence of low-lyingoptically inactive !dark" excitons. Radiative lifetimes inSWNTs are under intensive theoretical and experimen-tal investigation and results are still very scattered!Hagen et al., 2004, 2005; Wang et al., 2004; Spataru et al.,2005". Other topics, such as electroluminescence, basedon the recombination of electrons and holes injected atthe two different electrodes of an ambipolar transistor!Misewich et al., 2003" or generated by impact excitation!Chen, Perebeinos, Freitag, Tsang, Fu, Lin, and Avouris,2005; Marty et al., 2006", or photoconductivity, where, onthe contrary, the optically excited electron-hole pairs areseparated by an applied bias, are also under investiga-tion, and theoretical results are still very scarce !Perebei-nos and Avouris, 2006".

We conclude this section on the optical properties ofnanotubes by making a small incursion into the physicsof “composite” BCN tubes. Boron nitride nanotubes!Blase, Rubio, Cohen, and Louie, 1994; Rubio et al.,1994" are wide-gap insulators and strong excitonic ef-fects have been shown theoretically !Arnaud et al., 2006;Park et al., 2006; Wirtz et al., 2006" to explain the experi-mentally available optical results !Watanabe et al., 2004;Arenal et al., 2005; Lauret et al., 2005". The prospect ofobtaining lasing materials in the uv range !215 nm, Wa-tanabe et al., 2004" is strong motivation for pursuing thestudy of h-BN systems. Finally, intermediate betweenmetallic or small-gap CNTs and insulating BN tubes,composite BxCyNz systems have been synthesized andPL in the visible range has been demonstrated for sys-tems with a BC2N stoichiometry !Watanabe et al., 1996;Chen et al., 1999; Bai et al., 2000". It has been shown onthe basis of ab inito calculations that the band gap ofsuch systems could vary in the visible range dependingon the size of segregated pure carbon or BN sections, asegregation phenomenon which stabilizes the structure!Blase et al., 1997, 1999; Mazzoni et al., 2006". Such sys-tems, even though opening the way for the design oftube-based optoelectronic devices, remain much lessstudied than CNTs.

IV. TRANSPORT PROPERTIES OF CARBON NANOTUBES

A. Preliminary remarks

Coherent quantum transport in mesoscopic and low-dimensional systems can be rigorously investigated witheither the Kubo-Greenwood !Kubo, 1966" or the

FIG. 31. Excitons in nanotubes. !a" Quasiparticle band struc-ture and !b" optical absorption spectra !with and withoutelectron-hole interaction" for a semiconducting !8,0" carbonnanotube. Adapted from Spataru et al., 2004.

700 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Landauer-Büttiker formalisms !Büttiker et al., 1985".The first approach, which derives from the fluctuation-dissipation theorem, allows one to evaluate the intrinsicconduction regimes within the linear response and givesdirect access to the fundamental transport length scales,such as the elastic mean free path !!e" and localizationlength !A". While !e results from elastic backscatteringdriven by static perturbations !defects, impurities" of anotherwise clean crystalline structure, A denotes the scalebeyond which quantum conductance decays exponen-tially with the system length !L", owing to the accumu-lation of quantum interference effects that progressivelydrive the electronic system from weak to strong localiza-tion. The coherence length L* gives the scale beyondwhich localization effects are fully suppressed owing todecoherence mechanisms, such as electron-phonon!e-ph" or electron-electron !e-e" couplings, treated asperturbations on the otherwise noninteracting electronicgas !weak-localization regime". When !e becomes longerthan the length of the nanotube between voltage probes,the carriers propagate ballistically and contact effectsprevail. In such a situation, the Landauer-Büttiker for-malism becomes more appropriate, since it rigorouslytreats transmission properties for open systems and ar-bitrary interface geometries. In addition, its formal ex-tensions 'nonequilibrium Green’s functions !NEGFs"and the Keldysh formalism( further enable one to inves-tigate quantum transport in situations far from equilib-rium, of relevance for high-bias regimes or situationswith a dominating contribution of Coulomb interactions!Datta, 1995".

Interestingly, to investigate coherent quantum trans-port in a nanotube of length L with reflectionlesscontacts to external reservoirs, the two transport formal-isms are formally fully equivalent !Szafer and Stone,1988". Within the linear response theory, the Kubo con-ductance can be numerically computed as G!E ,L"= !2e2 /L"limt→BTr7+!E−H"D!E , t"8, where +!E−H" isthe spectral measure operator, the trace of whichgives the total density of states, whereas D!t"= 'X!t"−X!0"(2 / t is the diffusivity operator, defining X!t" as theposition operator in the Heisenberg representation andL as the relevant length scale associated with the nor-malization factor !Roche and Mayou, 1997; Roche,1999". In the presence of static disorder, the diffusivityfor a given wave packet will reach a saturation regimewhose value will be related to the elastic mean free path!e!E" through D!E"/v!E"!e!E", with v!E" the velocityof wave packets with energy E. The wave-packet quan-tum dynamics is numerically explored by solving thetime-dependent Schrödinger equation. Such an ap-proach, implemented using order-N computational tech-niques, has been successfully compared to analytical re-sults derived from Fermi’s golden rule !FGR" foruniform disorder !White and Todorov, 1998; Roche etal., 2000". Figure 32 !top" shows the various conductionregimes !ballistic, diffusive, and localized" for wavepackets propagating in CNTs with on-site random fluc-

tuations !Anderson-type elastic disorder". In Fig. 32!bottom", the quantum conductance obtained with theKubo formula for a clean infinite metallic armchairnanotube is shown to be quantized, retrieving theLandauer-Büttiker formulation in terms of conductingchannels.

On the other hand, the Landauer-Büttiker conduc-tance is evaluated from the transmission coefficient

T!E" = tr7(L!E"Gtube!+" !E"(R!E"Gtube

!−" !E"8 , !32"

given as a function of the retarded Green’s functionGtube

!+" !E"= 7EI−Htube− CL!E"− CR!E"8−1 where CR !CL" isthe self-energy accounting for the coupling with theright !left" electrode and (L= i!CL"− CL

!+" !Datta, 1995".These quantities are generally computed through someorder-N decimation technique !López-Sancho et al.,1984". The Landauer-Büttiker formula can be imple-mented with different effective models, such as a tight-binding Hamiltonian or a Hamiltonian derived from firstprinciples.

In the following, the main transport characteristics ofmetallic carbon nanotubes in ballistic or weakly disor-dered regimes will be first addressed. Transport lengthscales will be discussed, as well as conduction regimessuch as weak and strong localization. Further, the effectsof e-ph and e-e interactions will be scrutinized in regardto their fundamental contribution either to decoherenceand inelastic scattering or to the temperature depen-dence of the conductance. The possibility of a strongdeparture from Fermi-liquid behavior will also be dis-

FIG. 32. Conduction regime in nanotubes. Top: Diffusion co-efficient for three typical conduction regimes in !10,10" metal-lic nanotubes. From left to right: ballistic, diffusive, and local-ized regimes are seen at a long time scale. Bottom: Kuboconductance for the ballistic case.

701Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

cussed through a presentation of the Luttinger-liquidmodel, mainly derived for armchair nanotubes, the pre-dictions of which have received experimental supportingevidence.

B. The clean limit

1. Ballistic motion and conductance quantization

For a carbon nanotube of length L between metalliccontact reservoirs, the transport regime is ballistic if themeasured conductance is L independent and only givenby the energy-dependent number of available quantumchannels N!!E" times the conductance quantum G0=2e2 /h, that is, G!E"=2e2 /h$N!!E", including spin de-generacy. This occurs only in the case of perfect !reflec-tion less" or ohmic contacts between the CNT and themetallic voltage probes. In this regime, the expectedenergy-dependent conductance spectrum is easily de-duced, from band structure calculations, by counting thenumber of channels at a given energy. For instance, me-tallic armchair nanotubes present two quantum channelsat the Fermi energy EF=0, or charge-neutrality point,resulting in G!EF"=2G0. At higher energies, the conduc-tance increases as more channels become available toconduction. For illustration, the electronic bands andconductance of the !5,5" metallic tube are displayed inFig. 33 within the symmetric #-#* model.

These values are, however, the uppermost theoreticallimits that could be experimentally measured. In practi-cal situations, lower values are found since reflectionlesstransmission at the interface between the voltage probesand nanotubes is fundamentally limited by interfacesymmetry mismatch, inducing Bragg-type backscatter-ing. Additionally, topological and chemical disorder, aswell as intershell coupling, introduce intrinsic back-scattering along the tube, which also reduces the trans-mission capability. To account for both effects, one gen-erally introduces Tn!E"&1, the transmission amplitudefor a given channel, at energy E, so that G!E"=G0)n=1,N!

Tn!E" !Datta, 1995".

2. Transport properties of CNT-based junctions and contactresistance

Beyond the fundamental interest in understanding thetransport properties of 1D systems, the integration ofCNTs in electronic devices such as field-effect transistors!CNFETs" !Martel et al., 1998; Tans et al., 1998" raisesthe question of the contact resistance, that is, the abilityfor electrons to jump from a metallic electrode, used asthe source or drain, onto the nanotube. In particular, incontrast to the predictions of quantized conductance ob-tained for clean infinite systems, for a given nanotube/electrode contact geometry, a lowering of the transmis-sion across the interface will be systematically obtained.

As first analyzed by Chico and co-workers !Chico,Benedict, Louie, and Cohen, 1996", even for the mostfavorable case, i.e., for an intramolecular nanotube-based heterojunction, the symmetry mismatch betweenincoming and outgoing electronic states yields a trans-mission probability lower than 1. This is illustrated inFig. 34 for clean nanotubes with different helicities!Triozon et al., 2005". Note that such intramolecularjunctions have been experimentally observed by STM!Odom et al., 2002". The reduction of transmission at theinterface is general to all realistic nanoscale junctionsbetween a nanotube and a metallic electrode, or otherinterface geometries leading to different charge injec-tion capabilities.

To discuss this point, we first define two differentclasses of metal-nanotube junctions, namely, the metal–

FIG. 33. Band structure !left", density of states !middle", andconductance !right" for the !5,5" armchair nanotube.

FIG. 34. Quantum conductance in nanotube-based junctions.!a" Top: Illustration of a nanotube-based metal-!12,0"/semiconductor-!11,0"/metal-!12,0" heterojunction. Bottom:Close-up of the interface region with pentagon-heptagon pairdefect at the origin of chirality changes. !b" Correspondingconductance spectra for the single nanotube !11,0" showing theexact number of conduction channels !dotted line", togetherwith the conductance of the double junctions !11,0"-!12,0"!bold line" and !12,0"-!11,0"-!12,0" !bold dashed line".

702 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

metallic-nanotube–metal !M-MCNT-M" and metal–semiconducting-nanotube–metal !M-SCCNT-M" junc-tions. For the former case of metal-metal Ohmiccontacts, that is, in situations where there is hardly anyinterface potential barrier to tunnel through, the contactresistance mainly depends on the local atomic bondingand orbital rehybridization at the interface. For the lat-ter case of M-SCCNT-M junctions, several experimentssuggest that CNTFETs may operate as Schottky-barriertransistors, with a very large contact resistance at lowbias related to a tunneling barrier which can be tunedwith the gate voltage !Heinze et al., 2002; Chen, Appen-zeller, Knoch, Lin, and Avouris, 2005". The charge redis-tribution through the interface, associated with the phys-ics of band bending and its resulting depletion layers,and the possible occurrence of metal-induced gap states!Tersoff, 1984", are expected to depend strongly on therelative positions of the Fermi level and band edges ofthe metal and nanotube in contact. It is unclear, how-ever, if these concepts, accepted for standard 3D de-vices, should be valid in the case of nanotubes, whichcan be described as either molecular objects or 1D sys-tems. It has been shown in particular that various scalinglaws, such as the length of the depletion layer as a func-tion of dopant fraction or the interface dipole, differ sig-nificantly in 1D from their 3D analogs !Léonard andTersoff, 1999; Heinze et al., 2003".

We consider the case of a M-MCNT-M and assumethat #km-=)leikm·l#8m

l - !or #kF-=)leikF·l#8NTl -" are the

propagating states with km !kF" the wave vector in themetal !nanotube". We take #8NT

l - as the localized atomicbasis orbitals !pz like" in cell !l", which will have nonzerooverlap with #8m

l!- for only a few unit cells defining thecontact area '!l− l!" small(. The scattering rate betweenthe metal and nanotube can be qualitatively written fol-lowing the FGR and will be related to ,km#Hcontact#kF-,the coupling operator between the tube and electrodes.This matrix element is related to the chemical nature ofthe interface bonding !covalent, ionic, etc." and to theoverlap ,8NT

l #8ml!-, which will depend strongly on the ge-

ometry and contact configuration between the nanotubeand electrodes !end or side/bulk contacts, length of thecontact, etc." as illustrated in Fig. 35, together with theangular momentum of the atomic orbitals contributingto #km-. The coupling is further optimized wheneverwave-vector conservation is best satisfied, i.e., when km/kF. For instance, in the case of metallic armchairtubes, larger coupling will be achieved for km%2# /3$3acc. A much smaller metallic wave vector willyield a small coupling rate. The tunneling rate from themetal to the nanotube is qualitatively given by

1-

/2#1

2,km#Hcontact#kF-224NT!EF"4m!EF" , !33"

with 4NT!EF" '4m!EF"( the density of states of the nano-tube !metal" at the Fermi level. Note that these consid-erations are derived for the low-bias regime.

Intriguingly, some experiments on metallic tubes havemeasured only a single channel G%G0 at low bias, in-stead of the two theoretically predicted channels, assum-ing #-#* degeneracy at the charge-neutrality point.Anantram !2001" and Mingo and Han !2001" have pro-posed an interpretation in terms of imbalanced couplingstrength between the #-metal !jellium" contact and the#*-metal contact. In Fig. 36, the contribution of bothchannels to the conductance at charge-neutrality point isreported as a function of nanotube length and for twodifferent nanotube diameters. The contribution of the#* metal is shown to almost vanish for a sufficientlylarge diameter.

Several theoretical papers emphasized the importanceof the hybridization between carbon and metal orbitalsat the contact !Nardelli et al., 2001; Dag et al., 2003;Palacios et al., 2003; Okada and Oshiyama, 2005; Keet al., 2006; Nemec et al., 2006", while other work dis-cussed the role of the Schottky barrier !Dag et al., 2003;Shan and Cho, 2004; Xue and Ratner, 2004; Okada and

FIG. 35. Contact type between a nanotube and electrode firstlayers: !a" end contacts and !b" side or bulk contacts. Courtesyof J.J Palacios !Palacios et al., 2003".

FIG. 36. Contribution of # and #* channels at the charge-neutrality point to the total nanotube conductance for arm-chair !10,10" and !40,40" armchair tubes and modeling themetal contact by a jellium. Adapted from Mingo and Han,2001.

703Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Oshiyama, 2005; Park and Hong, 2005; Odbadrakh et al.,2006; Zhu and Kaxiras, 2006". The variations in contactgeometry !end, side, or melted" nanotube length, andmetal type can certainly explain that the conclusions arestill quite scattered. Further, while charge transfers, in-terface states, and the suggested modification of theSchottky barrier height by surrounding molecular di-poles !Auvray et al., 2005" are expected to be well de-scribed by ab initio simulations, it is yet impossible totackle with such accurate approaches micron-long tubesin the presence of a gate voltage.

Finally, for higher bias voltage between conductingprobes, due to the potential drop profile along the tube,the modifications of bands along the tube axis produceadditional backscattering !Anantram, 2000". This Braggreflection is a fundamental point that could explain theexperimental observation of limited turn-on currentwith increasing bias voltage !Frank et al., 1998; Pon-charal et al., 2002; Urbina et al., 2003".

C. Effect of disorder on transport

1. Electronic eigenstates and pseudospin symmetry

In the vicinity of the charge-neutrality point, the bal-listic character of transport properties in metallic carbonnanotubes or graphene is particularly strong, owing tothe linear dispersion relation in conjunction with thespecific symmetry of the eigenstates. These propertieshave been derived within the the so-called k ·p approxi-mation !Slonczewski and Weiss, 1958; DiVicenzo andMele, 1984". Instead of the tight-binding model, whichallows one to compute the full band structure, the k ·papproximation is a local description around the Fermisurface, where the Schrödinger equation is written bydecomposing the Bloch states as ,k=K++k!r"=ei+k·ruK!r",uK!r" obeying the general Bloch condition. For a givenperiodic potential V!r", the Schrödinger equation canthus be simplified as !DiVicenzo and Mele, 1984"

*+p2

2m+12+k2

2m+1+k · p

m+ V!r"+uK!r" = EK++kuK!r" ,

!34"

where p=−i# is the momentum operator and m theelectron mass. The task in the k ·p approximation con-sists in extracting information by expanding uk!r"around the Fermi level, in the same spirit as the tight-binding approximation. Ando and co-workers !Andoand Nakanishi, 1998; Ando, Nakanishi, and Saito, 1998"extended the k ·p approximation to the case of metallic!armchair" nanotubes by expanding the wave functionsaround the K and K! points. The properties of Blochwave functions in the vicinity of K points can be derivedas follows. First, their Wannier representation up to anormalization factor is given by

,k!r" = )! all cells

eik·!'b19A!r − !" + b29B!r − !"( , !35"

where 9i=A,B!r"=pz!r−ri=A,B" to account for the two or-bitals per unit cell, whereas !b1 ,b2" describe the ampli-tude of the pz orbital for the two carbon atoms in theunit cell. Then, following the definitions of Fig. 2 andusing Eq. !12", the eigenstates for k=K++k are derivedfrom

* E!k" − .0/!k"− .0/

*!k" E!k" +*b1

b2+ = *0

0+ , !36"

with /!k"=1+e−ik·a1 +e−ik·a2. By choosing K= !4# /3$3acc ,0", one obtains /!k"=1+e−2i#/3e−i+kxa/2

+e2i#/3e−i+kya/2 and the problem is recast into

* E!+k" 3.0acc!+kx + i+ky"/23.0acc!+kx − i+ky"/2 E!+k" +*b1

b2+ = *0

0+ .

!37"

The dispersion relations are found by setting the deter-minant to zero, E!+k"= ±1vF#+k# 'noticing that E!k"=E!K"++k $E /$k=E!+k"(, whereas the eigenvectorsmust satisfy b1

2!+kx− i+ky"=b22!+kx+ i+ky". An obvious

solution is b1e−i%k/2= ±b2ei%k/2 'defining %k=arctan!+ky /+kx", the angle between +k and the ky axiswhich corresponds to the tube axis direction(, yieldingtwo possible choices

#s = ± 1- =1$2

*s e−i%k/2

ei%k/2 + , !38"

where s=1 indicates positive energy, whereas s=−1 de-scribes states with negative energy, with respect to thecharge-neutrality point. In the basis 7#s=1- ; #s=−1-8, theHamiltonian reads H=1vF#+k#'z, with 'z the usual Paulimatrix. The Schrödinger equation in the k ·p approxima-tion can thus be viewed as a !decoupled" two-componentmatrix equation !one component for each sublattice",which is formally equivalent to the Dirac equation,where the spinor is not the electron spin but a pseu-dospin representing the sublattice. Additionally, sincethe energy of the bands touches EF, the problem isanalogous to a free massless neutrino on a cylinder!Ando, 2005". The vectors 1/$2!±1,1" are eigenstates of'x with eigenvalues ±1, and the pseudospin for a statewith arbitrary vector +k is deduced by applying to1/$2!±1,1" a rotation operator with angle %k about the zaxis 'perpendicular to the tube direction; Fig. 37!c"(,withthe corresponding rotation matrix !Ando, Naka-nishi, and Saito, 1998"

R'%k( = *ei%k/2 00 e−i%k/2 + . !39"

Thus, finally, in the vicinity of the K points, the elec-tronic wave functions can be expanded, up to some nor-malization factor, as

704 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

,k=K±+k,s=±1!r" /1$2

*se+i%k/2

e−i%k/2 +ei!+kxx++kyy". !40"

In Fig. 37 a schematic representation of eigenstates isprovided for the sake of illustration. Assuming an initialFermi energy slightly downshifted with respect to thecharge-neutrality point !s=−1", the two available orbit-als for elastic intravalley scattering are shown. The totalwave function is given by ,k=K±+k,s=−1!r" 'Eq. !40"( timesthe bonding or antibonding component !set as symbolsin Fig. 37", which are obtained in the limit #k-= #K-,where E!K"=0, and which gives two degenerate eigen-states formed by either a symmetric or an antisymmetriccombination of the pz orbitals !#,K-= 7#K+- , #K−-8":

,r#K+- = )!

eiK·!

$2'pz!r − rA − !" + pz!r − rB − !"(

!#-antibonding state",

,r#K−- = )!

eiK·!

$2'pz!r − rA − !" − pz!r − rB − !"(

!#*-bonding state".

2. Long-range disorder and the absence of backscattering

If we consider an impurity bound to the surface ofthe tube, typically by van der Waals coupling, the impu-rity potential U!r" is slowly varying on the scale of theinteratomic distance acc. U!r" can thus be regarded as aperturbation to the Hamiltonian Hk·p, and the matrixelements ,,k,s#U!r"#,k!,s!- of the potential between theBloch states 'Eq. !40"( describe the scattering probabil-ity amplitude k→k! due to the single impurity, which inprinciple results in decreasing conductance. Such a long-range potential generally involves low momentum trans-fer, which guarantees the applicability of the effectivemass approximation, generally ignoring interband tran-sitions.

Assuming a long-range impurity potential, Ando et al.!Ando and Nakanishi, 1998; Ando, Nakanishi, and Saito,1998" demonstrate that both intravalley !k=K±+k→k!=KD+k and the same changing K to K!" and intervalley!k=K±+k→k!=K!D+k and the same changing K toK!" scattering probabilities were vanishingly small. Thecase of intravalley scattering !say around K" was inves-tigated by computing the terms ,s ,+k#T#s! ,+k!-, develop-ing the T matrix recursively through a Dyson equation'G= !E−H0−U"−1(

T = U + UGU = U + UG0U + UG0UG0U + ¯= U + U

1E − H0

U + U1

E − H0U

1E − H0

U + ¯ . !41"

In this expansion, the k ·p Hamiltonian around the Kpoint can be reduced to H0=.0!'xpx+'ypy" !'x and 'ythe Pauli matrices", whereas U has a diagonal represen-tation, whose elements provide the impurity potentialon-site energies !Ando, Nakanishi, and Saito, 1998". Theterm of type ,s! ,+k!#T#s ,+k- can be expanded on the ba-sis of eigenstates, and one is left with

,s!,+k!#U#s,+k- % U!+k − +k!"!s ei%k/2,e−i%k/2"

$*s e−i%k!/s

e−i%k!/2+

% U!+k − +k!"!ss! e−i!%k−%k!"/2

+ e+i!%k+%k!"/2" , !42"

where U!+k−+k!"=3dr U!r"e−i!+k−+k!"·r. The backscatter-ing amplitude for the case !s=s!= ±1" thus becomes,s ,+k#U#s ,−+k-%U!2+k"cos!%k+%−k" /2=0. This can bestraightfowardly generalized to all higher-order terms inthe perturbation series !Ando, Nakanishi, and Saito,1998" given by

,s,− +k#T!E"p#s, + +k- % )s1k1

)s2k2

¯ )spkp

U!− +k − +kp"U!+kp − +kp−1" ¯ U!+kp − +k"'E − 6sp

!+kp"('E − 6sp−1!+kp−1"( ¯ 'E − 6s1

!+k1"(

$ ,s#R'%−k(R−1'%kp(#sp-,sp−1#R'%kp

('R−1'%kp−1(#sp−1-( ¯ ,s1#R'%k1

(R−1'%k(#s- , !43"

where the rotation matrix R'%kp( is defined by Eq. !39".

Therefore, because of the symmetries of eigenstates, alltime-reversal terms 'like those illustrated in Fig. 37, bot-tom, !a" and !b"( cancel out, so that the total amplitude isproportional to

,s#R'%k(R−1'%−k(#s- = cos!%k + %−k"/2, !44"

which equals zero since %k+%−k= ±# !see Fig. 37". Inconclusion, to all orders in the perturbation expansion,

backscattering is suppressed in the low-energy rangearound the charge-neutrality point. This property hasalso been confirmed by numerical calculations !Andoand Nakanishi, 1998; McEuen et al., 1999".

The applicability of this result is, however, restrictedto metallic nanotubes, in situations of slowly varying po-tential, and for energy windows that shrink to zeroaround the charge-neutrality point as the diameter ofthe nanotube increases. For semiconducting tubes, these

705Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

pseudospin properties do not apply and backscattering isfound to be much stronger. This picture has been dis-cussed on the basis of experimental data by McEuenet al. !1999".

3. Short-range disorder and elastic mean free path: Modelanalysis

For a more general and in-depth understanding of dis-order effects, including interband scattering in the pres-ence of short-range disorder, evaluation of the elasticmean free path is fundamental. For sufficiently weak dis-order, a perturbative treatment can be performed withinthe FGR, giving direct access to the elastic mean freepath !e=vF-. This was first derived by White andTodorov !1998", by reducing the band structure to a two-band approximation, as an effective model of the twodegenerate bands at the charge-neutrality point for arm-chair nanotubes. By further considering the on-siteAnderson-type disorder !see below", an analytical for-mula for !e was derived. !e was found to scale linearlywith diameter for a fixed disorder strength, while at afixed diameter the expected disorder scaling was shownto be !e/1/W2, W measuring the variation range of theon-site perturbing potential. The analytical derivation ofsuch a fundamental length scale first requires the calcu-lation of the total density of states !DOS" in the vicinityof the Fermi level. As shown in Sec. III, the DOS iswritten as 4!E"= 1

5Tr'+!E−H"( where the trace has to bedeveloped over a complete basis set. Using the DOSgiven by Eq. !22", application of the FGR yields

12-e!EF"

=2#1

2,,n1!kF"#U#,n2!− kF"-22

$4!EF"NcNring !45"

with Nc and Nring, respectively, the number of pair atoms

along the circumference and the total number of ringstaken in the unit cell used for diagonalization, whereasthe eigenstates at the Fermi level are rewritten as

#,n1,n2!kF"- =1

$Nring)

m=1,Nring

eimkF#/n1,n2!m"- ,

with

#/n1!m"- =1

$2Nc)n=1

Nc

e2i#n/Nc'#pzA!mn"- + #pz

B!mn"-( ,

#/n2!m"- =1

$2Nc)n=1

Nc

e2i#n/Nc'#pzA!mn"- − #pz

B!mn"-( .

!46"

The disorder considered here is an uncorrelated whitenoise !Anderson-type" distribution given by

,pzA!mn"#U#pz

A!m!n!"- = 6A!m,n"+mm!+nn!,

,pzB!mn"#U#pz

b!m!n!"- = 6B!m,n"+mm!+nn!,

,pzA!mn"#U#pz

A!m!n!"- = 0, !47"

where 6B!m ,n" and 6A!m ,n" are the on-site energies onatoms A and B in position !m ,n", randomly distributedwithin the interval '−W /2 ,W /2( and following some uni-form distribution with probability P=1/W. Then by re-placing Eq. !46" in Eq. !45" and using Eq. !47", a straight-forward calculation gives

1-e!EF"

=#4!EF"

1 * 1$NcNring

)NcNring

6A2

+1

$NcNring)

NcNring

6B2 + . !48"

Hence, if the disorder is described by random fluctua-tions of on-site energies with uniform probability 1/W!W the disorder bandwidth", the mean free path can fi-nally be analytically derived as !White and Mintmire,1998; Roche et al., 2000"

!e =18acc.0

2

W2$n2 + m2 + nm . !49"

For the armchair m=n=5 nanotube, with disorder W=0.2.0, by applying Eq. !49", one finds !e/560 nm,which is much larger than the circumference length. Asshown in Figs. 38 and 39, numerical studies !Triozon etal., 2004" confirm the scaling law of the mean free pathwith the nanotube diameter close to the charge-neutrality point. For semiconducting bands, the 1/W2

scaling law is still satisfied, but the mean free paths areseen to be much smaller and do not scale with diameter.

Besides such analytical results, a numerical analysis ofthe Landauer conductance in the case of such static uni-form disorder was first performed by Anantram andGovindan !1998". The conductance was found to bemuch more sensitive in regions of higher densities of

FIG. 37. Scattering states. Top panel: Representation of lineardispersion bands in the vicinity of a K point. The eigenstatesavailable for scattering are pinpointed for a given Fermi levelbelow the charge-neutrality point. Bottom panel: Schematicillustration of the pseudospin rotation corresponding to scat-tering processes !a" "k→"k1→"k2→−"k and !b" "k→−"k2→−"k1→−"k. We choose %k=0 and %−k=#. In !c", a represen-tation of the local axis orientations with respect to the nano-tube.

706 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

states, whereas it was almost unaffected by moderatedisorder close to the charge-neutrality point !Ando andSeri, 1997".

4. Influence of doping on transport properties

The issue of doping is central to the use of CNTs inelectronic devices. In particular, standard logic devicesare based on p- or n-doped junctions, even though it hasbeen proposed that a field effect could be achieved withundoped tubes thanks to a gate-voltage tuning of theSchottky barrier at the tube/electrode interface !Heinzeet al., 2002; Appenzeller et al., 2004; Chen, Appenzeller,Knoch, Lin, and Avouris, 2005".

While the desired effect of doping in semiconductingtubes is to bring the Fermi level in !or close" to thevalence or conduction bands, several theoretical workshave emphasized that the perturbing potential createdaround an impurity in CNTs can induce a strong back-scattering of the propagating wave packets at specific

energies, thus reducing the mean free path and mobilityof the corresponding free carriers !Ando and Nakanishi,1998; Ando, Nakanishi, and Saito, 1998; Choi et al., 2000;Kaun et al., 2002; Latil et al., 2004; Mahan, 2004; Son etal., 2005; Adessi et al., 2006". Similar effects can be as-cribed to the presence of defects such as vacancies, di-vacancies, or pentagon or heptagon rearrangements!Chico, Bendedict, Louie, and Cohen, 1996; Chico, Cre-spi, Benedict, Louie, and Cohen, 1996; Orlikowski et al.,2000". This reduction of conductance occurs in particularat the energy of the !quasi"bound states !Choi et al.,2000; Mahan, 2004" associated with the defects or impu-rities in the CNTs, leading to the terminology of reso-nant backscattering. The same physics of resonant back-scattering has been seen in the case of doped siliconnanowires !Fernández-Serra et al., 2006a, 2006b". Thescaling properties of such bound states in the case ofdisorder and mixed B and N doping have been analyzedby Lammert and co-workers !Lammert et al., 2001".

Several interesting effects related to the presence ofsuch bound states were theoretically proposed. The po-sition in energy of these quasibound states was shown tobe strongly affected by an applied electric field with thepossibility of switching the current with a transverse Efield !Son et al., 2005". Further, it was proposed that thetrapping of localized states by defects or impuritiesshould result in the formation of quantum dots along theCNT body !Chico et al., 1998".

Substitutional doping by nitrogen or boron impuritieshas certainly been the most studied at the theoreticallevel !Choi et al., 2000; Lammert et al., 2001; Kaun et al.,2002; Latil et al., 2004; Son et al., 2005; Adessi et al.,2006". Substitutional doping by nitrogen or boron, re-spectively, n- and p-type dopants !Yi and Bernholc,1993", was achieved very early, either intentionally or inseveral attempts to synthesize composite BxCyNz tubes.While incorporation of boron is found to be rather lim-ited, at least lower than 1% which is the resolution limitof electron-energy-loss spectroscopy !EELS" chemicalanalysis, nitrogen is believed to be incorporated in muchlarger quantities with several types of bonding !three-fold, pyridinelike, etc.", even though it induces at largepercentage severe topological modifications !bamboo-shaped tubes". A thorough review of N doping has beengiven by Ewels and Glerup !2005".

Figure 40 shows the effect of a single N impurity onthe DOS, the conductance, and the scattering phaseshifts of the two eigenchannels !Choi et al., 2000" for ametallic !10,10" nanotube. This work was the first ab ini-tio study of doped nanotubes !within the Lippman-Schwinger approach". Even though the case of a singleimpurity was studied !due to computer time limitations",such ab initio simulations provide a unique referencethat allows one to build realistic models of the scatteringpotential generated by dopants or defects. The contourplot !Fig. 40, right" shows the quasibound state at0.53 eV which is at the origin of strong backscattering,whereas the rest of the spectrum is almost unaffected bythe resonance.

FIG. 38. Energy-dependent mean free path as a function ofdiameter. Inset: 1 /W2 scaling in agreement with the Fermigolden rule. Adapted from Triozon et al., 2004.

FIG. 39. Mean free paths for the metallic !5,5" and semicon-ducting !8,0" tubes with the same value of disorder strength.The conductance results !inset" are equivalent in both theKubo and Landauer formalisms. Adapted from Triozon et al.,2004.

707Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

While most work has focused on the effect of a singleisolated defect, a few studies !Latil et al., 2004, 2005;Adessi et al., 2006", combining ab initio calculations witha semiempirical #-#* Kubo approach to transport, havestudied the effect of a random distribution of substitu-tional or physisorbed dopants at various concentrationsfor micron long tubes. Such studies allow one in particu-lar to extract relevant mesoscopic information such as!e!E". In Fig. 41, the mean free path for long metallicboron-doped nanotubes is shown as a function of impu-rity density and CNT diameter, at a fixed Fermi energy.The downscaling of !e with impurity density and the up-scaling of !e !at fixed density" with tube diameter arereproduced, showing good agreement with the FGR re-sults derived for uniform disorder !Latil et al., 2004".

In the work of Liu and co-workers !Liu et al., 2001",the electronic transport of boron-doped nanotubes hasbeen investigated experimentally. The concentration ofboron atoms was evaluated to be %1% whereas the di-ameters of tubes were estimated in the range'17 nm,27 nm(. Mean free paths on the order of !e=220–250 nm were inferred from weak-localizationtheory. Applying the analytical form of Eq. !49" for !ewith the corresponding parameters !the dopant concen-tration and on-site boron energy can be mapped onto aneffective W value", one finds a theoretical estimate of!e%274 nm for the tube with diameter 17 nm, in agree-ment with experimental estimates. Such studies allowone to test on realistic systems previous studies per-formed on various models of uniform disorder !Anan-tram and Govindan, 1998; White and Todorov, 1998;Triozon et al., 2004" and make a quantitative connectionwith experiments. The case of a limited number !a fewtens" of realistic scattering centers was also explored forcovalently functionalized !Lee et al., 2005" or irradiated!Biel et al., 2005; Gómez-Navarro et al., 2005" tubes andit was shown again that a strong modification of theCNT atomic structure should quickly lead to a regime ofAnderson localization, provided that the transport re-gime remains quantum-mechanically coherent !i.e., inthe absence of electron-phonon or electron-electron in-elastic scattering".

The large drop of the mean free path !or mobility" insubstitutionally doped tubes can be partially bypassedby adopting other doping strategies. It was shown in par-ticular that physisorption doping, where, e.g., alkali-metal atoms !Rao et al., 1997; Petit et al., 1999; Jougueletet al., 2000; Zhou et al., 2000; Bendiab et al., 2001; De-rycke et al., 2002; Appenzeller et al., 2004; Radosavljevicet al., 2004" or molecules !Kazaoui et al., 1999; Konget al., 2000; Kong and Dai, 2001; Takenobu et al., 2003;Auvray et al., 2005" are adsorbed on the tube, leads to amuch larger mean free path than substitutional doping!Latil et al., 2005; Adessi et al., 2006". Alkali-metal atomslocated either outside or inside CNTs act as donor im-purities !Miyamoto et al., 1995; Rubio et al., 1996" whilehalogen atoms, molecules, or chains act as acceptors!Rao et al., 1997; Grigorian et al., 1998; Kazaoui et al.,1999; Fan et al., 2000". As yet another example,fullerenes or metallofullerenes, encapsulated insideCNTs, have been used to tune the band gap and/orFermi level of the host tube !Smith et al., 1998; Hiraharaet al., 2000; Hornbaker et al., 2002; Lee et al., 2002". En-dohedral doping, that is, intercalation inside the tubes, isexpected to allow for good structural stability as the at-oms and molecules are not expected to desorb upon in-creasing temperature.

Several issues are still under debate. It has been ob-served that as-grown tubes present naturally a p-typebehavior in CNTFETs !Martel et al., 1998". The presenceof holes has been ascribed either to charge transfer frommetallic electrodes !Martel et al., 1998; Tans et al., 1998"or to the presence of oxygen adsorbed on the tube !Col-lins et al., 2000; Kong et al., 2000; Sumanasekera et al.,2000". Another important issue is related to the exis-

FIG. 40. !Color online" Bound states and resonant backscatter-ing. Left: Effects of a single nitrogen impurity on conductance!top", the local density of states !middle", and the phase shift ofeigenchannels !bottom" in the !10,10" nanotube. Right: Con-tour plot of the totally reflected state at 0.53 eV. Adapted fromChoi et al., 2000.

FIG. 41. Scaling of the mean free path at the Fermi level, for aB-doped !n ,n" nanotube. Left: In the case of a !10,10" nano-tube with various boron concentrations, !e behaves like theinverse of the doping rate. Right: For a fixed concentration ofB atoms, !e is a linear function of the nanotube’s diameter.

708 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

tence or not of a Schottky barrier at the tube/electrodeinterface. From this perspective, it is not clear if thechange in CNTFET characteristics upon doping is re-lated to a modification of the intrinsic properties of thetube or of the Schottky barrier at the tube/electrode in-terface !Derycke et al., 2002; Appenzeller et al., 2004;Radosavljevic et al., 2004; Auvray et al., 2005".

To conclude this section, we emphasize that the issueof doping by physisorption of molecules, or more gener-ally the modification of the electronic properties ofCNTs by molecular adsorption, is at the heart of a grow-ing and potentially important field, namely, that ofchemical sensors based on CNTs !Wong et al., 1998;Baughman et al., 2000; Collins et al., 2000; Kong et al.,2000; Giannozzi et al., 2003; Peng and Cho, 2003; Jhi etal., 2005". The key issue for such devices is selectivityand sensitivity; namely, can we distinguish from the CNTI /V modifications upon molecular adsorption betweentwo different donor !or acceptor" molecules, and whatminimum adsorbate concentration is needed to induce ameasurable effect on the conductance. The 1D characterof CNTs and the large variation of conductance dis-cussed above in the case of substitutional doping clearlysuggest that such a device should present unprecedentedsensitivity. The sensing properties of CNTs can be fur-ther modified or tailored by covalent functionalization.While many experimental syntheses of covalently func-tionalized CNTs have been performed !Wong et al.,1998; Bahr et al., 2001; Shim et al., 2001; Chiu et al., 2002;Kamaras et al., 2003; Strano et al., 2003", the theoreticalinvestigation of the related electronic and transportproperties is still in its infancy !Chiu et al., 2004; Lee etal., 2005".

5. Multishell conduction

Multiwalled nanotubes or bundles of single-wallednanotubes present additional geometrical complexitydue to the coupling between shells, yielding multishelltransport. Multiwalled nanotubes are made of a few totens of shells with random helicities weakly coupledthrough van der Waals interactions and weak electronicdelocalization !Charlier et al., 1994". The intershell cou-pling can be determined within a tight-binding schemeby keeping one p! orbital per carbon atom, zero on-siteenergies, constant nearest-neighbor hopping on eachlayer n, and some effective hopping form for describingneighboring-shell #-# coupling !Charlier andMichenaud, 1993; Saito et al., 1993; Lambin et al., 2000",leading to the following Hamiltonian:

H = .04)i,j

#p!j -,p!

i #5− E4)

i,jcos!%ij"e−!dij−a"/+#p!

j -,p!i #5 , !50"

where %ij is the angle between p!i and p!

j orbitals and dijdenotes their relative distance. Typical parameters are.0=2.9 eV, a=3.34 Å, and +=0.45 Å. The difference be-tween SWNTs and MWNTs stems from the parameter E.

An ab initio estimate gives E%.0 /8, which enables wavepackets to redistribute among the different shells of theMWNT !Lambin et al., 2000". Topologically speaking,two kinds of multiwall nanotube can be constructed.

The first class is made from nanotubes whose helici-ties allow for commensurability between shells. As a re-sult the full MWNT is a periodic object defined by asingle unit cell. This is, for instance, the case for!5,5"@!10,10" formed by two armchair metallic tubes or!6,4"@!12,8"@!18,12", which consists of two semiconduct-ing shells enclosed by a metallic one. Indeed, #T!5,5"#= #T!10,10"#%2.459 Å whereas #T!6,4"#= #T!12,8"#= #T!18,12"#%18.79 Å, so that all shells in the MWNT have the sametranslational vector unit along the common axis.

In contrast, in MWNTs such as !6,4"@!10,10"@!17,13"there exists an intrinsic incommensurability betweenshell registries. Indeed, the translational vectors alongeach shell are, respectively, #T!6,4"#=3$19acc, #T!10,10"#=$3acc, and #T!17,13"#=3$1679acc, so that the ratios of thelengths of the individual shell translational vectors be-come irrational numbers and no unit cell can be defined.

As a consequence, depending on the individual shellhelicity, one can obtain either translationnally invariantor aperiodic objects. The weak electronic coupling be-tween neigbhoring shells thus defines the possibility ofvery different intertube coupling and charge-transfercharacteristics, whose consequences on electronic bandstructure and transport properties are discussed in thenext section.

a. Commensurate multiwalled nanotubes

Since commensurate MWNTs are periodic objectswith a well-defined unit cell, the Bloch theorem appliesand their band structures can be easily computed. Giventhat shells interact only weakly, the conductance spec-trum of a MWNT in the ballistic conduction regime isgiven as the sum of all conducting channels at a givenenergy !Fig. 42". Accordingly, a very small intrinsic resis-tance is expected at EF for a metallic MWNT, providedballistic conduction is established and the charge is al-lowed to explore all available conducting channels.However, as discussed below, at various energies an in-tershell interaction might be at the origin of the stepwisereduction of conduction channels. We consider a genericMWNT made of coaxial metallic shells with perfectcommensurability, namely, armchair double-walled!5,5"@ !10,10" and triple-walled !5,5"@ !10,10"@ !15,15" nanotubes. Such MWNTs have a fivefold com-mon symmetry. Their respective orientation might alsopossess additional symmetry planes perpendicular to thetube axis. In that case, the interwall interaction yields nochanges over the whole spectrum, which is a superposi-tion of independent spectra. At the charge-neutralitypoint the conductance should thus be G=6G0. However,if the symmetry is lowered by disorienting !rotationallyand translationally" one nanotube with respect to an-other, then splitting of the degeneracy occurs andpseudogaps are formed !Kwon and Tománek, 1998;

709Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Lambin et al., 2000". Figure 42 illustrates such a phe-nomenon.

The presence of pseudogaps in the density of stateshas direct consequences on the available energy-dependent conduction channels. As shown by Sanvitoand co-workers !Sanvito et al., 2000", the conductance isreduced at the charge-neutrality point. One notes thatthis effect of intershell interaction is, however, specific torotational disorientations of neighboring shells with C5hsymmetry. Other commensurate MWNTs such as!6,6"@ !11,11" with no C5h symmetry will not be sensi-tive to this phenomenon.

b. Incommensurate multiwalled nanotubes

The case of incommensurate shells is even more in-triguing and challenging, since the Bloch theorem is nolonger applicable, owing to the lack of translational in-variance along the MWNT axis. To ascertain the intrin-sic quantum transport properties in these incommensu-rate systems, it is necessary to investigate howpropagating wave packets are sensitive to the intershell#-# orbital coupling.

Analysis of the time-dependent evolution of an elec-tronic wave packet initially localized in the outer shell isa first instructive step. This is achieved by solving thetime-dependent Schrödinger equation. In a commensu-rate system, some redistribution of the weight of the

wave packet on each inner shell was numerically foundto occur at a time scale -ll/1.0 /E2 defined by the inter-shell coupling strength and well understood within theFermi golden rule. This is illustrated in Fig. 43 where theredistribution of a wave packet initially localized in theouter shell is shown !Roche et al., 2001a". From thoseresults, one can estimate that for a source-drain spacingof the order of /1 "m, the ballistic time of flight/45001 /.0 will be two orders of magnitude larger than-ll !for E=.0 /8", which points toward the important con-tribution of multishell conduction.

Nevertheless, the nature of the intrinsic conductionregime has been strongly debated, with some numericalworks in favor of a negligible contribution of intershellscattering for charge energies at the charge-neutralitypoint, whatever the underlying aperiodic potential!Yoon et al., 2002; Mayer, 2005; Uryu and Ando, 2005".In contrast, by studying numerically the quantum dy-namics of wave packets over a larger range of energies,the situation was found to become more complex, with ageneral nonballistic regime, described by $D!t"t/At=

!Roche et al., 2001a; Triozon et al., 2004". The coefficient= is found to decrease from 1 to /1/2 depending on thedegree of registry mismatch between neighboring shellsand the energy of the charge carriers !Roche et al.,2001b". Figure 44 shows, at several energies, the timedependence of the diffusion coefficients for the incom-mensurate !6,4"@ !17,0"@ !15,15" and commensurate!5,5"@ !10,10"@ !15,15" MWNTs !Triozon et al., 2004".Whatever the Fermi energy of the wave packets, theconduction remains ballistic in a defect-free commensu-rate MWNT. In contrast, for incommensurate systems,depending on the considered energy of charge carriersand the resulting hybridization strength between neigh-boring shells, charge conduction displays a generalpower-law behavior of D!t". This anomalous diffusionyields a specific length scaling of conductance as shownin Fig. 44 !right frame". At the charge-neutrality point,wave packets essentially remain confined to the outer

FIG. 42. Effect of the rotational symmetry breaking for a com-mensurate !5,5"@!10,10"@!15,15" MWNT on !a" its electronicproperties, !b" its DOS, and !c" its band structure. Adaptedfrom Lambin et al., 2000. Pseudogaps !d" and associated con-ductance spectra !e" for !5,5"@!10,10"@!15,15". Adapted fromSanvito et al., 2000.

FIG. 43. Time-dependent evolution of total wave-functionprobability on a given shell !m ,n" of a multiwalled nanotube, ifat initial time !t=0" the wave packet is fully localized in theouter shell. Left: Commensurate case !6,4"@!12,8"@!18,12",with a close-up of the situation for shell !12,8" in the inset.Right: Incommensurate case !6,4"@!10,10"@!17,13".

710 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

shell as they spread in time and the carrier motion re-mains ballistic with a quantized conductance G=4e2 /h.In contrast, at energy E=1.5 eV, G!L"/!2e2 /h"$!L /L0"!=−1"/=, with L0 !or =" an energy-dependentcharacteristic length !exponent". This anomalous lengthscaling of the conductance has been obtained numeri-cally using both Kubo and Landauer calculations !Trio-zon et al., 2004; Chen and Yang, 2005".

Recently, Wang and Grifoni !2005" have succeeded ininvestigating analytically the electronic scattering rate ofelectrons propagating in the outer shell of a double-walled nanotube, due to an effective aperiodic potentialproduced by the inner shell, and treated perturbatively.General helicity-dependent selection rules were analyti-cally established, and in the case of incommensurateshells the contribution of the coupling to the inner shellwas shown to yield a diffusive regime in the outer shell,allowing for the extraction of an elastic mean free path!e. This elastic length scale was found to decrease withincreasing energy, showing a systematic strong suppres-sion at each new subband onset. For the !9,0"@ !10,10"CNT, the mean free path in the outer shell at the charge-neutrality point was found to be of the order of !e/20 "m and decreasing by one order of magnitude foreach higher subband.

The occurrence of a diffusive regime and intrinsicelastic mean free path due to intershell multiple-scattering phenomena was also confirmed by numericalcalculations on double-walled !9,0"@ !10,10" and triple-walled !6,4"@ !17,0"@ !15,15" nanotubes !Wang et al.,2006". This novel fundamental elastic length scale !!e",which results from the intrinsic aperiodicity of objectswith a high degree of crystallinity, is unprecedented inmesoscopic physics.

Experiments on boron-doped MWNTs have reportedon the anomalous scaling of the conductance !Krstic et

al., 2003". However, the obtained exponent =/1/2,pointing toward a diffusive regime, could not be unam-biguously attributed to multishell conduction, owing tothe superimposed contribution of chemical disorder.Some estimation of the intershell resistance of/10 k5 "m was performed !Bourlon et al., 2004", andalthough its value was found to be very small, this evi-dences the contribution of multishell conduction in realexperiments. Finally, it has been recently possible tofully characterize the chiral indices of individual shells ofdouble-walled nanotubes by means of electron diffrac-tion !Hirahara et al., 2006". This geometrical determina-tion of shell helicities in conjunction with transport mea-surements !Kociak et al., 2002" opens novel perspectivesfor an in-depth exploration of conductance scaling prop-erties in these objects.

c. Crossed carbon nanotubes junctions, bending and twistingdeformations

Crossed nanotube junctions result from interacting in-dividual SWNT shells, which are either present inbundles, on ropes of compacted nanotubes or intention-ally manufactured for a given application purpose. Incrossed-tube junctions, the intertube distance can to acertain extent be controlled by applying pressure, forinstance, by means of an atomic force microscope!AFM" tip. As a result, a change in the overlap ofneighboring-shell wave functions is induced by struc-tural deformations. This was analyzed by Yoon and co-workers !Yoon et al., 2001", who performed first-principles calculations of armchair-based crossed-tubejunctions, and found that the intertube conductancefluctuations was on the order of %!0.1–0.2"G0 depend-ing on the applied contact force, roughly a few to about15 pN !Fig. 45".

On the other hand, the effect of structural distortionson the electronic and transport properties has also beeninvestigated. Electronic band structure calculationsshowed that progressive bending of CNTs results in adecrease of the transmission coefficient in certain energyranges 'Fig. 46!a"(, where curvature-induced '-# hybrid-ization effects produce localized states and strongly en-hanced backscattering !Rochefort et al., 1999; Lammertet al., 2000". Similarly twisting operations were alsoshown to produce band-gap openings in otherwise gap-less metallic armchair nanotubes, with particular band-gap oscillations depending on the twisting angle 'Fig.46!b"(.

D. Quantum interference effects

1. Weak localization and the Aharonov-Bohm effect

Weak localization is a quantum interference phenom-enon that develops beyond the length scale of the elasticmean free path, provided the wave function maintainsits phase coherence !Altshuler et al., 1981". From quan-tum mechanics, the quantum transmission between twochosen points in real space, let us say P and Q, generallyreads

FIG. 44. Time-dependent diffusion coefficient for incommen-surate and commensurate disorder-free MWNTs !with E=.0 /8". Right: Length dependence of conductance for twoFermi energies for !6,4"@!17,0"@!15,15". Adapted from Trio-zon et al., 2004.

711Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

G =2e2

hPP→Q, !51"

where P, which is the probability for an electronic wavepacket to go from one site P to another Q, can be fur-ther expanded as

PP→Q = )i

#Ai#2 + )i#j

AiAjei!/i−/j", !52"

defining Aiei/i as the probability amplitude to go from Pto Q via the i path. In order to extract the main univer-sal transport features of a given disordered system, anaverage over a statistical distribution of random configu-rations has to be performed. In this averaging process,most of the interference terms in the second summationwill vanish. However, two scattering events !paths" topo-logically returning back to the origin !clockwise andcounterclockwise" will yield a constructive contributionof quantum interferences, thus reducing the absoluteconductance compared to its classical value. For thesepaths with topological symmetry, the probability of re-turn to the origin is written as

PO→O = #A+ei/+ + A−e+i/−#2 = 4#A0#2, !53"

which thus enhances the classical value by a factor of 2.To compute the total quantum correction !+GWL" due toweak-localization effects, one has to integrate over thewhole class of such paths, so that

+GWL /2e2D

h 00

B

PO→O!t"!e−t/-* − e−t/-e" . !54"

The quantum correction is thus phenomenologicallygiven by the integrated probability of return to the ori-gin between the elastic scattering time -e and coherencetime -*. The coherence time is the time scale that limitsthe contribution of quantum interference effects. Itoriginates from the intrinsic decoherence mechanismsbetween clockwise and counterclockwise paths, whichare driven by the coupling of the quantum phase to atime-dependent fluctuating potential mimicking either afluctuating electromagnetic field or a phonon bath!Chakravarty and Schmid, 1986". Applying a magneticfield is a powerful tool for unveiling these quantum in-terference effects. Indeed, switching on a magnetic fieldbreaks the time-reversal symmetry between these paths,resulting in an increase of conductance or decrease ofresistance !negative magnetoresistance". Anothermagnetic-field-induced quantum interference effect in aring or cylinder geometry is the modulation of resistancewith period *0 /2. The phase factor can then be writtenas !A is the vector potential"

/± = ±e1c 9 A · dr = ±

2#*09 A · dr , !55"

and so the amplitude is given by #A#2#1+ei!/+−/−"#2, result-ing in a modulation factor cos!2#* /*0". This phenom-enon was first reported in carbon nanotubes by Bachtoldand co-workers !Bachtold et al., 1999".

a. Application to metallic (armchair) carbon nanotubes

Here the weak-localization phenomena in metalliccarbon nanotubes are illustrated, on the basis of numeri-cal results !Roche et al., 2001a". The behavior of thefield-dependent diffusion coefficient D!-* ,* /*0" isshown in Fig. 47 for the !9,0" nanotube as a function of

FIG. 45. Calculated intratube and intertube conductances as afunction of the contact force for a !5,5" crossed junction. Solid!dashed" lines and left !right" y axis indicate intertube !in-tratube" conductances. Top: Structural relaxation of the !5,5"crossed CNT junction with a 15-nN contact force. Adaptedfrom Yoon et al., 2001.

FIG. 46. Transmission coefficient as a function of Fermi levelfor isolated bent !6,6" nanotubes with increasing bending angle!left" or for twisted models of distortions !right". Upper draw-ings show the corresponding nanotube structures. Adaptedfrom Rochefort et al., 1999.

712 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

!e using Eq. !49". By using Anderson-type disorder, thevalue of !e can be tuned by the disorder strength W andseveral situations of interest can be explored.

First, the weak-localization regime !Altshuler et al.,1981" is analyzed under the condition !e7 #Ch#7L!-*".Figure 47 shows that the diffusivity increases at lowfields !negative magnetoresistance" and that the periodicAharonov-Bohm oscillations are dominated by a *0 /2period, i.e., D!-* ,*+*0 /2"=D!-* ,*" in agreement withweak-localization theory. In contrast, when !e) #Ch#,L!-*72!e", the system exhibits a positive magnetoresis-tance associated with D!-* ,*+*0"=D!-* ,*". For thecase !e) #Ch#, L!-*)2!e", negative magnetoresistanceand Aharonov-Bohm oscillations with period *0 are ob-tained. Note that, with the analytical formula for themean free path and estimates of disorder values, onegets !e%104#Ch#, where #Ch# is the circumference of theouter nanotube in the experiment of Bachtold and co-workers !Bachtold et al., 1999". This leads to some in-consistency since the theoretical value of the mean freepath is a priori too large to be consistent with a *0 /2Aharonov-Bohm oscillation. In that respect, an impor-tant observation is that the magnetic field amplitudeneeded to observe conventional weak localization alsostrongly modifies the band structure, with a *0-periodicoscillation of 1D band positions as discussed in Sec.III.E.2. Although the band-gap opening and oscillations,as well as other band structure changes !Van Hove sin-gularity splitting and shifting", are likely to be smoothedby disorder, the magnetofingerprints will obviously re-sult from an entangled situation, which goes much be-yond the conventional theory of weak localization !Alt-shuler et al., 1981". Several early experiments suggestedsuch additional complexity in analyzing magnetotrans-port measurements !Fujiwara et al., 1999; Fedorov et al.,2005". Roche and Saito !2001" theoretically found that,

for a fixed disorder strength, magnetotransport finger-prints present strong fluctuations as a function of Fermilevel position, CNT diameter, and orientation of themagnetic field with respect to the tube axis. Thanks tothe engineering of efficient electrostatic gating of thenanotube, some experimental evidence of such multipleAharonov-Bohm effects, with a *0 /2 oscillation drivenby weak localization superimposed on to *0-periodic re-sistance fluctuations related to band structure modula-tions, have been reported !Stojetz et al., 2006".

The issue of the weak-localization regime in chemi-cally disordered carbon nanotubes has been investigatedrecently for the case of boron !Latil et al., 2005" andnitrogen doping !Avriller et al., 2006". For an axial mag-netic field, the interplay between field-dependent bandstructures and quantum interference effects was shownto induce strong electron-hole asymmetry of the magne-toresistance patterns. For a given chemical impurity con-centration and at a finite magnetic flux threading theinitially metallic nanotube, the contribution of boron-induced quasibound states was found to induce stronglocalization effects for hole transport; in contrast, elec-tron transport remains weakly affected by disorder, withquasiballistic conduction !Latil et al., 2005". In the caseof a magnetic field applied perpendicular to the nano-tube axis, an upward shift in energy of the nitrogen-induced quasibound states was found to be driven by thefield intensity, with large magnetoresistance fluctuationsresulting under small Fermi level shifts !Avriller et al.,2006".

Finally, some spectacular energy-dependent behaviorof the coherence length and elastic mean free path couldalso be measured !Stojetz et al., 2005". The obtained en-ergy dependence of !e was in full agreement with theo-retical results !Triozon et al., 2004". Roche and co-workers !Roche et al., 2005a" further studied the energydependence of the coherence length by computing thetotal Kubo conductance in nanotubes in the presence ofboth static disorder !Anderson type" and a time-dependent fluctuating potential !resulting from phononinduced atomic displacement field". By evaluating boththe full Kubo conductance and its classical value, thequantum correction could be deduced,

+GWL!E" = 2e2

hN!!e!E"L!E,t"

− G!E" , !56"

and the energy dependence of L*!E" in the weak-localization regime could be extrapolated on the basisof the conventional phenomenology, i.e., L*!E"=+GWL!E" /L!E , t" and -*!E"=L*

2 !E" / 'v!E"!e!E"(,where L!E , t" corresponds to the relevant length scaleentering in the Kubo normalization factor. In Fig. 48,various contributions to the conductance are shown fortwo selected values of static disorder and acoustic pho-non modulation !twist mode". L*!E" and -*!E" are seento decrease at each onset of new subbands, in agreementwith experiments !Stojetz et al., 2005". Further, for afixed energy L*!E" downscales with increasing static dis-order potential. For Anderson-type on-site disorder, one

FIG. 47. Diffusion coefficient D!-* ,* /*0" !in units of Å2.0 /1"for the !9,0" nanotube evaluated at time -*<-e for two disor-der strengths W /.0=3 and 1 such that the mean free path !!e/0.5 and 3 nm, respectively" is either shorter !dashed line" orlonger !solid line" than the nanotube circumference !#Ch#/2.3 nm". The right y axis is for the dashed line, and the left yaxis is for the solid line. Inset: D!-* ,* /*0" for !e=3 nm andL!-*"72!e.

713Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

gets L*!W=0.1.0"/75–400 nm, whereas L*!W=0.2.0"/50–200 nm and L*!W=0.5.0"/20–50 nm.

In the case of multiwalled carbon nanotubes, the situ-ation becomes even more complicated. First, each shellhas a different diameter, with a difference of /3 Å be-tween neighboring shells. So for a given *0 flux thread-ing one given shell, neighboring shells will be sensitiveto either Larger or smaller flux, leading to multiple con-tributions of incommensurate Aharonov-Bohm oscilla-tion periods. In addition, even if the MWNTs are freefrom any other source of contamination, the incommen-surability between neighboring shells produces an un-derlying aperiodic potential for #-electron motion, asexplained in Sec. IV.C.5. This phenomenon was shownto be at the origin of various energy-dependent magne-totransport fingerprints, such as *0-periodic magnetore-sistance oscillations at certain energies, that will trans-form into *0 /2 oscillations for a shifted Fermi levelposition !Roche et al., 2001a; Triozon et al., 2004".

2. From weak to strong localization

In low-dimensional systems, the relation between themean free path and the localization length is an impor-tant issue. Thouless !1973" derived the simple relationA=2!e between the two quantities in strictly 1D systems.By means of random matrix theory !Beenakker, 1997"this result was generalized for quasi-1D systems with alarge number of conduction channels A/N!!e. Fortransport regimes that are said to be ergodic, the aver-age properties do not depend on the precise nature ofthe underlying disorder, but are predicted to be drivenby the universal symmetry class of the Hamiltonian; thatis, A= 1

2 7E!N!−1"+28!e, with E=1 if the Hamiltonian issymmetric under the time-reversal operator and E=2otherwise.

In metallic carbon nanotubes at the charge-neutralitypoint, assuming uniform Anderson-type disorder !withstrength W", the localization length is thus expected,at zero field, to be given by A!E=0"= !36acc.0

2 /W2"$n2+m2+nm, and will consequently alsoscale linearly with the tube diameter for low disorder!Roche et al., 2000; Hjort and Stafström, 2001; Jiang etal., 2001". Its experimental observation assumes that anexponential increase of the resistance develops from acertain nanotube length L, i.e., G%!2e2 /h"exp!−L /A",and the localization length A!E" is predicted to be energydependent, with a systematic decrease at each onset ofnew subbands, following the mean-free-path pattern.

Some evidence of Anderson localization has been ob-tained experimentally !Shea et al., 2000; Gómez-Navarroet al., 2005". First, Shea and co-workers studied low-temperature magnetotransport in a ring of a rope ofSWNTs. Although a weak-localization signature was ob-served for T>3 K, a drastic resistance increase wasmeasured below 1 K, with strong departure of magne-toresistance behavior from weak-localization theory. Noclear understanding of the origin of localization or itsintrinsic features could be achieved. More recently,Gómez-Navarro and co-workers !Gómez-Navarro et al.,2005" reported an exponential increase of the resistancein Ar+-irradiated carbon nanotubes. By tuning the ionirradiation time exposure to enhance the defect density!assigned to bivacancies", the resulting resistance in-crease was analyzed in terms of decreasing localizationlength. These measurements were supported by ab initiocalculations !Biel et al., 2005", giving the first direct evi-dence of a metal-insulator transition in quasi-1D sys-tems.

Other recent work has further theoretically investi-gated simultaneously both the elastic mean free pathand the localization length !Avriller et al., 2006" for arealistic model of chemical disorder !substitutional ni-trogen impurities". The Thouless relationship betweenthe two was confirmed in the absence and presence of anexternal magnetic field !Thouless, 1977" and in agree-ment with the theoretical predictions of random matrixtheory !Beenakker, 1997".

E. Inelastic scattering

1. Electron-phonon coupling

Discussion of the vibrational properties of nanotubeswould require a full review that is beyond the scope ofthe present work. However, some aspects of the elec-tronic and transport properties of nanotubes cannot beunderstood without treating the coupling of electronswith phonons. Such aspects include !nonexhaustively"the charge density wave or superconducting instabilityof the Fermi sea !Sec. IV.F", the inelastic scattering ofelectrons by phonons in a transport experiment !Sec.IV.E.2", the Raman intensities, and the relaxation of hotelectrons in an optical experiment. Thorough reviews orpapers on the phonon properties in CNTs can be foundin the literature !Sánchez-Portal et al., 1999; Dresselhaus

FIG. 48. Quantum conductance and coherence length in disor-dered nanotubes. Top: Computed Kubo conductance for aweakly disordered !10,10" nanotube for two time scales 't= !3500,35 000"1 /.0(, together with the classical value and thededuced quantum correction. Bottom: Coherence lengthL*!E" for two values of static disorder and acoustic phononmodulation !twist mode". Adapted from Roche et al., 2005b.

714 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

and Eklund, 2000; Dubay and Kresse, 2003". A review ofthe role of electrons and phonons in CNT Raman spec-tra can be found in Dresselhaus et al. !2005".

As an introductory remark to electron-phonon cou-pling !EPC", we note that conservation of energy andmomentum imposes that only zone-center and zone-boundary phonons with momentum q=K can couplewith electrons in the case of metallic CNTs !in this sec-tion, q will label the phonon momentum". This stemsfrom the fact that phonon energies are much smallerthan the electronic Fermi energy. Therefore, rather fewphonon modes will be able to scatter electrons from oneband to another. Further, depending on the relative signsof the Fermi velocity for the initial and final electronicstates, the electron-phonon scattering processes are clas-sified as “forward” or “backward,” a notion that is cru-cial in transport theories. The different electron-phononscattering processes !here a phonon emission" are sum-marized in Fig. 49.

We first start with a discussion of the EPC in thegraphene sheet and reproduce in Fig. 50 the opticalmode branches combining accurate experimental and abinitio calculations !Maultzsch et al., 2005". At the zonecenter, the important modes for the EPC are the twofoldEg

2 high-energy in-plane modes which split away from (in a longitudinal and a transverse branch. At the zoneboundary, the q=K A1! mode strongly couples to elec-trons. A clear manifestation of the EPC can already be

found in the phonon band structures where a frequencysoftening can be observed. In the case of graphene, thepeculiar shape of the graphene BZ induces a significantphonon softening of the Eg

2 and K-A1! modes, related toa Kohn anomaly, which manifests itself by a linear dis-persion of the Eg

2 longitudinal and A1! modes away from( and K, respectively !Piscanec et al., 2004".

In the D2nh symmetry group of the achiral !n ,n" or!n ,0" tubes !Damnjanovic et al., 1999; Reich et al., 2004",the graphene (-Eg

2 degenerate mode splits into (-A1longitudinal !L" and transverse !T" polarization modes!labeled as well ILO or ITO for in-plane L or T opticalmodes". The (-A1 modes EPC coupling in tubes was firstshown to rationalize the redshift with decreasing radiusof the Raman G band !Dubay et al., 2002". In particular,the different evolution of the A1!L" mode for metallicand semiconducting zigzag tubes clearly pointed to anelectronic contribution to the frequency softening. Aclear illustration of the coupling is obtained by observ-ing the evolution of the band structure upon distortionof the atomic network along the phonon eigenmodeswith some amplitude +dq; !q and ; are the phonon mo-mentum and band index". As shown in Fig. 51, the A1!L"phonon opens a gap at the Fermi level of metallic zigzagtubes, thus strongly affecting the electronic properties.As a matter of fact, the deformation potential Dnk

q; !ineV/Å", which is a measure of the shift +6nk of the bandedges divided by +dq;, can be related to the intrabandEPC matrix elements ,Fnk#+Vq;#Fnk-, with +Vq; thechange upon lattice distortion of the potential seen byelectrons !Khan and Allen, 1984" in the case of totallysymmetric phonons.

The optical mode deformation potentials for !6,6" and!11,11" tubes have been determined with ab initio calcu-lations by Lazzeri et al. !2005". They were compared, inparticular, to the values obtained from a band-foldinganalysis of graphene (-Eg

2 and K-A1! deformation poten-tials !D=6.7 and 10.0 eV/Å, respectively", showing a/20% difference for the smaller tube !/8 Å diameter"as a manifestation of curvature effects. Similar valueswere obtained on the basis of a tight-binding approachfor a !10,10" tube !Jiang et al., 2005". However, thestrong dependence of the deformation potential on theparametrization of the distance derivative of the hop-ping integral leads to rather scattered values !Mahan,

FIG. 49. Electron-phonon scattering processes. !a" Symbolicscattering processes !phonon emission": (bs and (fs are zone-center !intravalley" backward and forward scattering, while Kbsand Kfs are zone-boundary !intervalley" backward and forwardprocesses. !b" Symbolic phonon emission process with the en-ergy and momentum of the initial and final electron and pho-non states.

FIG. 50. !Color online" Inelastic x-ray scattering and ab initiocalculations !open circles" of the phonon dispersion in graph-ite. Adapted from Maultzsch et al., 2005.

FIG. 51. Band gap opening by optical phonons. !a" Displace-ment pattern of the longitudinal !transverse" A1 mode in azigzag !armchair" tube. Band structure for a metallic zigzagtube in !b" the equilibrium positions and !c" for the distortioncompatible with the A1!L" mode. Adapted from Dubay et al.,2002.

715Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

2003; Park et al., 2004; Jiang et al., 2005; Perebeinos etal., 2005; Popov and Lambin, 2006b".

The differences between graphene and tubes can beseen more clearly in the case of acoustic modes. Themost documented example is that of the out-of-planeacoustic mode of graphene which becomes the radialbreathing mode !RBM" in nanotubes. Since a change inthe tube radius involves bond stretching and wagging,the RBM displays a nonzero frequency with a 1/R ra-dius dependence exploited to calibrate tubes in Ramanexperiments !Rao et al., 1997; Jorio et al., 2001; Machónet al., 2005; Meyer et al., 2005; Popov and Lambin,2006a". Further, evolution of the deformation potentialand related EPC matrix elements was shown on the ba-sis of ab initio calculations to strongly depend on thetube radius and helicity !Machón, 2005". In addition tothe RBM, the acoustic in-plane transverse mode of thegraphene sheet becomes the so-called twiston mode intubes, which has been suggested to lead to a significantEPC coupling on the basis of tight-binding !Jishi et al.,1993; Hertel and Moos, 2000; Mahan, 2003; Jiang et al.,2005" or continuous elastic theories !Suzuura and Ando,2002; De Martino and Egger, 2003".

An interesting issue is to distinguish the influence ofconfinement and curvature !namely, '-# rehybridiza-tion" on the evolution with the diameter of the phononfrequency and EPC strength. In an early work !Bene-dict, Crespi, Louie, and Cohen, 1995", quite general sym-metry arguments were developed to show that curvaturewould lead to a 1/R increase of the EPC matrix ele-ments with decreasing radius R. This stems from theevolution from pp# to pp' bonding upon increasing cur-vature, an effect that can be connected to the very largedeformation potential at the origin of the superconduct-ing transition in all-sp3 !or '-bonded" doped diamond!Blase et al., 2004" and clathrates !Connétable et al.,2003". In particular, modes such as the zone-center out-of-plane optical !ZO" and acoustic modes do not couplein the graphene sheet but show nonzero coupling in thecase of tubes. Further, electronic and vibrational eigen-state normalization leads to a 1/$R dependence ofthe EPC matrix elements !Benedict, Crespi, Louie, andCohen, 1995". This dependence will mainly affect modesthat are already large in the planar graphene sheet !(-Eg

2

and K-A1!".A quite general analysis of the evolution of the EPC

matrix elements with radius, chiral angle, and tube type!metallic types I and II or semiconducting" has been de-veloped on the basis of tight-binding analysis, allowing

for analytic formulas at high-symmetry points !Mahan,2003; Jiang et al., 2005; Popov and Lambin, 2006b". Suchmatrix elements were used to compare the experimentaland calculated PL and resonant Raman scattering inten-sities !Jorio et al., 2006". The importance of accuratelyevaluating EPC matrix elements has also been empha-sized recently in attempting to identify the origin andnature of the so-called high-energy G+ and G− bands!Lazzeri et al., 2006; Popov and Lambin, 2006a". Such anidentification is closely related to the above-mentionedKohn anomaly, leading to significant mode softening inthe limit of small radii.

2. Inelastic transport length scales

We now extend our discussion of the electron-phononcoupling to its influence on transport in the normal state!in contrast to the superconducting phase treated in Sec.IV.F". Electronic transport is sensitive to inelastic effectsstemming from either e-ph or e-e scattering. An investi-gation of the temperature dependence of conductanceprovides a wealth of information about decoherencemechanisms and inelastic scattering rates. Low-biasmeasurements show that G// /T !Yao et al., 2000", ascaling law that has been related to e-ph scatteringdriven by low-energy vibrational modes. By using a phe-nomenological relationship between the conductanceand the scattering rate,

G /2e2

h!ie

Ltube, !57"

a typical scattering length !ie/1–2 "m !300 K" was in-ferred and attributed to e-ph coupling involving acousticmodes. On the other hand, the inelastic scattering ratescan be theoretically computed by means of the FGRderived from either a first-principles !Lazzeri et al., 2005"or a semiempirical approach !Jiang et al., 2005". TheFGR consists here in calculating the scattering rate be-tween eigenstates of the zero-phonon Hamiltonian. Thisassumes that the phonon and electronic populations areat equilibrium and can be treated independently, thee-ph coupling being assumed to remain of a perturbativenature. In that framework, the inelastic scattering lengthassociated with a given phonon mode is readily deducedfrom !ie=v-ie, with v the relevant average velocity of thecharge carrier energy. Three important phonon modesyield contributions to inelastic backscattering. As de-picted in Fig. 52, the first process is driven by acousticphonons with low energy and small momentum. Within

FIG. 52. Schematic representa-tion of the main phonon contri-butions to backscattering!acoustic, optical, and zone-boundary modes".

716 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

the FGR, the scattering rate !with phonon emission"-e-ph

−1 !q" is written as

2#51

)k

2,k + q,nq + 1#(e-ph#k,nq-22+!6k−q − 6k − 1@q"

$!1 + nq"'1 − f!6k−q"(f!6k" , !58"

with 5 the surface of the tube and (e-ph the electron-phonon scattering operator, while nq and f!6k" give thephonon and electron distributions, respectively. In me-tallic tubes, the acoustic torsional mode !twisting modeor twiston" is a purely circumference-directional defor-mation, while its velocity is equal to a transverse acous-tic mode of the graphene sheet '@!q"=vtwist#q#(. A crudeestimation due to inelastic scattering gives -e-ph

−1

/!4# /1"D2!kBT /24Mvtwist2 " /hvF, with 4M the mass den-

sity and D the deformation potential !Park et al., 2004".It has to be noted that, unlike in ordinary metals, thelinear temperature dependence of the electronic resistiv-ity persists well below the Debye temperature, essen-tially because these phonon modes are heavily thermallypopulated !Kane et al., 1998". With reasonable param-eters, the inelastic acoustic scattering time is found to be%3$10−12 s, with a subsequent inelastic mean free path!e-ph=vF-e-ph%2.4 "m for a 1.8-nm nanotube !Yang andHan, 2000; Park et al., 2004". A theoretical derivationhas also predicted some helical-dependent contributionto electron-phonon backscattering and the resistancevalue in the high-temperature regime !Suzuura andAndo, 2002".

In the high-bias regime, experiments have reported ona Gtube/E /V scaling law, a behavior attributed to anelectronic coupling to zone-center optical as well aszone-boundary phonon modes. By using the same phe-nomenological relationship G/!2e2 /h"!ie /Ltube, Parkand co-workers !Park et al., 2004" experimentally esti-mated the inelastic mean free paths !ie in the high-biasregime. For bias voltage of the order of 1 V, !ie/10 nm was assigned to a contribution to both opticaland zone-boundary modes. Within the framework of theeffective mass formula and deformation potential ap-proximation, the theoretical electron–acoustic-phononscattering length was estimated to be %2.4 "m in thelow-bias regime, while optical and zone-boundarymodes were associated with !ie of the order of 180 and37 nm, respectively. By applying Matthiessen’s rule, thetotal inelastic length at high bias was deduced to be ofthe order of 30 nm.

In a different approach, Javey and co-workers !Javeyet al., 2004" used a CNT-FET experiment, and by fittingwith semiclassical Monte Carlo models, they estimate!ie=300 nm for acoustic modes and !ie=15 nm for opti-cal modes.

Thus, the reported values for inelastic mean free pathsstrongly fluctuate within the range '10 nm, 200 nm( forthe case of electron–!optical-"phonon coupling. Further,a comparison of experimental values with FGR calcula-tions from first principles leads to a disagreement ofabout one order of magnitude !Lazzeri et al., 2005".

Perebeinos, Tersoff, and Avouris !2005" recently pro-posed to investigate the effect of inelastic scatteringon the conductance by following the semiclassicalBloch-Boltzmann treatment of transport theory. The au-thors derive a phenomenological law for the zero-fieldcharge-carrier mobility "!T ,dtube"= "'!300 K" /T('dtube/!1 nm"(/, exhibiting some specific temperature and di-ameter dependences !here "=12 000 cm2/V s and //2.25".

In contrast, other theoretical works have investigatedthe influence of structural lattice fluctuations on theelectronic band structure !Dubay et al., 2002" and trans-port !Georghe et al., 2005; Roche et al., 2005b". The su-perimposed contribution of optical phonon vibrationshas yielded time-dependent band structure changeswhich affect the conductance scaling features !Roche etal., 2005b". A more general quantum treatment of in-elastic transport in metallic nanotubes, going beyond thelinear response and within a true many-body approach,has revealed the occurrence of a Peierls-like mechanismassociated with the longitudinal optical mode activation!Foa-Torres and Roche, 2006". These recent results high-light effects which are beyond the scope of semiclassicaltransport theories. Their impact on the simulation ofcarbon-nanotube–based field-effect transistors remainsan open issue.

3. Electron-electron scattering and Luttinger-liquid models

The contribution of e-e interactions can be envisionedfrom two perspectives. In the first case, high dimension-ality and screening effects are sufficient to warrant thatCoulomb interactions can be treated perturbatively,while charge transport remains well described within theFermi-liquid picture. The stability of the Fermi liquid isactually well established for 3D systems, owing to thefact that the Pauli exclusion principle strongly quenchesthe electron-electron interaction !Nozières and Pines,1999". At zero temperature, the discontinuity of theFermi-Dirac distribution at EF, combined with the con-servation of energy and momentum, causes the numberof final !empty" available states to which an electron ofenergy E&EF can be scattered to go quadratically tozero as a function of E−EF. This is the famous resultthat the lifetime -e-e of an electron, with respect toelectron-electron interactions, scales as 1/ !E−EF"2 closeto the Fermi level.

Such a Fermi-liquid description has been extensivelyemployed for describing quantum transport in MWNTswith large diameters, given the reported strong evidenceof weak localization !Bachtold et al., 1999; Stojetz et al.,2005". At low temperatures, the e-e interaction then actsas a source of decoherence in the weak-localization re-gime, limiting the contribution of quantum interferenceand localization effects. Similarly, screening by a metallicsubstrate, or a surrounding gate, seems to be at the ori-gin of good agreement between the measured STM den-sity of states in small-diameter SWNTs and tight-bindingcalculations performed assuming noninteracting states!see Sec. III.D". At higher temperature, e-e scattering

717Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

can drive the temperature dependence of transport co-efficients. For instance, Balents and Fisher !1997" dem-onstrated that umklapp scattering due to e-e interactionsyields a resistance linear in temperature. Within this re-gime, the transport physics is still generally well de-scribed within the standard Fermi-liquid single-particlepicture, where by starting from extended wave functionswith wave vector k the interactions appear as scatteringprocesses between states with different k values, the rel-evant events being forward and backward scatteringwith energies close to the Fermi surface.

On the other hand, carbon nanotubes also providenew opportunities to search for strong deviations fromthe Fermi-liquid theory, since, especially in the case ofsmall-diameter SWNTs, their low dimensionality consid-erably enhances the strength of repulsive Coulomb in-teractions. As a matter of fact, independent of the rangeand strength of the interaction between electrons, it canbe shown that scattering of a single charge carrier in-duces a “collective” response of the 1D electron gas.From that standpoint, the concept of single-particle scat-tering seems useless and one should adopt a descriptionwhere all electrons are collectively modified by an exter-nal pump or probe. Collective electronic excitations canbe described in terms of the well-known charge and spinwaves !plasmons and spinons". This point can be illus-trated by observing that, sufficiently close to the Fermilevel, an electronic band can always be linearizedaround kF: E!k"=vF!k−kF", with vF the Fermi velocity'Fig. 53!a"(. The excitation energy associated with an in-traband scattering can then be linearly related to thevariation of momentum through dE=vFdk. Clearly, con-servation of momentum and energy is preserved if onereplaces the !dk ,dE" single excitation by n !dk /p ,dE /p"processes involving p electrons. Namely, there is a mo-mentum and energy resonance between single-electron

scatterings and excitations involving an arbitrarily largenumber of particles. One says that single-particle excita-tions decay into collective plasmon modes 'Fig. 53!c"(.

To describe the charge and spin collective excitationsin 1D systems in the presence of a strong Coulomb in-teraction, a heuristic approach is used based on theWannier representation. In the Wannier picture, themany-electron Hamiltonian, represented in terms ofwave functions localized around the site m=1,2 ,3 , . . . ,N of the lattice, is a Hubbard type where thedominant interaction is between electrons at the samesite. The !bare" Coulomb interaction is, however, oflong-range nature, so the simple Hubbard model willrepresent only physical situations for which e-e interac-tions are strongly screened. By considering an extendedversion of the on-site Hubbard model !retaining e-e in-teractions between nearest neighbors", one can enlargethe range of the Coulomb potential to nearest-neighborsites. The Wannier version of the Hamiltonian is thenwritten as !Baeriswyl and Degiorgi, 1990"

H = H0 + Hint = − .0)m'

!cm'† cm+1' + cm+1'

† cm'"

+ U0)m

nm↑nm↓ + V0)m

nmnm+1, !59"

where cm'† !cm'" creates !annihilates" an electron at site

m with spin projection '= ↑ ,↓, nm'=cm'† cm', and nm

=nm↑+nm↓. For a half-filled band !one electron per site",the U0 term favors an alternating charge density. If onenow imposes periodic boundary conditions, i.e., cN+1'=c1', the Bloch representation can be introducedthrough the canonical transformation cm'

= !1/$N")keikmck', with k=2#; /N and −N /2&;&N /2,i.e., k can be chosen to lie in the first Brillouin zone−#&k&#. This transformation diagonalizes the firstterm of the Hamiltonian as H0=)k6kck'

† ck' !kinetic en-ergy", with 6k=−2.0 cos k. If one is restricted to the lin-ear part of the spectrum and defines ,+,k'=ckF+k,' and,−,k'=c−kF+k,', which is just a gauge transformation, weobtain

H0 = )k'1vFk!,+,k'

† ,+,k' − ,−,k'† ,−,k'" , !60"

the ,+,k' and ,−,k' operators representing the right-and left-moving states with wave vectors +kF and −kF,respectively. These states were introduced by Luttinger!1963". Rewriting Hint in terms of these new operatorsone gets

Hint =1N )

k1,k2,k3,k4,','!

+k1+k2,k3+k4*g1,+,k1'† ,−,k2'!

† ,+,k3'!,−,k4'+ g2,+,k1'

† ,−,k2'!† ,−,k3'!,+,k4'

+g3

2!,+,k1'

† ,+,k2'!† ,−,k3'!,−,k4'

+ H.c." +g4

2!,+,k1'

† ,+,k2'!† ,+,k3'!,+,k4'

+ ,−,k1'† ,−,k2'!

† ,−,k3'!,−,k4'"+ , !61"

FIG. 53. Elementary excitations in 1D systems. !a" Symbolicrepresentations of a linear band around kF. The decay of asingle-electron excitation into n=3 subprocesses is repre-sented. !b", !c" Single-particle and plasmon !energy, momen-tum" diagrams in 3D and 1D systems. Note that long-wavelength single-particle excitation and plasmon @pl energiesare decoupled in 3D but resonant in 1D.

718 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

where terms that can be incorporated within the chemi-cal potential have been neglected. The coupling con-stants gi are related to the Hubbard parameters as fol-lows: g1=g3=U0−2V0 and g2=g4=U0+2V0. Allscattering processes in Hint can be pictorially repre-sented by Feynman diagrams. The first process g1 corre-sponds to backward scattering, while the process g2 is aforward-scattering event, and g3 arises as an umklappprocess, which becomes irrelevant far from half-filling.Finally g4 leads to a small renormalization of the Fermivelocity, which is usually neglected. The whole Hamil-tonian H0+Hint defines the one-dimensional Fermi gasmodel !Solyom, 1979". A simple solvable case of theone-dimensional Fermi gas model is the Tomonaga-Luttinger model !Tomonaga, 1950; Luttinger, 1963",where only forward scattering !g2" is taken into account!g1=g3=g4=0". It has been solved by Mattis and Lieb!1965", who showed that this model describes a particu-lar type of system where the conventional Fermi surface,defined in terms of a step in the momentum distribution,does not exist for arbitrarily small g2=g. Haldane !1981"later extended their analysis to a more general situationand coined the term “Luttinger liquid” !LL" in analogywith the Fermi liquid. If for simplicity one is restricted tothe the case of spinless fermions, the LL Hamiltonian iswritten

H = H0 + Hint = )k'1vFk!,+,k'

† ,+,k' − ,−,k'† ,−,k'"

+1N)

qg!q"41!q"42!q" , !62"

with 41!q"=)k,+,k† ,+,k+q while 42!q"=)k,−,k

† ,−,k+q. Inthe ground state of H0, all negative-energy states areoccupied, while all positive-energy states remain empty.The density operators 4i!q" act like Bose creation andannihilation operators of elementary excitations withenergy 1vF#q# and momentum q !the so-called bosoniza-tion scheme". Several important quantities can be ex-actly calculated for the LL model, including the momen-tum distribution function !Mattis and Lieb, 1965" andvarious response functions !Solyom, 1979", which gener-ally exhibit power-law behavior !Voit, 1995; Giamarchi,2004".

Despite the early predictions of the LL transition, thedifficulty in performing low-temperature experiments onisolated 1D systems explains why experimental confir-mation of LL behavior has remained scarce. In that re-spect, synthesis of CNTs has provided a unique play-ground to test the theoretical concepts. A formaldescription of the LL in armchair metallic SWNTs wasproposed !Egger and Gogolin, 1997, 1998; Kane et al.,1997". In regard to the strict single-channel case, carbonnanotubes display more complex quasi-1D characteris-tics, which are required to reconsider !and extend" thebasics of LL theory. First, the Fermi surface is describedby four kF points of the Brillouin zone, instead of thetwo kF points found for a single channel. In addition,depending on the CNT diameter and chirality, the den-

sity of states varies for small Fermi level shifts, whichcomplicates the extension of analytical results obtainedfor a 1D channel with constant DOS. In particular, ateach onset of new subbands, large fluctuations of theDOS !/1/$E" make the LL description technically in-appropriate !Giamarchi, 2004". Finally, in real experi-ments, the structural quality of CNTs as well as the effi-ciency of electronic contact with external voltage probesare often insulticiently high, all factors that may alsolimit the applicability range of the LL model in CNTs.

Notwithstanding, whenever the CNT/electrode inter-face is dominated by a weak tunneling contact and aslong as one is restricted to low-energy transport proper-ties, extensions of the LL model to account for addi-tional complexities such as elastic scatterers, intershelltunneling, and multichannel degeneracy have been de-veloped !Egger and Gogolin, 1997, 1998; Kane et al.,1997; Egger, 1999; Mora et al., 2006".

For the sake of illustration, we derive the main LLproperties in CNTs, restricting ourselves for simplicity tothe spinless electron case !following Mora et al., 2006".We define x as the coordinate along the CNT axis, whiler! denotes the coordinate in the perpendicular direc-tion, so that the wave functions can be expanded as fol-lows !n=1,2 for the channel degeneracy":

,± = )n=1

2

e±knx*n!r!"Fn,±!x" , !63"

where *n!r!" are the transverse eigenmodes normalizedaccording to 3dr!*n

*!r!"*n!r!"=+mn. Explicitly, *n!r!"= #Ch#−1/2 exp!2#iny / #Ch#", with #Ch#=2#rtube, while y isan angular variable. Each one of the two channels willintersect the Fermi surface at k= ±kn, with its ownFermi momentum kn and Fermi velocity vn. The kineticpart of the Hamiltonian at low energy is rewritten as!Egger and Gogolin, 1997"

H0 = − ivF0 dx',+†!x"$x,+!x" − ,−

†!x"$x,−!x"( , !64"

with the noninteracting DOS given by ;=2/#vF. Theexact repulsive Coulomb interaction UCoulomb amongelectrons can be described by the extended Hubbard-Wannier model as previously described. RecentlyLópez-Sancho and co-workers !López-Sancho et al.,2001" established, within the mean-field unrestrictedHartree-Fock approximation, a phase diagram !U0 , V0"for the spectrum modifications of metallic armchair andzigzag nanotubes. They found that a true metallic phasepersists if on-site and nearest-neighbor interaction pa-rameters are such that U0&2.0 , V&.0, whereas chargeor spin density wave phases develop for larger values,along with small gap openings.

However, from a more general perspective, the e-einteraction term should include the screened long-rangepart of the potential, which can only be estimated insome approximations. For low-energy properties, fol-lowing Mora and co-workers !Mora et al., 2006", the in-teraction is taken as long ranged on length scales larger

719Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

than #Ch#, so that the long-range tail of the interactiondominates all 1D Coulomb matrix elements, giving

Umn =0 dr!dr!! UCoulomb!x − x!,r!,r!! "

$#*n!r!"#2#*m!r!! "#2. !65"

For #x−x!#< #Ch#, UCoulomb becomes nearly independentof the transverse coordinates and the projected interac-tion is independent of the channel indices Umn=U!x−x!". By expanding the wave functions, the resulting in-teraction term for the LL !keeping only forward scatter-ing" reads

12)

+,−)

n,m=1,20 dx dx!U!x − x!",n,+

† !x",m,−† !x!"

$,m,−!x!",n,+!x" , !66"

which reduces to 12 3dx dx!4!x"U!x−x!"4!x!", indicating

that the interaction induces effective coupling between1D charge density fluctuations. In the long-wavelengthlimit, one can approximate the Fourier transform U!k"by a constant U0=U!0"−U!2kF" !which will set the inter-action strength", to end with a final expression for theinteraction term as HI= !U0 /23"3dx 42!x", with 3 the rel-evant dielectric constant. In real situations, the Coulombinteraction can be externally screened on a scale Lscr,which remains long compared to the CNT radius butshorter than the CNT length. This would occur by as-suming a surrounding cylinder of radius Lscr placedaround the tube. In this case, from elementary electro-statics, the energy to charge the nanotube with an elec-tron density e4tot will be !e2 /3"ln!Lscr /rtube"3dx 4tot

2 .For this LL model in the metallic armchair tube, a

single interaction parameter g will drive the power-lawtemperature-dependent !for eV?kBT" and voltage-dependent !for eV<kBT" tunneling conductances. Thedensity of states for an electron tunneling from the me-tallic electrode into the nanotube is 4tun!E"/E/b with anexponent /b= !g+g−1−2" /8, provided electrons tunnelfrom the metallic !Fermi-liquid" contact into the centerof the nanotube !referred to as the bulk contact". Ac-cordingly, the low-temperature conductance dI /dV=G%V/b, while the linear conductance becomes G!T"%T/b. The conductance suppression at low temperatureor bias has been shown to become even more dramaticfor tunneling into the end of a long nanotube, with anexponent that now reads /e= !g−1−1" /4 !Egger andGogolin, 1997". On the other hand, the generic form ofthe Luttinger parameter is g= !1+2U0 /2"−1/2 with U0 thecharging energy, whereas 2 is the single-particle levelspacing. If 2 is unequivocally given by 1vF /2Ltube, thecharging energy follows from the capacitive propertiesof the metal-nanotube junction and from the electronicstructure, so that no universal value can be derived. Inthe weak-screening limit, the tube length becomes thephysical cutoff of the e-e interactions, i.e., Lscr/Ltube

!Kane et al., 1997, Egger and Gogolin, 1998", which al-lows a phenomenological form of the interaction param-eter:

g = *1 +8e2

#31vFln

Ltube

rtube+−1/2

. !67"

Taking as a typical value Ltube/rtube/103, the theoreticalinteraction parameter for a metallic armchair nanotubebecomes g%0.28. Subsequently, the bulk-tunneling andend-tunneling exponents are, respectively, given by /b%0.24 and /e%0.65 !Egger and Gogolin, 1997; Kane etal., 1997". More generally, the differential conductancefor a single tunnel junction is given by a universal scalingcurve

dIdV

= AT/b,e cosh*. eV2kBT

+1(*1 + /b,e

2

+ .ieV

2#kBT+12

, !68"

which means that !dI /dV" /T/b,e is a universal function ofeV /kBT and (!x" is the Gamma function.

The non-Ohmic behavior of the conductance at lowbias voltage is often referred to as the zero-bias anomaly!ZBA" and is a clear signature of a tunneling contactbetween a Fermi liquid and a strongly correlated system.Some experiments have reported on power-law conduc-tance behaviors with exponent values in the range oftheoretical predictions either for individual single-wallednanotubes !Bockrath et al., 1999; Yao et al., 1999" or forcrossed metallic junctions of SWNTs !Gao et al., 2004",giving confidence in the manifestation of a Luttinger-liquid state in small-diameter SWNTs. Alternatively, bymeans of angle-integrated photoemission measurementsof SWNTs, some power-law behavior of the spectralfunction and intensities was also found to be in goodagreement with LL model predictions !Ishii et al., 2003".

Similarly, STM experiments on SWNTs have providedsome possible alternative signatures for the non-Fermi-liquid properties of metallic nanotubes !Lee et al., 2004".In this work, the tunneling properties of electrons froma metallic tip to a metallic tube deposited on a goldsubstrate were analyzed in terms of e-e interaction-induced charge-spin separation. The strength of theCoulomb interaction inside the nanotube was, however,found to be reduced from its expected theoretical value!Eggert, 2000", possibly due to the screening effect of theunderlying metallic substrate. This is illustrated in Fig.54, where a tight-binding calculation shows the twostanding waves with different wavelengths caused byseparate spin and charge bosonic excitations. The slopescalculated near the K points, ±8.8 and ±11.9 cm−1, cor-respond to a larger charge-mode group velocity of/vF /0.55, whereas the spin-mode velocity remains simi-lar to the Fermi velocity vF obtained for noninteractingelectrons. The deduced value for the g parameter is/0.55, much larger than the predicted value given by theunscreened Coulomb potential, g/0.3 !Kane et al.,1997". This indicates a possible screening of e-e interac-

720 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

tions, induced by the metallic substrate, which can besubstantiated by replacing Ltube by a screened length inEq. !67". A straightforward evaluation yields /1.4rtube tofit the experimental data !Lee et al., 2004".

In the case of MWNTs composed of N metallic arm-chair shells, intershell coupling has been predicted toinduce additional screening of the Coulomb interaction,screening that can be recast by renormalizing the power-law exponents by a factor of 1/N !for both cases /b /Nand /e /N". This produces an increase of g which tends to1 in the limit N→B !Fermi-gas limit" !Egger, 1999". Onealso notes that, in the case of a tunneling contact toMWNTs, the observed zero-bias anomaly and power-lawbehaviors of transport quantities have been assigned toa different physical mechanism known as the environ-mental Coulomb blockade, which can, like the LLmodel, describe the same kind of universalities in theconductance scaling anomalies !Rollbühler and Grabert,2001; Tarkiainen et al., 2001; Dayen et al., 2005". Further,several groups !Egger and Gogolin, 2001; Mishchenko etal., 2001; Mishchenko and Andreev, 2002" have per-formed a nonperturbative calculation of the e-e interac-tion in disordered MWNTs, showing a crossover fromthe Luttinger-liquid result !valid at sufficiently high en-ergy" to a new low-energy behavior of the density ofstates.

We end by discussing the case of graphite, which wehave often used to illuminate the properties of CNTsthrough band-folding arguments. Several theoretical!González et al., 1996; Spataru et al., 2001" and experi-mental !Xu et al., 1996; Moos et al., 2001" studies haverevealed an anomalous !E−EF" linear behavior of theinverse 1/-ee lifetime, deviating from the standardFermi-liquid theory. However, such effects stem fromthe specific band structure of graphite and cannot beused for laying the grounds for a LL transition in nano-tubes.

4. Transport spectroscopy in the Coulomb blockade regime

In the situation of high contact resistance betweenmetallic or semiconducting CNTs and voltage probes,

the low-temperature transport properties turn out to bedominated by the Coulomb-blockade effect. This phe-nomenon, first observed in semiconductor quantum dotsand small metallic grains !Grabert and Devoret, 1992",occurs at low enough temperature, when the total ca-pacitance C of a metallic island becomes so small thatadding even a single electron requires an electrostaticenergy Ec=e2 /2C larger than the thermal energy kBT.This situation generally develops when the conductingisland is weakly coupled to source and drain leadsthrough tunnel barriers with a resistance larger than thequantum resistance h /e2.

As a matter of illustration, if one considers a nano-tube at a distance z away from a conducting substrate!metallic gate", the total capacitance is C=2#3rG0Ltube/ ln!2z /rtube", 3r being the average dielectricconstant of the environment. Using Gr%2 !for compari-son, 3r=3.9 for SiO2", z=300 nm, and rtube=0.7 nm, thecharging energy becomes Ec%!5 meV" / 'Ltube !"m"(.Thus for a typical /1 "m long tube, Coulomb blockadeshould set in below %50 K !kBT=5 meV". For smallelectrode spacing, the total capacitance is often domi-nated by the capacitance of the leads.

Level splitting due to the finite size of the nanotubeis another relevant energy scale. A simple particle-in-a-box estimate yields 2E=hvF /4Ltube%!1 meV" /'Ltube !"m"(; the factor of 2 accounts for the channeldegeneracy at the charge-neutrality point. Both Ec and2E scale inversely with length !up to a logarithmic fac-tor", but the ratio Ec /2E is thus roughly independent oflength, i.e., the level spacing is always a small but appre-ciable fraction of the charging energy.

In Fig. 55 !main frame", the experimental conductancedI /dV at small bias and as a function of gate voltage isshown for various temperatures for a single-walled car-bon nanotube. When kBT7Ec, single-electron tunnelingprevails as revealed by the fine structure of the conduc-tance spectrum. Each conductance peak represents the

FIG. 54. !Color online" Fourier-transformed map of dI /dV!density of states" as a function of electron momentum k andsample bias V. Ovals near the Fermi levels indicate the cornersof the Brillouin zone nearest !elongated black dots" or secondnearest !elongated white dots" to the ( point. Curves give theenergy dispersions of the !19,7" tube by tight binding, whereassuperimposed color lines indicate the Luttinger-liquid result.Adapted from Eggert, 2000.

FIG. 55. !Color online" Conductance spectrum for severaltemperatures as a function of external gate voltage applied tothe single-walled nanotube contacted with noble metal. Inset:G!Vg" for a device at 4.2 K showing a regular series of Cou-lomb conductance peaks. Adapted from Nygard et al., 1999.

721Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

addition of an extra charge to the nanotube, whereas thepeak spacing is given by !2Ec+2E"C /eCg, with Cg and Cthe capacitance of the gate and the total capacitance,respectively. The regularity !periodicity" of the peaks isrelated to the size of the coherent conducting island!nanotube". In the case of an irregular conductance spec-trum, the nanotube is believed to be split into a series ofconducting parts separated by local tunneling contacts.

The overall diagram of conductance as a function ofbias and gate voltage generally appears as a diamond-shaped structure 'Fig. 55, inset !b"(, referred to as theCoulomb diagram. For a fixed gate voltage, the currentincreases stepwise with increasing bias voltage, produc-ing the excited-state spectrum. Each step in the currentis related to a new higher-lying energy level that entersthe bias window 'Fig. 55, inset !a", Vg1(. Within eachdiamond, the electron number of the nanotube is fixedand the current vanishes 'Fig. 55, inset !a", Vg2(. Theboundary of each diamond represents the transition be-tween N and N+1 electrons, and the parallel lines out-side the diamonds correspond to excited states. Such aplot is well understood within the constant-interactionmodel, in which the capacitance is independent of theelectronic states. Some significant deviations from thissimple picture were, however observed !Tans et al.,1998". The ground-state spin configuration in a nanotubewas determined by studying the transport spectrum in amagnetic field. Cobden and co-workers !Cobden et al.,1998" observed that the level spectrum is split by theZeeman energy g"BB, where "B is the Bohr magnetonand the g factor is found to be 2, indicating the absenceof orbital effects as expected for nanotubes; the totalspin of the ground state alternates between 0 and 1/2 assuccessive electrons are added, demonstrating a simpleshell-filling, or even-odd, effect, i.e., successive electronsoccupy the levels in spin-up and spin-down pairs. Thesemiconducting case was treated by Jarillo-Herrero et al.!2004". Some value of the orbital magnetic momentcould also be estimated using the magnetic field effect tolift the orbital degeneracy !Jarillo-Herrero et al., 2005".

Finally, in the Coulomb-blockade regime, transportmeasurements on suspended single-wall carbon nano-tubes have shown spectacular signatures of phonon-assisted tunneling, mediated by longitudinal vibrational!stretching" modes !Sapmaz et al., 2006". In this experi-ment, the current-voltage characteristics show multiplesteps whose heights are in reasonable agreement withthe Franck-Condon predictions of a large e-ph couplingconstant. On the other hand, in this regime, Coskun andco-workers !Coskun et al., 2004" succeeded in measuringAharonov-Bohm *0 periodic oscillations of the bandstructure for a MWNT.

On the theoretical side, a calculation of the totaltransmission coefficient, based on expanding the many-body wave function into all possible single-particle wavefunctions, was shown to provide a good description ofCoulomb blockade in CNTs !Mehrez et al., 2001". Fur-ther, Bellucci and co-workers !Bellucci et al., 2005" stud-ied the crossover from a Luttinger liquid to theCoulomb-blockade regime in CNTs. They extended the

LL description by incorporating the effects of a single-particle spectrum and found that the intermediate re-gime is characterized by a power-law conductance, withpower exponent oscillating with applied gate voltage.This scheme tends to support similar experimental mea-surements obtained in MWNTs !Kanda et al., 2005".

F. Superconducting and charge-density-wave instabilities

The field of superconductivity !SC" in nanotubesstarted experimentally in 1998 with the discovery of astrong proximity-induced SC in isolated or bundledSWNTs connected to superconducting leads !Kasumovet al., 1998; Mopurgo et al., 1998". In these experiments,the NTs were considered to be in the normal !N" statebut with a phase coherence length L* and a thermallength LT larger than the superconducting coherencelength, allowing for the SNS junction to sustain a veryhigh supercurrent below the lead transition temperature.Three years later, however, intrinsic SC in nanotubeswas discovered in bundles of large-diameter SWNTs!Kociak et al., 2001; Kasumov et al., 2003" and in zeolite-inserted SWNTs of small !/4 Å" diameter !Tang et al.,2001". While in the first case a TC=0.55 K was observedon the basis of resistivity measurements, the small-diameter SWNT samples led to TC/15 K, as evidencedfrom the Meissner effect. These early observations wereconfirmed with the observation of a SC transition withTC up to 12 K in MWNTs encapsulated in large pores ofzeolite !Takesue et al., 2006".

Before continuing, it is important to comment on thelow-energy excitation phase diagram of 1D systems ingeneral, complementing our discussion of the Luttingerliquid !Sec. IV.E.3" by switching on the electron-phononinteraction. Upon coupling of both electrons andphonons, the superconducting phase in 1D systems en-ters into competition with another type of quantum or-der, the charge-density-wave !CDW" phase, which mani-fests itself through a modulation of the charge densitywith a wave vector q=2kF, where kF is the Fermi wavevector !not necessarily commensurate with the nano-tube". The well-known case of the Peierls transition inmonatomic chains at half-filling, accompanied by adimerization and a band-gap opening, is a specific ex-ample of such an instability related to the more generalKohn anomaly !Kohn, 1959". While the SC transitioninduces the creation or destruction of electron !Cooper"pairs, the CDW is induced by the spontaneous forma-tion of electron-hole excitations. The CDW instability isvery specific to 1D systems while the SC one occurs ir-respective of the dimension. An important point relatedto the CDW and SC instabilities is that they are in gen-eral incompatible, meaning that the occurrence of oneusually destroys the other. As a result, the discussion ofSC in nanotubes needs to be associated with that of theCDW !or Peierls" transition.

Further, even if the SC prevails over the CDW insta-bility, its manifestation in nanotubes should be very pe-culiar as, in 1D systems, the existence of a phase-

722 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

coherent order over macroscopic distances is stronglysuppressed by both thermal !Mermin and Wagner, 1966"and quantum fluctuations. By 1D systems, we mean sys-tems for which the largest transverse direction is signifi-cantly smaller than the longitudinal superconducting co-herence length A. The physics of quantum fluctuationsstems from the phenomenon of phase slip !Langer andAmbegaokar, 1967; Tinkham, 1996" which manifests it-self by the appearance of an intrinsic resistive characterbelow the bulk TC value in a narrow superconductingwire. In particular, the resistance of the wire, instead ofdropping abruptly to zero below TC, smoothly decayswith nonzero values down to 0 K. The manifestation ofphase slips was also provided in the case of ultrathinsuperconducting wires !Bezryadin et al., 2000".

After giving many good reasons for not observing aSC order in nanotubes, the fact remains that it has beenclearly seen evidenced experimentally, with a ratherlarge TC in the a priori most disfavorable case of isolated!that is, more 1D-like" nanotubes synthesized in pores ofzeolites. This explains the large interest generated in thetheory community with several attempts to refine thedescription of the electron-electron and electron-phonon interactions at low energy !that is, for energiesaround that of relevant phonons". In particular, and asthe electronic states around EF were already wellknown, two important questions mainly arose: !i" whichphonons are responsible for the EPC and !ii" what is theinfluence of putting nanotubes in a bundle geometry,both on the screening of the Coulomb interactions andon the possibility for Cooper pairs to tunnel !Josephsoncoupling" from one tube to another. The relevance ofthis last point is clearly to question the effective dimen-sionality of the tubes in order to circumvent the above-mentioned difficulty of survival of SC order in 1D sys-tems.

As in the case of fullerenes, the weakness of intertubeinteractions leads to the conclusion that on-tubephonons are responsible for the main EPC channels. Assuch, early studies of the electron-phonon interaction fo-cused on isolated tubes and in particular on the possibleoccurrence of a Peierls instability. Such an instability isalways expected to occur in 1D systems, and the rel-evant question is to know the transition temperatureTCDW !as the instability is quenched at sufficiently hightemperature". This was the idea behind the title “Arefullerene tubules metallic?” of one of the first theoreti-cal studies of nanotubes !Mintmire et al., 1992". By com-parison with the case of polyacethylene, Mintmire andco-workers concluded that the mean-field Peierls transi-tion temperature in nanotubes, with respect to couplingto q=2kF phonons, should be extremely small, below1 K.

The Peierls !or CDW" instability in nanotubes wassubsequently studied in several papers !Saito et al., 1992;Harigaya and Fujita, 1993; Huang et al., 1996; Tanaka etal., 1997; Sédéki et al., 2000", where specific deformationmodes !in-plane, out-of-plane, etc." and parametrizedmodel interactions were considered, leading to a varietyof results with, in particular, TCDW ranging from /9.1 K

!Huang et al., 1996" to 15 K !Sédéki et al., 2000" for a!5,5" tube. Such temperatures are clearly larger than, orequivalent to, the experimental TC for the SC instability.

Following our discussion of electron-phonon coupling!Sec. IV.E.1", the coupling to long-wavelength acousticmodes such as twistons or radial breathing modes !de-rived from the transverse acoustic modes of graphite"was also studied as a means to induce a CDW instability!Figge et al., 2001; De Martino and Egger, 2003". Therelated Peierls transition temperature was estimated byFigge et al. to be around 10 K for an !8,8" tube, which isagain larger than or equivalent to the experimental TC.

The softening of phonons by electron-phonon interac-tions and the Peierls transition was carefully studied inthe specific case of small 4-Å tubes using DFT calcula-tions !Bohnen et al., 2004; Connétable et al., 2005". Theincrease of the coupling with radius !Sec. IV.E.1" wasshown to lead to a Peierls distortion at several hundredKelvin mediated by 2kF phonons in the !3,3" armchaircase !Bohnen et al., 2004; Connétable et al., 2005". Fur-ther, in the case of the !5,0" tube, the other possiblecandidate for a SC transition, a long-wavelength“squashing mode” was found by Connétable and co-workers !2005" to induce a band gap opening mechanicalinstability at room temperature !Fig. 56". Such resultsseem incompatible with the observed SC transition at/15 K !Tang et al., 2001". However, the same !5,0" tubewas studied within a self-consistent tight-binding ap-proach !Barnett et al., 2005", yielding results compatiblewith the experimental observation, namely, that theCDW instability can be made weaker than the SC one,provided that Coulomb interactions are treated beyondthe mean field. This last point raises the important ques-tion of the validity of mean-field techniques, such as theDFT, to describe low-energy excitations in nanotubes.

The possible failure of single-particle theories pavesthe way to many-body techniques such as those based onbozonization and the renormalization group !RG". Suchapproaches have been used to study electron-electron

FIG. 56. Schematic representation of a Peierls instability in a!5,0" nanotube !left" compared to the perfectly cylindrical !5,0"nanotube !right". This instability opens spontaneously a bandgap !0.2 eV" in the electronic structure of the perfect !D5dsymmetry" tube. Adapted from Connétable et al., 2005.

723Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

interactions in the Luttinger-liquid phase and can begeneralized to address the CNT quantum phase diagramupon switching of the electron-phonon interactions. Thetrue many-body functional form of the Hamiltonian ispreserved but several approximations are performed,such as the linearization of bands around the Fermilevel. Further, the strengths of the electron-electron andelectron-phonon interactions !the gi constants of Sec.IV.E.3 and the deformation potentials of Sec. IV.E.1" aretaken as adjustable parameters, so that the results areoften presented as a phase diagram in parameter spacewith areas dominated by CDW or SC instabilities, and itis not easy to decide which parameters should be takenfor realistic systems.

Using such RG techniques, Kamide et al. !2003" con-cluded that a SC order may dominate in the !5,0" tubeprovided that the electron-phonon interaction is strongenough. This conclusion contradicts previous studiesbased on RG analysis which concluded, on the contrary,that, in isolated nanotubes, Coulomb repulsion shouldeasily overcome the attractive interaction mediated byphonons !González, 2002; Sédéki et al., 2002; Alvarezand González, 2003; De Martino and Egger, 2004". Thisconclusion led these authors to determine that SC fluc-tuations are expected to occur in bundles containing alarge number of !metallic" tubes, as confirmed by theevolution of TC with the number of estimated tubes invarious SWNT bundles !Kasumov et al., 2003". Both thebetter screening in nanotube bundles, which allows oneto reduce long-range Coulomb repulsion, and the possi-bility for Cooper pairs to tunnel from one tube to an-other, thus reducing the 1D character of the supercon-ducting sample, are strong arguments in favor of theimportant role of tube-tube interactions. Upon inclusionof quantum phase slip effects, the experimentaltemperature-dependent profile of the resistance belowTC for nanotube bundles !Kasumov et al., 2003" couldbe reproduced on the basis of theory !De Martino andEgger, 2004". In the case of zeolite-inserted small-radiustubes, the screening by the zeolite, by contacting elec-trodes, and by other tubes, has also been invoked as animportant factor that may decide the strongest relevantinstability !González and Perfetto, 2005", even though apossible dominant triplet-state superconducting instabil-ity was suggested to arise from the specific three-bandtopology at the Fermi level of isolated C!5,0" tubes!Carpentier and Orignac, 2006".

The physics of superconductivity in nanotubes re-mains a challenging subject. The difficulties in estimat-ing the transition temperatures can be related to ourdiscussion of the EPC deformation potential strength inSec. IV.E.1. In the normal state, the relevant quantities,such as the inelastic mean free path, depend quadrati-cally on the deformation potential through the Fermigolden rule. In the case of the superconducting transi-tion temperature, the dependence is exponential as illus-trated in the McMillan formula

TC =1@log

1.2kBexp4 − 1.04!1 + :"

: − "*!1 + 0.62:"5 , !69"

where @log is some average phonon frequency, : is thee-ph coupling constant !proportional to an average overthe Fermi surface of the EPC matrix elements squared",and "* is the screened and retarded Coulomb repulsionparameter. The validity of such a formula for CNTs iscertainly questionable but Eq. !69" illustrates qualita-tively that the difficulty in obtaining accurate electron-electron and electron-phonon interaction parametersprevents the emergence of a clear and conclusive under-standing of the experimental situation.

G. Field emission from nanotubes

Field emission !FE" from nanotubes !Chernozatonskiiet al., 1995; De Heer et al., 1995; Rinzler et al., 1995", thatis, the use of CNTs as a source of electrons under ap-plied electric field, is one of the most promising fields ofapplication and several prototypes have been demon-strated, including flat panel displays, lighting elements,high-brightness electron microscopy sources, rf amplifi-ers, portable x-ray systems, and ionization vacuumgauges !see Purcell et al., 2006, for detailed references".Several extensive articles have been written in the field!Lovall et al., 2000; Bonard et al., 2001; de Jonge andBonnard, 2004", and we provide below just a summaryof the underlying physical ideas and research issues. Ageneral review of field emission can be found in Gadzukand Plummer !1973".

The basic FE principles are illustrated in Fig. 57!b".Electrons at the Fermi level in solids need to overcomea potential barrier * to be emitted through the surfaceinto the vacuum. * is the work function specific to thematerial and surface crystallographic direction. This bar-rier can be overcome by providing thermal energy to thecarriers. This is the thermoionic effect used in standardcathodic tubes. However, under application of an elec-tric field, the potential barrier V!z" seen by electrons can

FIG. 57. !Color online" Symbolic energy diagram for coldcathodes Left: The shaded area represents the Fermi-Diracdistribution of occupied states. Inclusion of the image chargepotential reduces the triangular barrier V!z" !thin line" to therounded one !thick line". Right: Illustration of the resonanttunneling process involving tip states. The work function * ofCNTs, which is radius dependent, is of the order of 4.5–5.0 eV.

724 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

be reduced dramatically by a quantity −eFz, z being thedistance to the surface and F the magnitude of the elec-tric field. The thinning of the potential barrier allows forelectrons to tunnel out of the solid even at zero tem-perature. This is the principle of field emission used incold cathodes.

The probability of emission P!E" increases with theelectron energy E. However, the temperature-dependent Fermi-Dirac distribution fT,EF

!E" dramati-cally reduces the number of electrons above the Fermilevel available for tunneling. The current density J!E"results from a trade-off between the evolution of P!E"and fT,EF

!E":

J!E" = 2e0k

fT,EF!E"P!E"vz

d3k!2#"3 , !70"

with k the momentum of the electronic states and vz=1kz /m the electron velocity in the direction of emis-sion within the free-electron model. This tunneling cur-rent can be calculated analytically by assuming a semi-infinite jellium of electrons and a tunnel probabilityP!E" given by the semiclassical Wentzel-Kramers-Brillouin !WKB" approximation, namely,

PWKB = exp4− 2*2m12 +1/20

z1

z2

dz$V!z" − Ez5 , !71"

with Ez=12kz2 /2m the kinetic energy in the direction of

emission. The integral limits !z1 ,z2" are the classicalturning points defined by V!zi"=Ez. Assuming a triangu-lar potential barrier V!z"=Evac−eFz and solving !Evac−Ez"3/2 to first order in EF−Ez, one obtains

PWKB = exp4−4*3/2

3eF*2m12 +1/25

$exp4*2m12 +1/22*1/2

eF!Ez − EF"5 . !72"

Equation !72" relies on several severe approximations,including neglect of the image charge potential !interac-tion of the electron with the hole left behind", but it isknown to work qualitatively well for metallic surfaces.Equation !72" can then be used to obtain the Fowler-Nordheim equation for the emission current densitywhich, at zero temperature, reads

JFN =e

4!2#"21*F2 exp4−

4$2m*3/2

31eF5 . !73"

While the use of such a formula in the case of a thinmetallic object such as a CNT is certainly subject to criti-cisms !Fransen et al., 1999; Lovall et al., 2000; Bonard etal., 2004", it clearly illustrates that the emitted currentdensity J depends exponentially on the material workfunction and the value of the electrostatic field F at theCNT cap. The great advantage of nanotubes in this re-spect is the well-known field enhancement effect atsharp metallic tips resulting from self-consistent rear-rangement of charges upon applied external field. Thelocal electric field Fl!tip" is much larger than the applied

field with a proportionality factor . which is a purelygeometrical factor; namely, Fl!tip"=.F=.V /d, with Vthe drop in potential between two planar electrodesseparated by a distance d. This amplification of the fieldwas already exploited in the so-called Spindt cathodesmade of sharp conical metallic emitters. The values of .can be shown to be proportional to h /r for a verticallyaligned model metallic cylinder of length h terminatedby an hemisphere of radius r !h?r" !Bonard et al., 1998;Edgcombe and Valdré, 2001". This scaling is the crucialdifficulty for theoretical approaches as it requires one tostudy prohibitively long tubes, a difficulty that is oftenbypassed by studying short tubes with a very large exter-nal applied field !Adessi and Devel, 2002; Han et al.,2002; Buldum and Lu, 2003; Zheng et al., 2004; Khazaeiet al., 2005".

A high . value related to this qualitative h /r behaviorapplies to isolated tubes. Upon gathering of tubes inmats or bundles, the . factor collapses dramatically asthe electric field at the tip of a given CNT is stronglyscreened by neighboring tubes. It has been estimatedthat tubes must be separated by a distance l>2h in or-der to recover the isolated tube . value !Nilsson et al.,2000". To maximize the emitted current per surface area,a trade-off must be found between the emitter surfacedensity and the amplification factor.

An interesting issue concerning the physics of CNTemission is the role of tip states. The analysis of theemission patterns, that is, the shape of the bright spotsobserved on electrosensitive screens facing an emittingisolated CNT, was interpreted in several works as pro-viding a direct signature of the atomic structure and re-lated local electronic structure of tube tips !Carroll et al.,1997; Saito, Hata, and Murata, 2000". This interpretationhinges on the physics of resonant tunneling as illustratedin Fig. 57. The tunneling probability is related to thedecay of the electronic wave functions into the vacuumacross the potential barrier. As such, it is expected to berelated to the electronic states at the tube tip. However,electrons which will tunnel can only be carried from theanode to the emitting tip by extended Bloch states cor-responding to the tube body. Such propagating wavepackets will first tunnel into the tip states before beingemitted. One may thus expect that the energy and spa-tial decomposition of the current carry information onthe CNT caps.

The interest in FE from CNTs does not reside only inits technological applications. Field emission is also apowerful characterization tool. The analysis of the cur-rent density 'Eq. !70"( shows that valuable informationon the work function, CNT bulk and apex density ofstates, tip temperature, etc., can be extracted from theI /V characteristics and the energy-resolved decomposi-tion of the emitted current. It can also be used to ob-serve directly the mechanical vibration resonances ofCNTs from which elastic moduli can be inferred !Purcellet al., 2002b". Further, the analysis of the temperature atthe tube apex and knowledge of the emitted current pro-vide quantitative information on the tube electrical re-

725Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

sistivity, even though it is not a trivial task to separatethe contribution from heat radiation and Joule heating!Purcell et al., 2002a; Vincent et al., 2002". Finally, FEfrom growing CNTs has been used to provide some es-timate of the tube growth rates in a CVD reactor!Bonard and Croci, 2002".

V. CONCLUSION

The field of nanotubes is still rapidly growing. As em-phasized, many questions are still unanswered. The dy-namics of hot electrons !and electron-hole pairs" in op-tical experiments, the nature of the contact resistance atmetallic electrode interfaces, the effect of an out-of-equilibrium phonon distribution on inelastic scattering,and the domain of existence of the Luttinger-liquid,charge-density-wave, and superconducting phases arestill subjects which require a considerable amount ofwork and understanding. Further, and beyond the intrin-sic properties of nanotubes, the physics of functional-ized, chemisorbed, doped, or excited CNTs is driven bypotential applications in molecular electronics, optoelec-tronics, and sensors. Such themes are still largely unex-plored areas for theorists: while early theoretical paperspreceded experiments on the discussion of the basicelectronic properties of pristine tubes, such complex sys-tems and applications have now been demonstrated ex-perimentally and theory is lagging behind.

The field of nanotubes has fostered much interest inrelated systems such as graphene or semiconductingnanowires. The actual synthesis of isolated graphenesheets or few-layer graphite materials !Novoselov et al.,2004" and the sudden interest generated by such a syn-thesis come nearly 15 years after the development ofnanotubes. This is an amazing twist of history as theproperties of nanotubes are usually derived, as in Sec.III, from those of graphene. Charge carriers around thecharge-neutrality point in graphene show a very highmobility with a Dirac-like behavior, namely, an energy-independent velocity !Novoselov et al., 2005, 2006;Zhang et al., 2005; Berger et al., 2006; Ohta et al., 2006,Zhou et al., 2006". In the case of graphene nanoribbons,confinement effects induce a width- and orientation-dependent band-gap opening !Son et al., 2006a" and oneis back to the size and helicity selection that complicatesthe use of nanotubes in applications. Other interestingproperties, such as a half-metalic behavior, wherespin-up and spin-down electrons display a different me-tallicity, have been proposed !Son et al., 2006b".

Semiconducting nanowires !Si, GaN, etc." also offeran interesting alternative to nanotubes as they do notexhibit the problem of the variation of the band gapwith chirality. Through confinement, an effect well de-scribed within simple effective mass or more sophisti-cated quasiparticle approaches !Niquet et al., 2006", theband gap depends only on the wire radius. Further,while the band gap of nanotubes lies in the infrared,with difficulties in obtaining a strong PL signal, III-V orII-VI nanowires and their related heterostructures arewell adapted to optoelectronic applications in the visible

range !Duan et al., 2001; Bjork et al., 2002". Topics suchas integration in FETs !Duan et al., 2001; Huang et al.,2001; Martensson et al., 2004; Wang et al., 2006" andfunctionalization for chemical sensing !Cui et al., 2001"are also being developed and discussed in the field ofnanowires. It is interesting to note that, while the chan-nel of existing standard Si-based transistors is now rou-tinely reaching the few tens of nanometer range, semi-conducting nanowires are regarded as new objects withstrong technological potential. The difficulty in obtain-ing structurally perfect wires with controlled radius, sur-face roughness, and dopant density is certainly as large achallenge as controlling the radius and helicity of tubesduring synthesis.

ACKNOWLEDGMENTS

The authors acknowledge in particular T. Ando, M. A.Cazalilla Gutierrez, R. Egger, M.-V. Fernández-Serra, S.Latil, S. Purcell, R. Saito, and F. Triozon for a criticalreading of all, or selected sections, of the manuscript.J.C.C. and X.B. are supported by the Belgian FNRS andthe French CNRS, respectively. S.R. was supported bythe French Ministry of Research under Grant RTB:PostCMOS moléculaire 200 mm and the CEA ChimTro-nique program.

REFERENCES

Adessi, Ch., and M. Devel, 2002, Phys. Rev. B 65, 075418.Adessi, Ch., S. Roche, and X. Blase, 2006, Phys. Rev. B 73,

125414.Aharonov, Y., and D. Bohm, 1959, Phys. Rev. 115, 485.Ajayan, P. M., T. W. Ebbesen, T. Ichihashi, S. Iijima, K. Tani-

gaki, and H. Hiura, 1993, Nature !London" 362, 522.Ajiki, H., and T. Ando, 1993, J. Phys. Soc. Jpn. 62, 1255.Ajiki, H., and T. Ando, 1994, Physica B 201, 349.Ajiki, H., and T. Ando, 1996, J. Phys. Soc. Jpn. 65, 505.Altshuler, B. L., and A. G. Aronov, 1985, in Electron-Electron

Interactions in Disordered Systems, edited by A. L. Efros andM. Pollak !North-Holland, Amsterdam".

Altshuler, B. L., A. G. Aronov, and B. Spivak, 1981, JETPLett. 33, 94.

Alvarez, J. V., and J. González, 2003, Phys. Rev. Lett. 91,076401.

Anantram, M. P., 2000, Phys. Rev. B 62, R4837.Anantram, M. P., 2001, Appl. Phys. Lett. 78, 2055.Anantram, M. P., and T. R. Govindan, 1998, Phys. Rev. B 58,

4882.Ando, T., 1997, J. Phys. Soc. Jpn. 66, 1066.Ando, T., 2004, J. Phys. Soc. Jpn. 73, 3351.Ando, T., 2005, J. Phys. Soc. Jpn. 74, 777.Ando, T., and T. Nakanishi, 1998, J. Phys. Soc. Jpn. 67, 1704.Ando, T., T. Nakanishi, and R. Saito, 1998, J. Phys. Soc. Jpn.

67, 2857.Ando, T., and S. Seri, 1997, J. Phys. Soc. Jpn. 66, 3558.Appenzeller, J., J. Knoch, M. Radosavljevic, and Ph. Avouris,

2004, Phys. Rev. Lett. 92, 226802.Arenal, R., O. Stéphan, M. Kociak, D. Taverna, A. Loiseau,

and C. Colliex, 2005, Phys. Rev. Lett. 95, 127601.Arnaud, B., S. Lebégue, P. Rabiller, and M. Alouani, 2006,

726 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Phys. Rev. Lett. 96, 026402.Auvray, S., V. Derycke, M. Goffman, A. Filoramo, O. Jost, and

J.-P. Bourgoin, 2005, Nano Lett. 5, 451.Avriller, R., S. Latil, F. Triozon, X. Blase, and S. Roche, 2006,

Phys. Rev. B 74, 121406.Bachilo, S. M., M. S. Strano, C. Kittrell, R. H. Hauge, R. E.

Smalley, and R. B. Weisman, 2002, Science 298, 2361.Bachtold, A., C. Strunk, J.-P. Salvetat, J.-M. Bonard, L. Forró,

T. Nussbaumer, and C. Schönenberger, 1999, Nature !Lon-don" 397, 673.

Baeriswyl, D., and L. Degiorgi, 1990, Strong Interactions inLow Dimensions !Kluwer Academic, Dordrecht".

Bahr, J. L., J. P. Yang, D. V. Kosynkin, M. J. Bronikowski, R.E. Smalley, and J. M. Tour, 2001, J. Am. Chem. Soc. 123,6536.

Bai, X. D., E. G. Wang, and J. Yu, Hui Yang, 2000, Appl. Phys.Lett. 77, 67.

Balents, L., and M. P. A. Fisher, 1997, Phys. Rev. B 55, R11973.Banhart, F., 1999, Rep. Prog. Phys. 62, 1181.Barnett, R., E. Demler, and E. Kaxiras, 2005, Phys. Rev. B 71,

035429.Baughman, R. H., Anvar A. Zakhidov, and Walt A. de Heer,

2000, Science 297, 787.Bellucci, S., J. Gonzalez, and P. Onorato, 2005, Phys. Rev. Lett.

95, 186403.Beenakker, C. W., 1997, Rev. Mod. Phys. 69, 731.Bendiab, N., L. Spina, A. Zahab, P. Poncharal, C. Marliere, J.

L. Bantignies, E. Anglaret, and J. L. Sauvajol, 2001, Phys.Rev. B 63, 153407.

Benedict, L. X., V. H. Crespi, S. G. Louie, and M. L. Cohen,1995, Phys. Rev. B 52, 14935.

Benedict, L. X., S. G. Louie, and M. L. Cohen, 1995, Phys.Rev. B 52, 8541.

Berger, C., Z. Song, X. Li, X. Wu, N. Brown, C. Naud, D.Mayou, T. Li, J. Hass, A. N. Marchenkov, E. H. Conrad, P. N.First, and W. A. de Heer, 2006 Science 312, 1191.

Bethune, D. S., C. H. Kiang, M. S. de Vries, G. Gorman, R.Savoy, J. Vazquez, and R. Beyers, 1993, Nature !London"363, 605.

Bezryadin, A., C. N. Landau, and M. Tinkham, 2000, Nature!London" 404, 971.

Biel, B., F. J. García-Vidal, A. Rubio, and F. Flores, 2005, Phys.Rev. Lett. 95, 266801.

Bjork, M. T., B. J. Ohlsson, T. Sass, A. I. Persson, C. The-lander, M. H. Magnusson, K. Deppert, L. R. Wallenberg, andL. Samuelson, 2002, Appl. Phys. Lett. 80, 1058.

Blase, X., Ch. Adessi, and D. Connétable, 2004, Phys. Rev.Lett. 93, 237004.

Blase, X., L. X. Benedict, E. L. Shirley, and S. G. Louie, 1994,Phys. Rev. Lett. 72, 1878.

Blase, X., J.-C. Charlier, A. De Vita, and R. Car, 1997, Appl.Phys. Lett. 70, 197.

Blase, X., A. De Vita, J.-C. Charlier, and R. Car, 1999, Appl.Phys. A: Mater. Sci. Process. 68, 293.

Blase, X., A. Rubio, M. L. Cohen, and S. G. Louie, 1994, Eu-rophys. Lett. 28, 335.

Bockrath, M., D. H. Cobden, J. Lu, A. G. Rinzler, R. E. Smal-ley, L. Balents, and P. L. McEuen, 1999, Nature !London"397, 598.

Bohnen, K.-P., R. Heid, H. J. Liu, and C. T. Chan, 2004, Phys.Rev. Lett. 93, 245501.

Bonard, J.-M., and M. Croci, 2002 Appl. Phys. Lett. 81, 2836.Bonard, J.-M., K. Dean, B. Coll, and C. Klinke, 2004, Phys.

Rev. Lett. 89, 197602.Bonard, J.-M., H. Kind, T. Stöckli, and L. A. Nilsson, 2001,

Solid-State Electron. 45, 893.Bonard, J.-M., T. Stöckli, F. Maier, W. A. de Heer, and A.

Chatelain, 1998, Phys. Rev. Lett. 81, 1441.Bourlon, B., C. Miko, L. Forro, D. C. Glattli, and A. Bachtold,

2004, Phys. Rev. Lett. 93, 176806.Buldum A., and J. P. Lu, 2003, Phys. Rev. Lett. 91, 236801.Büttiker, M., Y. Imry, R. Landauer, and S. Pinhas, 1985, Phys.

Rev. B 31, 6207.Cabria, I., J. W. Mintmire, and C. T. White, 2003, Phys. Rev. B

67, 121406.Cao, J., Q. Wang, M. Rolandi, and H. Dai, 2004, Phys. Rev.

Lett. 93, 216803.Carpentier, D., and E. Orignac, 2006, Phys. Rev. B 74, 085409

!2006".Carroll, D. L., Ph. Redlich, P. M. Ajayan, J.-C. Charlier, X.

Blase, A. De Vita, and R. Car, 1997, Phys. Rev. Lett. 78, 2811.Chakravarty, S., and A. Schmidt, 1986, Phys. Rep. 140, 193.Chang, E., G. Bussi, A. Ruini, and E. Molinari, 2004, Phys.

Rev. Lett. 92, 196401.Charlier, J.-C., 2002, Acc. Chem. Res. 35, 1063.Charlier, J.-C., T. W. Ebbesen, and Ph. Lambin, 1996, Phys.

Rev. B 53, 11108.Charlier, J.-C., X. Gonze, and J.-P. Michenaud, 1991, Phys.

Rev. B 43, 4579.Charlier, J.-C., X. Gonze, and J.-P. Michenaud, 1994, Euro-

phys. Lett. 28, 403.Charlier, J.-C., X. Gonze, and J.-P. Michenaud, 1995, Euro-

phys. Lett. 29, 43.Charlier, J.-C., and Ph. Lambin, 1998, Phys. Rev. B 57, R15037.Charlier, J.-C., and J.-P. Michenaud, 1993, Phys. Rev. Lett. 70,

1858.Charlier, J.-C., and G.-M. Rignanese, 2001, Phys. Rev. Lett. 86,

5970.Chen, J., V. Perebeinos, M. Freitag, J. Tsang, Q. Fu, J. Liu, and

P. Avouris, 2005, Science 310, 1171.Chen, J., and L. Yang, 2005, J. Phys.: Condens. Matter 17, 957.Chen, Y., J. C. Barnard, R. E. Palmer, and M. O. Watanabe,

1999, Phys. Rev. Lett. 83, 2406.Chen, Z. H., J. Appenzeller, J. Knoch, Y. M. Lin, and P.

Avouris, 2005, Nano Lett. 5, 1497.Chernozatonskii, L. A., Y. V. Gulyaev, Z. J. Kosakovskaja, N.

I. Sinitsyn, G. V. Torgashov, Y. F. Zakharchenko, E. A. Fe-dorov, and V. P. Val’chuk, 1995, Chem. Phys. Lett. 233, 63.

Chico, L., L. X. Benedict, S. G. Louie, and M. L. Cohen, 1996,Phys. Rev. B 54, 2600.

Chico, L., V. H. Crespi, L. X. Benedict, S. G. Louie, and M. L.Cohen, 1996, Phys. Rev. Lett. 76, 971.

Chico, L., M. P. López Sancho, and M. C. Muñoz, 1998, Phys.Rev. Lett. 81, 1278.

Chiu, P. W., G. S. Duesberg, U. Dettlaff-Weglikowska, and S.Roth, 2002, Appl. Phys. Lett. 80, 3811.

Chiu, P.-W., M. Kaempgen, and S. Roth, 2004, Phys. Rev. Lett.92, 246802.

Choi, H. J., J. Ihm, S. G. Louie, and M. L. Cohen, 2000, Phys.Rev. Lett. 84, 2917.

Cobden, D. H., et al., 1998, Phys. Rev. Lett. 81, 681.Collins, P. G., K. Bradley, M. Ishigami, and A. Zettl, 2000,

Science 287, 1801.Connétable, D., G.-M. Rignanese, J.-C. Charlier, and X. Blase,

2005, Phys. Rev. Lett. 94, 015503.Connétable, D., V. Timoshevskii, B. Masenelli, J. Beille, J.

727Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Marcus, B. Barbara, A. M. Saitta, G.-M. Rignanese, P. Méli-non, S. Yamanaka, and X. Blase, 2003, Phys. Rev. Lett. 91,247001.

Coskun, U. C., T.-C. Wei, S. Vishveshwara, P. M. Goldbart, andA. Bezryadin, 2004, Science 304, 1132.

Crespi, V. H., M. L. Cohen, and A. Rubio, 1997, Phys. Rev.Lett. 79, 2093–2096.

Cui, Y., Q. Wei, H. Park, and C. M. Lieber, 2001, Science 293,1289.

Dag, S., O. Gulseren, S. Ciraci, and T. Yildirim, 2003, Appl.Phys. Lett. 83, 3180.

Damnjanovic, M., I. Miloševic, T. Vukovic, and R. Sredanovic,1999, Phys. Rev. B 60, 2728.

Datta, S., 1995, Electronic Transport in Mesoscopic Systems!Cambridge University Press, Cambridge, England".

Dayen, J.-F., T. L. Wade, M. Konczykowski, J.-E. Wegrowe,and X. Hoffer, 2005, Phys. Rev. B 72, 073402.

De Heer, W. A., A. Chatelain, and D. Ugarte, 1995, Science270, 1179.

de Jonge, N., and J.-M. Bonnard, 2004, Philos. Trans. R. Soc.London, Ser. A 362, 2239.

Delaney, P., H. J. Choi, J. Ihm, S. G. Louie, and M. L. Cohen,1998, Nature !London" 391, 466.

De Martino, A., and R. Egger, 2003, Phys. Rev. B 67, 235418.De Martino, A., and R. Egger, 2004, Phys. Rev. B 70, 014508.Derycke, V., R. Martel, J. Appenzeller, and Ph. Avouris, 2002,

Appl. Phys. Lett. 15, 2773.De Vita, A., J.-C. Charlier, X. Blase, and R. Car, 1999, Appl.

Phys. A: Mater. Sci. Process. 68, 283.DiVicenzo, D. P., and E. J. Mele, 1984, Phys. Rev. B 29, 1685.Dresselhaus, M. S., G. Dresselhaus, and Ph. Avouris, 2001,

Carbon Nanotubes, Topics in Applied Physics Vol. 80!Springer-Verlag, Berlin".

Dresselhaus, M. S., G. Dresselhaus, and P. C. Eklund, 1996,Science of Fullerenes and Carbon Nanotubes !Academic, SanDiego, CA".

Dresselhaus, M. S., G. Dresselhaus, R. Saito, and A. Jorio,2005, Phys. Rep. 409, 47.

Dresselhaus, M. S., and P. C. Eklund, 2000, Adv. Phys. 49,705–814.

Duan, X. F., Y. Huang, Y. Cui, J. F. Wang, and C. M. Lieber,2001, Nature !London" 409, 66.

Dubay, O., and G. Kresse, 2003, Phys. Rev. B 67, 035401.Dubay, O., G. Kresse, and H. Kuzmany, 2002, Phys. Rev. Lett.

88, 235506.Dunlap, B. I., 1994, Phys. Rev. B 49, 5643.Ebbesen, T. W., 1997, Carbon Nanotubes: Preparation and

Properties !CRC, Boca Raton, FL".Edgcombe, C., and U. Valdré, 2001, J. Microsc. 203, 188.Egger, R., 1999, Phys. Rev. Lett. 83, 5547.Egger, R., and A. O. Gogolin, 1997, Phys. Rev. Lett. 79, 5082.Egger, R., and A. O. Gogolin, 1998, Eur. Phys. J. B 3, 281.Egger, R., and A. O. Gogolin, 2001, Phys. Rev. Lett. 87,

066401.Eggert, S., 2000, Phys. Rev. Lett. 84, 4413.El-Barbary, A. A., R. H. Telling, C. P. Ewels, M. I. Heggie, and

P. R. Briddon, 2003, Phys. Rev. B 68, 144107.Elliott, R. J., 1957, Phys. Rev. 108, 1384.Endo, M., S. Iijima, and M. S. Dresselhaus, 1996, Carbon

Nanotubes !Pergamon, Amsterdam".Ewels, C. P., and M. Glerup, 2005, J. Nanosci. Nanotechnol. 5,

1345.Ewels, C. P., M. I. Heggie, and P. R. Briddon, 2002, Chem.

Phys. Lett. 351, 178.Fan, X., E. C. Dickey, P. C. Eklund, K. A. Williams, L. Grigo-

rian, R. Buczko, S. T. Pantelides, and S. J. Pennycook, 2000,Phys. Rev. Lett. 84, 4621.

Fan, Y., B. R. Goldsmith, and P. G. Collins, 2005, Nat. Mater.4, 906.

Fedorov, G., B. Lassagne, M. Sagnes, B. Raquet, J. M. Broto,F. Triozon, S. Roche, and E. Flahaut, 2005, Phys. Rev. Lett.94, 066801.

Fernández-Serra, M.-V., 2006, unpublished.Fernández-Serra, M.-V., Ch. Adessi, and X. Blase, 2006a, Phys.

Rev. Lett. 96, 166805.Fernández-Serra, M.-V., Ch. Adessi, and X. Blase, 2006b,

Nano Lett. 6, 2674.Figge, M. T., M. Mostovoy, and J. Knoester, 2001, Phys. Rev.

Lett. 86, 4572.Foa-Torres, L., and S. Roche, 2006, Phys. Rev. Lett. 97, 076804.Frank, S., P. Poncharal, Z. L. Wang, and W. A. de Heer, 1998,

Science 280, 1744.Fransen, M., T. van Rooy, and P. Kruit, 1999, Appl. Surf. Sci.

146, 312.Fujiwara, A., K. Tomiyama, H. Suematsu, M. Yumura, and K.

Uchida, 1999, Phys. Rev. B 60, 13492.Gadzuk, J. W., and E. W. Plummer, 1973, Rev. Mod. Phys. 45,

487.Gao, B., A. Komnik, R. Egger, D. C. Glattli, and A. Bachtold,

2004, Phys. Rev. Lett. 92, 216804.Gavillet, J., 2001, Ph.D. thesis !ONERA–Universitè Paris VI"Georghe, M., R. Gutierrez, A. Pecchia, A. di Carlo, and G.

Cuniberti, 2005, Europhys. Lett. 71, 438.Giamarchi, T., 2004, Quantum Physics in One Dimension !Ox-

ford Science, Oxford".Giannozzi, P., R. Car, and G. Scoles, 2003, J. Chem. Phys. 118,

1003.Gómez-Navarro, G., P. J. De Pablo, J. Gómez-Herrero, B.

Biel, F.-J. Garcia-Vidal, A. Rubio, and F. Flores, 2005, Nat.Mater. 4, 534.

González, J., 2002, Phys. Rev. Lett. 88, 076403.González, J., F. Guinea, and M. A. H. Vozmediano, 1996, Phys.

Rev. Lett. 77, 3589 !1996".González, J., and B. Perfetto, 2005, Phys. Rev. B 72, 205406.Grabert, H., and M. H. Devoret, 1992, Single Electron Tunnel-

ling: Coulomb Blockade Phenomena in Nanostructure !Ple-num, New York".

Grigorian, L., K. A. Williams, S. Fang, G. U. Sumanasekera,A. L. Loper, E. C. Dickey, S. J. Pennycook, and P. C. Eklund,1998, Phys. Rev. Lett. 80, 5560.

Guo, T., C.-M. Jin, and R. E. Smalley, 1995, Chem. Phys. Lett.243, 49.

Haeckel, E., 1998, Art Forms in Nature !Prestel-Verlag, Ber-lin".

Hagen, A., G. Moos, V. Talalaev, and T. Hertel, 2004, Appl.Phys. A: Mater. Sci. Process. 78, 1137 !2004".

Hagen, A., M. Steiner, M. B. Raschke, C. Lienau, T. Hertel, H.Qian, A. J. Meixner, and A. Hartschuh, 2005, Phys. Rev. Lett.95, 197401 !2005".

Haldane, F. D. M., 1981, J. Phys. C 14, 2585.Hamada, N., S. Sawada, and A. Oshiyama, 1992, Phys. Rev.

Lett. 68, 1579.Han, S., M. H. Lee, and J. Ihm, 2002, Phys. Rev. B 65, 085405.Harigaya, K., and M. Fujita, 1993, Phys. Rev. B 47, 16563.Harris, P. J. F., 1999, Carbon Nanotubes and Related Structures

!Cambridge University Press, Cambridge, England".

728 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Hashimoto, A., K. Suenaga, A. Gloter, K. Urita, and S. Iijima,2004, Nature !London" 430, 870.

Heinze, S., M. Radosavljevic, J. Tersoff, and Ph. Avouris, 2003,Phys. Rev. B 68, 235418.

Heinze, S., J. Tersoff, R. Martel, V. Derycke, J. Appenzeller,and Ph. Avouris, 2002, Phys. Rev. Lett. 89, 106801.

Hertel, T., and G. Moos, 2000, Phys. Rev. Lett. 84, 5002.Hirahara, K., M. Kociak, S. Bandow, T. Nakahira, K. Ito, Y.

Saito, and S. Iijima, 2006, Phys. Rev. B 73, 195420.Hirahara, K., K. Suenaga, S. Bandow, H. Kato, T. Okazaki, H.

Shinohara, and S. Iijima, 2000, Phys. Rev. Lett. 85, 5384.Hjort, M., and S. Stafström, 2001, Phys. Rev. B 63, 113406.Hornbaker, D. J., S.-J. Kahng, S. Misra, B. W. Smith, A. T.

Johnson, E. J. Mele, D. E. Luzzi, and A. Yazdani, 2002, Sci-ence 295, 828.

Huang, Y., X. F. Duan, Y. Cui, L. J. Lauhon, K. H. Kim, and C.M. Lieber, 2001, Science 294, 1313.

Huang, Y., M. Okada, K. Tanaka, and T. Yamabe, 1996, Phys.Rev. B 53, 5129.

Imry, Y., 1997, Introduction to Mesoscopic Physics !OxfordUniversity Press, Oxford".

Iijima, S., 1991, Nature !London" 354, 56.Iijima, S., and T. Ichihashi, 1993, Nature !London" 363, 603.Ishii, H., et al., 2003 Nature !London" 426, 540.Jarillo-Herrero, P., J. Kong, H. S. J. van der Zant, C. Dekker,

L. P. Kouwenhoven, and S. De Franceschi, 2005, Phys. Rev.Lett. 94, 156802.

Jarillo-Herrero, P., S. Sapmaz, C. Dekker, L. P. Kouwenhoven,and H. S. J. van der Zant, 2004, Nature !London" 429, 389.

Javey, A., J. Guo, M. Paulsson, Q. Wang, D. Mann, M. Lund-strom, and H. Dai, 2004, Phys. Rev. Lett. 92, 106804.

Jensen, P., J. Gale, and X. Blase, 2002, Phys. Rev. B 66, 193403.Jhi, S.-H., S. G. Louie, and M. L. Cohen, 2005, Phys. Rev. Lett.

95, 226403.Jiang, J., J. Dong, and D. Y. Xing, 2000, Phys. Rev. B 62, 13209.Jiang, J., J. Dong, H. T. Yang, and D. Y. Xing, 2001, Phys. Rev.

B 64, 045409.Jiang, J., R. Saito, Ge. G. Samsonidze, S. G. Chou, A. Jorio, G.

Dresselhaus, and M. S. Dresselhaus, 2005, Phys. Rev. B 72,235408.

Jishi, R. A., M. S. Dresselhaus, and G. Dresselhaus, 1993,Phys. Rev. B 48, 11385.

Jorio A., C. Fantini, M. A. Pimenta, D. A. Heller, M. S.Strano, M. S. Dresselhaus, Y. Oyama, J. Jiang, and R. Saito,2006, Appl. Phys. Lett. 88, 023109.

Jorio, A., A. G. S Filho, G. Dresselhaus, M. S. Dressellhaus, R.Saito, J. H. Hafner, C. M. Lieber, F. M. Matinaga, M. S. S.Dantas, and M. A. Pimenta, 2001, Phys. Rev. B 63, 245416.

Jouguelet, E., C. Mathis, and P. Petit, 2000, Chem. Phys. Lett.318, 561.

Kamaras, K., M. E. Itkis, H. Hu, B. Zhao, and R. C. Haddon,2003, Science 301, 1501.

Kamide, K., T. Kimura, M. Nishida, and S. Kurihara, 2003,Phys. Rev. B 68, 024506.

Kanda, A., K. Tsukagoshi, Y. Aoyagi, and Y. Ootuka, 2005,Phys. Rev. Lett. 92, 036801.

Kanda, A., S. Uryu, K. Tsukagoshi, Y. Ootuka, and Y. Aoyagi,2002, Physica B 323, 246.

Kane, C. L., L. Balents, and M. P. A. Fisher, 1997, Phys. Rev.Lett. 79, 5086.

Kane, C. L., and E. J. Mele, 1997, Phys. Rev. Lett. 78, 1932.Kane, C. L., and E. J. Mele, 2003, Phys. Rev. Lett. 90, 207401.Kane, C. L., E. J. Mele, R. S. Lee, J. E. Fischer, P. Petit, H.

Dai, A. Thess, R. E. Smalley, A. R. M. Verschueren, S. J.Tans, and C. Dekker, 1998, Europhys. Lett. 41, 683.

Kasumov, A. Y., R. Deblock, M. Kociak, B. Reulet, H. Bou-chiat, I. I. Khodos, Y. B. Gorbatov, V. T. Volkov, C. Journet,and M. Burghard, 1998, Science 284, 1508.

Kasumov, A., M. Kociak, M. Ferrier, R. Deblock, S. Guéron,B. Reulet, I. Khodos, O. Stéphan, and H. Bouchiat, 2003,Phys. Rev. B 68, 214521.

Kataura, H., Y. Kumazawa, Y. Maniwa, I. Umezu, S. Suzuki, Y.Ohtsuka, and Y. Achiba, 1999, Synth. Met. 103, 2555.

Kaun, C. C., B. Larade, H. Mehrez, J. Taylor, and H. Guo,2002, Phys. Rev. B 65, 205416.

Kazaoui, S., N. Minami, R. Jacquemin, H. Kataura, and Y.Achiba, 1999, Phys. Rev. B 60, 13339.

Ke, S.-H., W. Yang, and H. U. Baranger, 2006, J. Chem. Phys.124, 181102.

Khan, F., and P. Allen, 1984, Phys. Rev. B 29, 3341.Khazaei, M., A. A. Farajian, and Y. Kawazoe, 2005, Phys. Rev.

Lett. 95, 177602.Kociak, M., A. Y. Kasumov, S. Guéron, B. Reulet, I. I. Kho-

dos, Yu. B. Gorbatov, V. T. Volkov, L. Vaccarini, and H. Bou-chiat, 2001, Phys. Rev. Lett. 86, 2416.

Kociak, M., K. Suenaga, K. Hirahara, Y. Saito, T. Nakahira,and S. Iijima, 2002, Phys. Rev. Lett. 89, 155501.

Kohn, W., 1959, Phys. Rev. Lett. 2, 393.Kong, J., and H. Dai, 2001, J. Phys. Chem. B 105, 2890.Kong, J., N. R. Franklin, C. Zhou, M. G. Chapline, S. Peng, K.

Cho, and H. Dai, 2000, Science 28, 622.Krstic, V., S. Blumentritt, J. Muster, S. Roth, and A. Rubio,

2003, Phys. Rev. B 67, 041401!R".Kubo, R., 1966, Rep. Prog. Phys. 29, 255.Kwon, Y-K., and D. Tománek, 1998, Phys. Rev. B 58, R16001.Lambin, Ph., A. Fonseca, J.-P. Vigneron, J. B. Nagy, and A. A.

Lucas, 1995, Chem. Phys. Lett. 245, 85.Lambin, Ph., V. Meunier, and A. Rubio, 2000, Phys. Rev. B 62,

5129.Lambin, Ph., L. Philippe, J.-C. Charlier, and J.-P. Michenaud,

1994, Comput. Mater. Sci. 2, 350.Lammert, P. E., V. H. Crespi, and A. Rubio, 2001, Phys. Rev.

Lett. 87, 136402.Lammert, P. E., P. Zhang, and V. H. Crespi, 2000, Phys. Rev.

Lett. 84, 2453.Langer, J. S., and V. Ambegaokar, 1967, Phys. Rev. 164, 498.Latil, S., S. Roche, and J.-C. Charlier, 2005, Nano Lett. 5, 2216.Latil, S., S. Roche, D. Mayou, and J.-C. Charlier, 2004, Phys.

Rev. Lett. 92, 256805.Latil, S., F. Triozon, and S. Roche, 2005, Phys. Rev. Lett. 95,

126802.Lauret, J. S., R. Arenal, F. Ducastelle, A. Loiseau, M. Cau, B.

Attal-Tretout, E. Rosencher, and L. Goux-Capes, 2005, Phys.Rev. Lett. 94, 037405.

Lazzeri, M., S. Piscanec, F. Mauri, A. C. Ferrari, and J. Rob-ertson, 2005, Phys. Rev. Lett. 95, 236802.

Lazzeri, M., S. Piscanec, F. Mauri, A. C. Ferrari, and J. Rob-ertson, 2006, Phys. Rev. B 73, 155426.

Lee, J., S. Eggert, H. Kim, S. J. Kahng, H. Shinohara, and Y.Kuk, 2004, Phys. Rev. Lett. 93, 166403.

Lee, J., H. Kim, S.-J. Kahng, G. Kim, Y.-W. Son, J. Ihm, H.Kato, Z. W. Wang, T. Okazaki, H. Shinohara, and Y. Kuk,2002, Nature !London" 415, 1005.

Lee, J.-O., J.-R. Kim, J.-J. Kim, J. Kim, N. Kim, J. W. Park, andK.-H. Yoo, 2000, Solid State Commun. 115, 467.

Lee, H.-W, and D. S. Novikov, 2003, Phys. Rev. B 68, 155402.

729Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Lee, Y.-S., M. Buongiorno Nardelli, and N. Marzari, 2005,Phys. Rev. Lett. 95, 076804.

Lefebvre, J., Y. Homma, and P. Finnie, 2003, Phys. Rev. Lett.90, 217401.

Lehtinen, P. O., A. S. Foster, A. Ayuela, A. Krasheninnikov,K. Nordlund, and R. M. Nieminen, 2003, Phys. Rev. Lett. 91,017202.

Lemay, S. G., J. W. Janssen, M. van den Hout, M. Mooij, M. J.Bronikowski, P. A. Willis, R. E. Smalley, L. P. Kouwenhoven,and C. Dekker, 2001, Nature !London" 412, 617.

Léonard, F., and J. Tersoff, 1999, Phys. Rev. Lett. 83, 5174.Liu, H. J., and C. T. Chan, 2002, Phys. Rev. B 66, 115416.Liu, K., P. Avouris, R. Martel, and W. K. Hsu, 2001, Phys. Rev.

B 63, 161404!R".Lin, M. F., and K. W.-K. Shung, 1995, Phys. Rev. B 51, 7592.Loiseau, A., P. Launois, P. Petit, S. Roche, and J.-P. Salvetat,

2006, Understanding Carbon Nanotubes From Basics to Ap-plications, Lecture Notes in Physics Vol. 677 !Springer-Verlag,Berlin".

López Sancho, M. P., J. M. López Sancho, and J. Rubio, 1984,J. Phys. F: Met. Phys. 14, 1205.

López Sancho, M. P., M. C. Muñoz, and L. Chico, 2001, Phys.Rev. B 63, 165419.

Loudon, R., 1959, Am. J. Phys. 27, 649.Lovall, D., M. Buss, E. Graugnard, R. P. Andres, and R. Reif-

enberger, 2000, Phys. Rev. B 61, 5683.Lu, J.-P., 1995, Phys. Rev. Lett. 74, 1123.Luttinger, J. M., 1951, Phys. Rev. 84, 814.Luttinger, J. M., 1963, J. Math. Phys. 4, 1154.Machón, M., S. Reich, C. Thomsen, D. Sánchez-Portal, and P.

Ordejón, 2002, Phys. Rev. B 66, 155410.Machón, M., et al., 2005, Phys. Rev. B 66, 155410.Mahan, G. D., 2003, Phys. Rev. B 68, 125409.Mahan, G. D., 2004, Phys. Rev. B 69, 125407.Marinopoulos, A. G., L. Reining, A. Rubio, and N. Vast, 2003,

Phys. Rev. Lett. 91, 046402.Martel, R., T. Schmidt, H. R. Shea, T. Hertel, and Ph. Avouris,

1998, Appl. Phys. Lett. 73, 2447.Martensson, T., P. Calberg, M. Borgstrom, L. Montelius, W.

Seifert, and L. Samuelson, 2004, Nano Lett. 4, 699.Marty, L., E. Adam, L. Albert, R. Doyon, D. Ménard, and R.

Martel, 2006, Phys. Rev. Lett. 96, 136803.Mattis, D. C., and E. H. Lieb, 1965, J. Math. Phys. 6, 304.Maultzsch, J., R. Pomraenke, S. Reich, E. Chang, D. Prezzi, A.

Ruini, E. Molinari, M. S. Strano, C. Thomsen, and C. Lienau,2005, Phys. Rev. B 72, 241402!r".

Mayer, A., 2005, Carbon 43, 717.Mazzoni, M. S. C., R. W. Nunes, S. Azvedo, and H. Chacham,

2006, Phys. Rev. B 73, 073108.McEuen, P. L., M. Bockrath, D. H. Cobden, Y.-G. Yoon, and S.

G. Louie, 1999, Phys. Rev. Lett. 83, 5098.Mehrez, H., H. Guo, J. Wang, and C. Roland, 2001, Phys. Rev.

B 63, 245410.Mermin, N. D., and H. Wagner, 1966, Phys. Rev. Lett. 17, 1133.Meunier, V., M. Buongiorno Nardelli, J. Bernholc, T. Zacharia,

and J.-C. Charlier, 2002, Appl. Phys. Lett. 81, 5234.Meyer, A., et al., 2005, Carbon 43, 717.Mintmire, J. W., B. I. Dunlap, and C. T. White, 1992, Phys.

Rev. Lett. 68, 631.Mintmire, J. W., and C. T. White, 1998, Phys. Rev. Lett. 81,

2506.Minot, E. D., Y. Yaish, V. Sazonova, and P. L. McEuen, 2004,

Nature !London" 428, 536.

Mingo, N., and J. Han, 2001, Phys. Rev. B 64, 201401.Mishchenko, E. G., and A. V., Andreev, 2002, Phys. Rev. B 65,

235310.Mishchenko, E. G., Andreev, and L. I. Glazman, 2001, Phys.

Rev. Lett. 87, 246801.Misewich, J. A., R. Martel, Ph. Avouris, J. C. Tsang, S. Heinze,

and J. Tersoff, 2003, Science 300, 783.Miyamoto, Y., A. Rubio, X. Blase, M. L. Cohen, and S. G.

Louie, 1995, Phys. Rev. Lett. 74, 2993.Miyamoto, Y., S. Saito, and D. Tománek, 2001, Phys. Rev. B

65, 041402!R".Moos, M., et al., 2001, Phys. Rev. Lett. 87, 267402.Mopurgo, A. F., J. Kong, C. M. Marcus, and H. Dai, 1998,

Science 286, 263.Mora, C., R. Egger, and A. Altland, 2006, Phys. Rev. B 75,

035310.Nardelli, M. B., J.-L. Fattebert, and J. Bernholc, 2001, Phys.

Rev. B 64, 245423.Nemec, N., and G. Cuniberti, 2006, Phys. Rev. B 74, 165411.Nemec, N., D. Tománek, and G. Cuniberti, 2006, Phys. Rev.

Lett. 96, 076802.Nilsson, L., O. Groening, C. Emmenegger, O. Kuettel, E.

Schaller, L. Schlapbach, H. Kind, J.-M. Bonard, and K. Kem,2000, Appl. Phys. Lett. 76, 2071.

Niquet, Y.-M., A. Lherbier, N. H. Quang, X. Blase, and Ch.Delerue, 2006, Phys. Rev. B 73, 165319.

Novoselov, K. S., A. K. Geim, S. V. Morozov, D. Jiang, S. V.Dubonos, I. V. Girgorieva, and A. A. Firsov, 2004, Science306, 666.

Novoselov, K. S., A. K. Geim, S. V. Morozov, D. Jiang, M. I.Katsnelson, I. V. Girgorieva, S. V. Dubonos, and A. A. Firsov,2005, Nature !London" 438, 197.

Novoselov, K. S., E. McCann, S. V. Morozov, V. I. Fal’ko M. I.Katsnelson, U. Zeitler, D. Jiang, F. Schedin, and A. K. Geim,2006, Nat. Phys. 2, 177.

Nozières, P., and D. Pines, 1999, Theory of Quantum Liquids!Perseus, New York".

Nygard, J., et al., 1999, Appl. Phys. A 69, 297.O’Connell, M. J., S. M. Bachilo, C. B. Huffman, V. C. Moore,

M. S. Strano, E. H. Haroz, K. L. Rialon, P. J. Boul, W. H.Noon, C. Kittrell, J. Ma, R. H. Hauge, R. B. Weisman, and R.E. Smalley, 2002, Science 297, 593.

Odbadrakh, K., P. Pomorski, and Ch. Roland, 2006, Phys. Rev.B 73, 233402.

Odom, T. W., J. L. Huang, P. Kim, and C. M. Lieber, 1998,Nature !London" 391, 62.

Odom, T. W., J.-L. Huang, and C. M. Lieber, 2002, J. Phys.:Condens. Matter 14, R145.

Ogawa, T., and T. Takagahara, 1991a, Phys. Rev. B 43, 14325.Ogawa, T., and T. Takagahara, 1991b, Phys. Rev. B 44, 8138.Ohta, T., A. Bodtwick, T. Seyller, K. Horn, and E. Rotenberg,

2006, Science 313, 951.Okada, S., and A. Oshiyama, 2005, Phys. Rev. Lett. 95, 206804.Orlikowski, D., M. Buongiorno Nardelli, J. Bernholc, and C.

Roland, 2000, Phys. Rev. B 61, 14194.Ouyang, M., J.-L. Huang, C. L. Cheung, and C. M. Lieber,

2001a, Science 291, 97.Ouyang, M., J. L. Huang, C. L. Cheung, and C. M. Lieber,

2001b, Science 292, 702.Palacios, J. J., A. J. Perez-Jimenez, E. Louis, E. SanFabian,

and J. A. Verges, 2003, Phys. Rev. Lett. 90, 106801.Papadopoulos, C., A. Rakitin, J. Li, A. S. Vedeneev, and J. M.

Xu, 2000, Phys. Rev. Lett. 85, 3476.

730 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Park, C.-H., C. D. Spataru, and S. G. Louie, 2006, Phys. Rev.Lett. 96, 126105.

Park, J.-Y., S. Rosenblatt, Y. Yaish, V. Sazonova, H. Ustunel, S.Braig, T. A. Arias, P. W. Brouwer, and P. L. McEuen, 2004,Nano Lett. 4, 517.

Park, N., and S. Hong, 2005, Phys. Rev. B 72, 045408.Peierls, R E., 1933, Z. Phys. 80, 763.Peng, S., and K. Cho, 2003, Nano Lett. 3, 513.Perebeinos, V., and Ph. Avouris, 2006, Phys. Rev. B 74, 121410.Perebeinos, V., J. Tersoff, and Ph. Avouris, 2004, Phys. Rev.

Lett. 92, 257402.Perebeinos, V., J. Tersoff, and Ph. Avouris, 2005, Phys. Rev.

Lett. 94, 086802.Petit, P., C. Mathis, C. Journet, and P. Bernier, 1999, Chem.

Phys. Lett. 305, 370.Piscanec, S., M. Lazzeri, F. Mauri, A. C. Ferrari, and J. Rob-

ertson, 2004, Phys. Rev. Lett. 93, 185503.Poncharal, P., C. Berger, Z. L. Wang, and W. A. de Heer, 2002,

J. Phys. Chem. 106, 12104.Popov, V. N., and L. Henrard, 2004, Phys. Rev. B 70, 115407.Popov, V. N., and Ph. Lambin, 2006a, Phys. Rev. B 73, 085407.Popov, V. N., and Ph. Lambin, 2006b, Phys. Rev. B 74, 075415.Purcell, S., P. Vincent, C. Journet, and V. T. Binh, 2002a, Phys.

Rev. Lett. 88, 105502.Purcell, S., P. Vincent, C. Journet, and V. T. Binh, 2002b, Phys.

Rev. Lett. 89, 276103.Purcell, S., P. Vincent, M. Rodriguez, C. Journet, S. Vignoli, D.

Guillot, and A. Ayari, 2006, Chem. Vap. Deposition 12, 331.Radosavljevic, M., J. Appenzeller, Ph. Avouris, and J. Knoch,

2004, Appl. Phys. Lett. 84, 3693.Rao, A. M., P. C. Ecklund, S. Bandow, A. Thess, and R. E.

Smalley, 1997, Nature !London" 388, 257.Reich, S., J. Maultzsch, C. Thomsen, and P. Ordejón, 2002,

Phys. Rev. B 66, 035412.Reich, S., C. Thomsen, and J. Maultzsch, 2004, Carbon Nano-

tubes, Basic Concepts and Physical Properties !Wiley-VCHVerlag GmbH, Weinheim".

Reich, S., C. Thomsen, and P. Ordejón, 2002, Phys. Rev. B 65,155411.

Reich, S., C. Thomsen, and J. Robertson, 2005, Phys. Rev.Lett. 95, 077402.

Rinzler, A. G., J. H. Hafner, P. Nikolaev, L. Lou, S. G. Kim, D.Tománek, P. Nordlander, D. T. Colbert, and R. E. Smalley,1995, Science 269, 1550.

Roche, S., 1999, Phys. Rev. B 59, 2284.Roche, S., G. Dresselhaus, M. S. Dresselhaus, and R. Saito,

2000, Phys. Rev. B 62, 16092.Roche, S., J. Jiang, F. Triozon, and R. Saito, 2005a, Phys. Rev.

Lett. 95, 076803.Roche, S., J. Jiang, F. Triozon, and R. Saito, 2005b, Phys. Rev.

B 72, 113410.Roche, S., and D. Mayou, 1997, Phys. Rev. Lett. 79, 2518.Roche, S., and R. Saito, 2001, Phys. Rev. Lett. 87, 246803.Roche, S., F. Triozon, A. Rubio, and D. Mayou, 2001a, Phys.

Rev. B 64, 121401.Roche, S., F. Triozon, A. Rubio, and D. Mayou, 2001b, Phys.

Lett. A 285, 94.Rochefort, A., Ph. Avouris, F. Lesage, and D. R. Salahub,

1999, Phys. Rev. B 60, 13824.Rocquefelte, X., G.-M. Rignanese, V. Meunier, H. Terrones,

M. Terrones, and J.-C. Charlier, 2004, Nano Lett. 4, 805.Rollbühler J., and H. Grabert, 2001, Phys. Rev. Lett. 87,

126804.

Rubio, A., J. Corkill, and M. L. Cohen, 1994, Phys. Rev. B 49,5081.

Rubio, A., Y. Miyamoto, X. Blase, M. L. Cohen, and S. G.Louie, 1996, Phys. Rev. B 53, 4023.

Rubio, A., D. Sánchez-Portal, E. Artacho, P. Ordejón, and J.M. Soler, 1999, Phys. Rev. Lett. 82, 3520.

Saito, R., G. Dresselhaus, and M. S. Dresselhaus, 1993, J.Appl. Phys. 73, 494.

Saito, R., G. Dresselhaus, and M. S. Dresselhaus, 1994, Phys.Rev. B 50, 14698.

Saito, R., G. Dresselhaus, and M. S. Dresselhaus, 1996, Phys.Rev. B 53, 2044.

Saito, R., G. Dresselhaus, and M. S. Dresselhaus, 1998, Physi-cal Properties of Carbon Nanotubes !Imperial College Press,London".

Saito, R., G. Dresselhaus, and M. S. Dresselhaus, 2000, Phys.Rev. B 61, 2981.

Saito, R., M. Fujita, G. Dresselhaus, and M. S. Dresselhaus,1992, Appl. Phys. Lett. 60, 2204.

Saito, Y., K. Hata, and T. Murata, 2000, Jpn. J. Appl. Phys.,Part 2 39, L271.

Sánchez-Portal, D., et al., 1999, Phys. Rev. B 59, 12678.Sanvito, S., Y. K. Kwon, D. Tománek, and C. J. Lambert, 2000,

Phys. Rev. Lett. 84, 1974.Sapmaz, S., P. Jarillo-Herrero, Ya. M. Blanter, C. Dekker, and

H. S. J. van der Zant, 2006 Phys. Rev. Lett. 96, 026801.Sédéki, A., L. G. Caron, and C. Bourbonnais, 2000, Phys. Rev.

B 62, 6975.Sédéki, A., L. G. Caron, and C. Bourbonnais, 2002, Phys. Rev.

B 65, 140515.Seri, T., and T. Ando, 1997, J. Phys. Soc. Jpn. 66, 169.Shan, B., and K. Cho, 2004, Phys. Rev. B 70, 233405.Shea, H. R., R. Martel, and P. Avouris, 2000, Phys. Rev. Lett.

84, 4441.Shim, M., A. Javey, N. W. S. Kam, and H. Dai, 2001, J. Am.

Chem. Soc. 123, 11512.Shyu, F. L., C. P. Chang, R. B. Chen, C. W. Chiu, and M. F. Lin,

2003, Phys. Rev. B 67, 045405.Slonczewski, J. C., and P. R. Weiss, 1958, Phys. Rev. 109, 272.Smith, B. W., M. Monthioux, and D. E. Luzzi, 1998, Nature

!London" 396, 323.Solyom, J., 1979, Adv. Phys. 28, 201.Son, Y.-W., M. L. Cohen, and S. G. Louie, 2006a, Phys. Rev.

Lett. 97, 216803.Son, Y.-W., M. L. Cohen, and S. G. Louie, 2006b, Nature !Lon-

don" 444, 347.Son, Y.-W., J. Ihm, M. L. Cohen, S. G. Louie, and H. J. Choi,

2005, Phys. Rev. Lett. 95, 216602.Spataru, C. D., M. A. Cazalilla, A. Rubio, L. X. Benedict, P. M.

Echenique, and S. G. Louie, 2001, Phys. Rev. Lett. 87,246405.

Spataru, C. D., S. Ismail-Beigi, L. X. Benedict, and S. G.Louie, 2004, Phys. Rev. Lett. 92, 077402.

Spataru, C. D., S. Ismail-Beigi, R. B. Capaz, and S. G. Louie,2005, Phys. Rev. Lett. 95, 247402.

Stojetz, B., C. Miko, L. Forro, and Ch. Strunk, 2005, Phys. Rev.Lett. 94, 186802.

Stojetz, B., S. Roche, C. Miko, F. Triozon, L. Forro, and Ch.Strunk, 2006, unpublished.

Stone, A. J., and D. J. Wales, 1986, Chem. Phys. Lett. 128, 501.Strano, M. S., C. A. Dyke, M. L. Usrey, P. W. Barone, M. J.

Allen, H. Shan, C. Kittrell, R. H. Hauge, J. M. Tour, and R.E. Smalley, 2003, Science 301, 1519.

731Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

Suenaga, K., C. Colliex, N. Demoncy, A. Loiseau, H. Pascard,and F. Willaime, 1997, Science 278, 653.

Sumanasekera, G. U., C. K. W. Adu, S. Fang, and P. C. Eklund,2000, Phys. Rev. Lett. 85, 1096.

Suzuura, H., and T. Ando, 2002, Phys. Rev. B 65, 235412.Szafer, A., and A. D. Stone, 1988, IBM J. Res. Dev. 32, 84.Takesue, I., J. Haruyama, N. Kobayashi, S. Chiashi, S.

Maruyama, T. Sugai, and H. Shinohara, 2006, Phys. Rev. Lett.96, 057001.

Takenobu, T., T. Takano, M. Shiraishi, Y. Murakami, M. Ata,H. Kataura, Y. Achiba, and Y. Iwasa, 2003, Nat. Mater. 2, 683.

Tamura, T., and M. Tsukada, 1995, Phys. Rev. B 52, 6015.Tanaka, K., et al., 1997, Int. J. Quantum Chem. 63, 637.Tang, Z. K., Lingyun Zhang, N. Wang, X. X. Zhang, G. H.

Wen, G. D. Li, J. N. Wang, C. T. Chan, and P. Sheng, 2001,Science 292, 2462.

Tans, S. J., A. R. M. Verschueren, and C. Dekker, 1998, Nature!London" 393, 49.

Tarkiainen, R., M. Ahlskog, J. Penttilä, L. Roschier, P. Ha-konen, M. Paalanen, and E. Sonin, 2001, Phys. Rev. B 64,195412.

Telling, R. H., C. P. Ewels, A. A. El-Barbary, and M. I. Heggie,2003, Nat. Mater. 2, 333.

Terrones, M., F. Banhart, N. Grobert, J.-C. Charlier, H. Ter-rones, and P. M. Ajayan, 2002, Phys. Rev. Lett. 89, 075505.

Terrones, M., H. Terrones, F. Banhart, J.-C. Charlier, and P. M.Ajayan, 2000, Science 288, 1226.

Terrones, H., M. Terrones, E. Hernandez, N. Grobert, J.-C.Charlier, and P. M. Ajayan, 2000, Phys. Rev. Lett. 84, 1716.

Tersoff, J., 1984, Phys. Rev. Lett. 52, 465.Thouless, D. J., 1973, J. Phys. C 6, 249.Thouless, D. J., 1977, Phys. Rev. Lett. 39, 1167.Tian, W., and S. Datta, 1994, Phys. Rev. B 49, 5097.Tinkham, M., 1996, An Introduction to Superconductivity

!McGraw-Hill, New York", Chap. 8.Tománek, D., and R. J. Enbody, 1999, Science and Application

of Nanotubes !Kluwer Academic, Dordrecht".Tomonaga, S., 1950, Prog. Theor. Phys. 5, 544.Triozon, F., Ph. Lambin, and S. Roche, 2005, Nanotechnology

16, 230.Triozon, F., S. Roche, A. Rubio, and D. Mayou, 2004, Phys.

Rev. B 69, 121410.Urbina, U., I. Echeverria, A. Perez-Garrido, A. Diaz-Sanchez,

and J. Abellan, 2003, Phys. Rev. Lett. 90, 106603.Uryu, S., and T. Ando, 2005, Phys. Rev. B 72, 245403.Venema, L. C., V. Meunier, Ph. Lambin, and C. Dekker, 2000,

Phys. Rev. B 61, 2991.Venema, L. C., J. W. G. Wildöer, J. W. Janssen, S. J. Tans, H. L.

J. Temminck, Tuinstra, L. P. Kouwenhoven, and C. Dekker,1999, Science 283, 52.

Vincent, P., S. T. Purcell, C. Journet, and V. T. Binh, 2002, Phys.Rev. B 66, 075406.

Voit, J., 1995, Rep. Prog. Phys. 58, 977.Vucovic, T., I. Miloševic, and M. Damnjanovic, 2002, Phys.

Rev. B 65, 045418.Wallace, P. R., 1947, Phys. Rev. 71, 622.

Wang, D., B. Sheriff, and J. R. Heath, 2006, Nano Lett. 6, 1096.Wang, F., G. Dukovic, L. E. Brus, and T. F. Heinz, 2004, Phys.

Rev. Lett. 92, 177401.Wang, F., G. Dukovic, L. E. Brus, and T. F. Heinze, 2005a,

Science 308, 838.Wang, F., G. Dukovic, L. E. Brus, and T. F. Heinze, 2005b,

Science 309, 1677.Wang, N., Z. K. Tang, G. D. Li, and J. S. Chen, 2000, Nature

!London" 408, 50.Wang, S., and M. Griffoni, 2005, Phys. Rev. Lett. 95, 266802.Wang, S., M. Griffoni, and S. Roche, 2006, Phys. Rev. B 74,

121407.Watanabe, K., T. Taniguchi, and H. Kanda, 2004, Nat. Mater. 3,

404.Watanabe, M. O., S. Itoh, T. Sasaki, and K. Mizushima, 1996,

Phys. Rev. Lett. 77, 187.Webb, R., S. Washburn, C. Umbach, and R. Laibowitz, 1985,

Phys. Rev. Lett. 54, 2696.White, C. T., and J. W. Mintmire, 1998, Nature !London" 394,

29.White, C. T., and T. N. Todorov, 1998, Nature !London" 393,

240.Wildöer, J. W. G., L. C. Venema, A. G. Rinzler, R. E. Smalley,

and C. Dekker, 1998, Nature !London" 391, 59.Wirtz, L., A. Marini, and A. Rubio, 2006, Phys. Rev. Lett. 96,

126104.Wong, S. S., E. Joselevich, A. T. Woolley, C. L. Cheung, and C.

M. Lieber, 1998, Nature !London" 394, 52.Xu, S., et al., 1996, Phys. Rev. Lett. 76, 483.Xue, Y., and M. Ratner, 2004, Phys. Rev. B 70, 205416.Yang, L., and J. Han, 2000, Phys. Rev. Lett. 85, 154.Yao, Z., C. L. Kane, and C. Dekker, 2000 Phys. Rev. Lett. 84,

2941.Yao, Z., H. W. Postma, L. Balents, and C. Dekker, 1999, Na-

ture !London" 402, 273.Yi, J.-Y., and J. Bernholc, 1993, Phys. Rev. B 47, 1708.Yoon, Y.-G., P. Delanay, H. J. Choi, J. Ihm, and S. G. Louie,

2002, Phys. Rev. B 69, 073407.Yoon, Y.-G., M. S. C. Mazzoni, H. J. Choi, J. Ihm, and S. G.

Louie, 2001, Phys. Rev. Lett. 86, 688.Zaric, S., G. N. Ostojic, J. Kono, J. Shaver, V. C. Moore, M. S.

Strano, R. H. Hauge, R. E. Smalley, and X. Wei, 2004, Sci-ence 304, 1129.

Zaric, S., et al., 2005, Phys. Rev. Lett. 96, 016406.Zhang, Y., Y. W. Tan, H. L. Stormer, and Ph. Kim, 2005, Na-

ture !London" 438, 201.Zheng, X., G. Chen, Z. Li, S. Deng, and N. Xu, 2004, Phys.

Rev. Lett. 92, 106803.Zhou, C., J. Kong, E. Yenilmez, and H. Dai, 2000, Science 290,

1552.Zhou, S. Y., G.-H. Gweon, J. Graf, A. V. Fedorov, C. D. Spa-

taru, R. D. Diehl, Y. Kopelevich, D.-H. Lee, S. G. Louie, andA. Lanzara, 2006, Nat. Phys. 2, 595.

Zhou, X., J.-Y. Park, S. Huang, J. Liu, and P. L. McEuen, 2005,Phys. Rev. Lett. 95, 146805.

Zhu, W. G., and E. Kaxiras, 2006, Nano Lett. 6, 1415.

732 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007